Calcium orthophosphate-based biocomposites and hybrid biomaterials
- 8.1k Downloads
In this review article, the state-of-the-art of calcium orthophosphate-based biocomposites and hybrid biomaterials suitable for biomedical applications is presented. This subject belongs to a rapidly expanding area of science and research, because these types of biomaterials offer many significant and exciting possibilities for hard tissue regeneration. Through the successful combinations of the desired properties of matrix materials with those of fillers (in such systems, calcium orthophosphates might play either role), innovative bone graft biomaterials can be designed. The review starts with an introduction to locate the reader. Further, general information on composites and hybrid materials including a brief description of their major constituents are presented. Various types of calcium orthophosphate-based bone-analogue biocomposites and hybrid biomaterials those are either already in use or being investigated for various biomedical applications are then extensively discussed. Many different formulations in terms of the material constituents, fabrication technologies, structural and bioactive properties, as well as both in vitro and in vivo characteristics have been already proposed. Among the others, the nano-structurally controlled biocomposites, those with nanosized calcium orthophosphates, biomimetically fabricated formulations with collagen, chitin and/or gelatin, as well as various functionally graded structures seem to be the most promising candidates for clinical applications. The specific advantages of using calcium orthophosphate-based biocomposites and hybrid biomaterials in the selected applications are highlighted. As the way from a laboratory to a hospital is a long one and the prospective biomedical candidates have to meet many different necessities, the review also examines the critical issues and scientific challenges that require further research and development.
Ethylene-vinyl alcohol copolymer
Injectable bone substitute
Partially stabilized zirconia
Polyvinyl alcohol phosphate
Starch/ethylene vinyl alcohol copolymer
The fracture of bones due to various traumas or natural aging is a typical type of a tissue failure. An operative treatment frequently requires implantation of a temporary or a permanent prosthesis, which still is a challenge for orthopedic surgeons, especially in the cases of large bone defects. A fast aging of the population and serious drawbacks of natural bone grafts make the situation even worse; therefore, there is a high clinical demand for bone substitutes. Unfortunately, a medical application of xenografts (e.g., bovine bone) is generally associated with potential viral infections. In addition, xenografts have a low osteogenicity, an increased immunogenicity and, usually, resorb more rapidly than autogenous bone. Similar limitations are also valid for human allografts (i.e., tissue transplantation between individuals of the same species but of non-identical genetic composition), where the concerns about potential risks of transmitting tumor cells, a variety of bacterial and viral infections, as well as immunological and blood group incompatibility are even stronger [1, 2, 3]. Moreover, harvesting and conservation of allografts (exogenous bones) are additional limiting factors. Autografts (endogenous bones) are still the “golden standard” among any substitution materials because they are osteogenic, osteoinductive, osteoconductive, completely biocompatible, non-toxic, and do not cause any immunological problems (non-allergic). They contain viable osteogenic cells, bone matrix proteins, and support bone growth. Usually, autografts are well accepted by the body and rapidly integrated into the surrounding bone tissues. Due to these reasons, they are used routinely for a long period with good clinical results [3, 4]; however, it is fair to say on complication cases, those frequently happened in the past [5, 6]. Unfortunately, a limited number of donor sites restrict the quantity of autografts harvested from the iliac crest or other locations of the patient’s own body. Also, their medical application is always associated with additional traumas and scars resulting from the extraction of a donor tissue during a superfluous surgical operation, which requires further healing at the donation site and can involve long-term postoperative pain [1, 6, 7, 8, 9]. Thus, any types of a biologically derived transplant appear to be imperfect solutions, mainly due to a restricted quantity of donor tissues, donor site morbidity, as well as potential risks of an immunological incompatibility and disease transfer [7, 9, 10]. In this light, man-made materials (alloplastic or synthetic bone grafts) stand out as a reasonable option because they are easily available, might be processed and modified to suit the specific needs of a given application [11, 12]. What’s more, there are no concerns about potential infections, immunological incompatibility, sterility, and donor site morbidity. Therefore, investigations on artificial materials for bone tissue repair appear to be one of the key subjects in the field of biomaterials research for clinical applications .
Currently, there are several classes of synthetic bone grafting biomaterials for in vivo applications [14, 15, 16, 17]. The examples include natural coral, coral-derived materials, bovine porous demineralized bone, human demineralized bone matrix, bioactive glasses, glass–ceramics, and calcium orthophosphates . All of these biomaterials are biocompatible and osteoconductive, guiding bone tissue from the edges toward the center of the defect, and aim to provide a scaffold of interconnected pores with pore dimensions ranging from 200 [18, 19] to 2 mm , to facilitate tissue and vessel ingrowths. Among them, porous bioceramics made of calcium orthophosphates appear to be very prominent due to both the excellent biocompatibility and bonding ability to living bone in the body. This is directly related to the fact that the inorganic material of mammalian calcified tissues, i.e., of bone and teeth, consists of calcium orthophosphates [21, 22, 23]. Due to this reason, other artificial materials are normally encapsulated by fibrous tissue, when implanted in body defects, while calcium orthophosphates are not . Several types of calcium orthophosphate-based bioceramics with different chemical composition are already on the market [9, 25]. Unfortunately, as for any ceramic material, calcium orthophosphate bioceramics by itself lack the mechanical and elastic properties of the calcified tissues; namely, scaffolds made of calcium orthophosphates only suffer from a low elasticity, a high brittleness, a poor tensile strength, a low mechanical reliability, and fracture toughness, which leads to the concerns about their mechanical performance after implantation [26, 27, 28]. Besides, in many cases, it is difficult to form calcium orthophosphate bioceramics into the desired shapes.
The biochemical composition of bone 
Calcium orthophosphates (biological apatite)
Collagen type I
Non-collagenous proteins: osteocalcin, osteonectin, osteopontin, thrombospondin, morphogenetic proteins, sialoprotein, serum proteins
Other traces: polysaccharides, lipids, cytokines
Primary bone cells: osteoblasts, osteocytes, osteoclasts
Other traces: Cl−, F−, K+ Sr2+, Pb2+, Zn2+, Cu2+, Fe2+
It remains a great challenge to design the ideal bone graft that emulates nature’s own structures or functions. Certainly, the successful design requires an appreciation of the structure of bone. According to expectations, the ideal bone graft should be benign, available in a variety of forms and sizes; all with sufficient mechanical properties for use in load-bearing sites form a chemical bond at the bone/implant interface, as well as be osteogenic, osteoinductive, osteoconductive, biocompatible, completely biodegradable at the expense of bone growth and moldable to fill and restore bone defects [26, 36, 39]. Further, it should resemble the chemical composition of bones (thus, the presence of calcium orthophosphates is mandatory), exhibit contiguous porosity to encourage invasion by the live host tissue, as well as possess both viscoelastic and semi-brittle behavior, as bones do [40, 41, 42, 43]. Moreover, the degradation kinetics of the ideal implant should be adjusted to the healing rate of the human tissue with absence of any chemical or biological irritation and/or toxicity caused by substances, which are released due to corrosion or degradation. Ideally, the combined mechanical strength of the implant and the ingrowing bone should remain constant throughout the regenerative process. Furthermore, the substitution implant material should not disturb significantly the stress environment of the surrounding living tissue . Finally, there is an opinion, that in the case of a serious trauma, bone should fracture rather than the implant . A good sterilizability, storability, and processability, as well as a relatively low cost are also of a great importance to permit a clinical application. Unfortunately, no artificial biomaterial is yet available, which embodies all these requirements and unlikely it will appear in the nearest future. Until now, most of the available biomaterials appear to be either predominantly osteogenic or osteoinductive or else purely osteoconductive .
Careful consideration of the bone type and mechanical properties are needed to design bone substitutes. Indeed, in high load-bearing bones such as the femur, the stiffness of the implant needs to be adequate, not too stiff to result in strain shielding, but rigid enough to present stability. However, in relatively low load-bearing applications such as cranial bone repairs, it is more important to have stability and the correct three-dimensional shapes for esthetic reasons. One of the most promising alternatives is to apply materials with similar composition and nanostructure to that of bone tissue . Mimicking the structure of calcified tissues and addressing the limitations of the individual materials, development of organic–inorganic hybrid biomaterials provides excellent possibilities for improving the conventional bone implants. In this sense, suitable biocomposites of tailored physical, biological, and mechanical properties with the predictable degradation behavior can be prepared by combining biologically relevant calcium orthophosphates with bioresorbable polymers [45, 46]. As a rule, the general behavior of these bioorganic/calcium orthophosphate composites is dependent on nature, structure, and relative contents of the constitutive components, although other parameters such as the preparation conditions also determine the properties of the final materials. Currently, biocomposites with calcium orthophosphates incorporated as either a filler or a coating (or both) either into or onto a biodegradable polymer matrix, in the form of particles or fibers, are increasingly considered for using as bone tissue engineering scaffolds due to their improved physical, biological, and mechanical properties [47, 48, 49, 50, 51, 52, 53]. In addition, such biocomposites could fulfill general requirements to the next generation of biomaterials, those should combine the bioactive and bioresorbable properties to activate in vivo mechanisms of tissue regeneration, stimulating the body to heal itself and leading to the replacement of the implants by the regenerating tissue [46, 54, 55]. Thus, through the successful combinations of ductile polymer matrixes with hard and bioactive particulate bioceramic fillers, optimal materials can be designed and, ideally, this approach could lead to a superior construction to be used as either implants or posterior dental restorative material .
A lint-reinforced plaster was the first composite used in clinical orthopedics as an external immobilizer (bandage) in the treatment of bone fracture by Mathijsen in 1852 , followed by Dreesman in 1892 . A great progress in the clinical application of various types of composite materials has been achieved since then. Based on the previous experience and newly gained knowledge, various composite materials with tailored mechanical and biological performance can be manufactured and used to meet various clinical requirements . However, this review presents only a brief history and advances in the field of calcium orthophosphate-based biocomposites and hybrid biomaterials suitable for biomedical application. The majority of the reviewed literature is restricted to the recent publications; a limited number of papers published in the 20th century have been cited. Various aspects of the material constituents, fabrication technologies, structural and bioactive properties, and phase interaction have been considered and discussed in details. Finally, several critical issues and scientific challenges that are needed for further advancement are outlined.
General information on composites and biocomposites
According to Wikipedia, the free encyclopedia, “composite materials (or composites for short) are engineered materials made from two or more constituent materials with significantly different physical or chemical properties and which remain separate and distinct on a macroscopic level within the finished structure” . Thus, composites are always heterogeneous. Following the point of view of some predecessors, we also consider that “for the purpose of this review, composites are defined as those having a distinct phase distributed through their bulk, as opposed to modular or coated components” [61, p. 1329]. For this reason, with a few important exceptions, the structures obtained by soaking of various materials in supersaturated solutions containing ions of calcium and orthophosphate (e.g., Refs. [62, 63, 64, 65, 66, 67]), those obtained by coating of various materials by calcium orthophosphates (e.g., Refs. [68, 69, 70, 71, 72, 73]), as well as calcium orthophosphates coated by other compounds  have not been considered; however, composite coatings have been considered. Occasionally, porous calcium orthophosphate scaffolds filled by cells inside the pores [75, 76], as well as calcium orthophosphates impregnated by biologically active substances  are also defined as composites; nevertheless, such structures have not been considered in this review either.
In any composite, there are two major categories of constituent materials: a matrix (or a continuous phase) and (a) dispersed phase(s). In order to create a composite, at least one portion of each type is required. General information on the major fabrication and processing techniques might be found elsewhere . The continuous phase is responsible for filling the volume, as well as it surrounds, and supports the dispersed material(s) by maintaining their relative positions. The dispersed phase(s) is(are) usually responsible for enhancing one or more properties of the matrix. Most of the composites target an enhancement of mechanical properties of the matrix, such as stiffness and strength; however, other properties, such as erosion stability, transport properties (electrical or thermal), radiopacity, density, or biocompatibility, might also be of a great interest. This synergism produces the properties, which are unavailable from the individual constituent materials . What’s more, by controlling the volume fractions and local and global arrangement of the dispersed phase, the properties and design of composites can be varied and tailored to suit the necessary conditions. For example, in the case of ceramics, the dispersed phase serves to impede crack growth. In this case, it acts as reinforcement. A number of methods, including deflecting crack tips, forming bridges across crack faces, absorbing energy during pullout and causing a redistribution of stresses in regions adjacent to crack tips, can be used to accomplish this . Other factors to be considered in composites are the volume fraction of (a) dispersed phase(s), its(their) orientation and homogeneity of the overall composite. For example, higher volume fractions of reinforcement phases tend to improve the mechanical properties of the composites, while continuous and aligned fibers best prevent crack propagation with the added property of anisotropic behavior. Furthermore, the uniform distribution of the dispersed phase is also desirable, as it imparts consistent properties to the composite [60, 78].
In general, composites might be simple, complex, graded, and hierarchical. The term “a simple composite” is referred to the composites those result from the homogeneous dispersion of one dispersed phase throughout a matrix. The term “a complex composite” is referred to the composites those result from the homogeneous dispersion of several dispersed phases throughout one matrix. The term “a graded composite” is referred to the composites those result from the intentionally structurally inhomogeneous dispersion of one or several dispersed phases throughout one matrix. The term “a hierarchical composite” is referred to the cases, when fine entities of either a simple or a complex composite is somehow aggregated to form coarser ones (e.g., granules or particles) which afterwards are dispersed inside another matrix to produce the second hierarchical scale of the composite structure. Another classification type of the available composites is based on either the matrix materials (metals, ceramics and polymers) or the reinforcement dimensions/shapes (particulates, whiskers/short fibers, and continuous fibers) .
In most cases, three interdependent factors must be considered in designing of any composite: (i) selection of the suitable matrix and dispersed materials, (ii) choice of appropriate fabrication and processing methods, (iii) internal and external designs of the device itself . Besides, any composite must be formed to shape. To do this, the matrix material can be added before or after the dispersed material has been placed into a mold cavity or onto the mold surface. The matrix material experiences a melding event, depending upon the nature of the matrix material, that can occur in various ways such as chemical polymerization, setting, curing, or solidification from a melted state. Due to a general inhomogeneity, the physical properties of many composite materials are not isotropic, but rather orthotropic (i.e., there are different properties or strengths in different orthogonal directions) [60, 78].
General respective properties from the bioorganic and inorganic domains, to be combined in various composites and hybrid materials 
High refractive index
Mixed valence slate (red-ox)
The major constituent materials of biocomposites for biomedical applications
The main driving force behind the use of calcium orthophosphates as bone substitute materials is their chemical similarity to the mineral component of mammalian bones and teeth [21, 22, 23]. As a result, in addition to being non-toxic, they are biocompatible, not recognized as foreign materials in the body and, most importantly, both exhibit bioactive behavior and integrate into living tissue by the same processes active in remodeling healthy bone. This leads to an intimate physicochemical bond between the implants and bone, termed osteointegration . More to the point, calcium orthophosphates are also known to support osteoblast adhesion and proliferation [82, 83]. Even so, the major limitations to use calcium orthophosphates as load-bearing biomaterials are their mechanical properties; namely, they are brittle with poor fatigue resistance [26, 27, 28]. The poor mechanical behavior is even more evident for highly porous ceramics and scaffolds because porosity >100 μm is considered as the requirement for proper vascularization and bone cell colonization [84, 85, 86], i.e., why, in biomedical applications calcium orthophosphates are used primarily as fillers and coatings .
Existing calcium orthophosphates and their major properties
Ca/P ionic ratio
Solubility at 25 °C, −log(Ks)
Solubility at 37 °C, −log(Ks)
pH stability range in aqueous solutions at 25 °C
Monocalcium phosphate monohydrate (MCPM)
Ca(H2PO4)2 · H2O
Data not found
Monocalcium phosphate anhydrous (MCPA)
Data not found
Dicalcium phosphate dihydrate (DCPD), mineral brushite
CaHPO4 · 2H2O
Dicalcium phosphate anhydrous (DCPA), mineral monetite
Octacalcium phosphate (OCP)
Ca8(HPO4)2(PO4)4 · 5H2O
α-Tricalcium phosphate (α-TCP)
β-Tricalcium phosphate (β-TCP)
Amorphous calcium phosphate (ACP)
CaxHy(PO4)z · nH2O, n = 3–4.5; 15–20% H2O
Calcium-deficient hydroxyapatite (CDHA)e
Ca10−x(HPO4)x(PO4)6−x(OH) 2− x f (0 < x < 1)
Tetracalcium phosphate (TTCP), mineral hilgenstockite
Polymers are a class of materials consisting of large molecules, often containing many thousands of small units, or monomers, joined together chemically to form one giant chain, thus creating very ductile materials. In this respect, polymers are comparable with major functional components of the biological environment: lipids, proteins, and polysaccharides. They differ from each other in chemical composition, molecular weight, polydispersity, crystallinity, hydrophobicity, solubility, and thermal transitions. Besides, their properties can be fine-tuned over a wide range by varying the type of polymer, chain length, as well as by copolymerization or blending of two or more polymers [94, 95]. Opposite to ceramics, polymers exhibit substantial viscoelastic properties and can easily be fabricated into complex structures, such as sponge-like sheets, gels, or complex structures with intricate porous networks and channels . X-ray transparent and non-magnetic polymeric materials are fully compatible with the modern diagnostic methods such as computed tomography and magnetic resonance imaging. Unfortunately, most of them are unable to meet the strict demands of the in vivo physiological environment. Namely, the main requirements to polymers suitable for biomedical applications are that they must be biocompatible, not eliciting an excessive or chronic inflammatory response upon implantation and, for those that degrade, that they breakdown into non-toxic products only. Unfortunately, polymers, for the most part, lack rigidity, ductility, and ultimate mechanical properties required in load-bearing applications. Moreover, the sterilization processes (autoclave, ethylene oxide, and 60Co irradiation) may affect the polymer properties .
There is a variety of biocompatible polymers suitable for biomedical applications. For example, polyacrylates, poly(acrylonitrile-co-vinylchloride) and polylysine have been investigated for cell encapsulation and immunoisolation [98, 99]. Polyorthoesters and poly(ε-caprolactone) (PCL) have been investigated as drug-delivery devices, the latter for long-term sustained release because of their slow degradation rates . PCL is a hydrolytic polyester having appropriate resorption period and releases non-toxic byproducts upon degradation . Other polyesters and polytetrafluoroethylene (PTFE) are used for vascular tissue replacement. Polyurethanes are in use as coatings for pacemaker lead insulation and have been investigated for reconstruction of the meniscus [102, 103]. Polymers considered for orthopedic purposes include polyanhydrides, which have also been investigated as delivery devices (due to their rapid and well-defined surface erosion), for bone augmentation or replacement since they can be photopolymerized in situ [100, 104, 105]. To overcome their poor mechanical properties, they have been copolymerized with imides or formulated to be crosslinkable in situ . Other polymers, such as polyphosphazenes, can have their properties (e.g., degradation rate) easily modified by varying the nature of their side groups and have been shown to support osteoblast adhesion, which makes them candidate materials for skeletal tissue regeneration . PPF has emerged as a good bone replacement material, exhibiting good mechanical properties (comparable to trabecular bone), possessing the capability to crosslink in vivo through the C=C bond and being hydrolytically degradable. It has also been examined as a material for drug-delivery devices [100, 104, 105, 106, 107]. Polycarbonates have been suggested as suitable materials to make scaffolds for bone replacement and have been modified with tyrosine-derived amino acids to render them biodegradable . Polydioxanone has been also tested for biomedical applications . Polymethylmethacrylate (PMMA) is widely used in orthopedics, as a bone cement for implant fixation, as well as to repair certain fractures and bone defects, for example, osteoporotic vertebral bodies . However, PMMA sets by a polymerization of toxic monomers, which also evolves significant amounts of heat that damages tissues. Moreover, it is neither degradable nor bioactive, it does not bond chemically to bones and might generate particulate debris leading to an inflammatory foreign body response [104, 110]. A number of other non-degradable polymers applied in orthopedic surgery include PE in its different modifications such as low density PE, high-density polyethylene (HDPE), and Ultrahigh molecular weight polyethylene (used as the articular surface of total hip replacement implants [111, 112]), polyethylene terepthalate, polypropylene, and PTFE, which are applied to repair knee ligaments . Polyactive™, a block copolymer of polyethylene glycol (PEG) and polybutyleneterephthalate (PBT), was also considered for biomedical application [114, 115, 116, 117, 118]. Cellulose  and its esters  are also popular. Finally yet importantly, polyethylene oxide, polyhydroxybutyrate (PHB), and blends thereof have also been tested for biomedical applications .
Major properties of several FDA approved biodegradable polymers 
Thermal propertiesa (°C)
Tensile modulus (GPa)
Degradation time (months)
Polyglycolic acid (PGA)
tg = 35–40, tm = 225–230
6–12 (strength loss within 3 weeks)
l-polylactic acid (LPLA)
tg = 60–65, tm = 173–178
d,l-polylactic acid (DLPLA)
tg = 55–60 amorphous
85/15 d,l-polylactic-co-glycolic acid (85/15 DLPLGA)
tg = 50–55 amorphous
75/25 d,l-polylactic-co-glycolic acid (75/25 DLPLGA)
tg = 50–55 amorphous
65/35 d,l-polylactic-co-glycolic acid (65/35 DLPLGA)
tg = 45–50 amorphous
50/50 d,l-polylactic-co-glycolic acid (50/50 DLPLGA)
tg = 45–50 amorphous
tg = (–60)–(–65), tm = 58–63
Several classifications of the biomedically relevant polymers are possible. For example, some authors distinguish between synthetic polymers like PLA and PGA or their copolymers with PCL, and polymers of biological origin like polysaccharides (starch, alginate, chitin/chitosan2 [138, 139, 140], gelatin, cellulose, hyaluronic acid derivatives), proteins (soy, collagen, fibrin , silk), and a variety of biofibers, such as lignocellulosic natural fibers [8, 141, 142]. Other authors differentiate between resorbable or biodegradable (e.g., poly(α-hydroxyesters), polysaccharides and proteins) and non-resorbable (e.g., PE, PMMA, and cellulose) polymers [56, 142]. As synthetic polymers can be produced under the controlled conditions, they in general exhibit predictable and reproducible mechanical and physical properties such as tensile strength, elastic modulus, and degradation rate. Control of impurities is a further advantage of synthetic polymers. The list of synthetic biodegradable polymers used for biomedical application as scaffold materials is available as Table 1 in Ref. , while further details on polymers suitable for biomedical applications are available in the literatures [97, 134, 143, 144, 145, 146, 147, 148, 149, 150, 151] where the interested readers are referred. Good reviews on the synthesis of different biodegradable polymers , as well as on the experimental trends in polymer nanocomposites  are available elsewhere.
Inorganic materials and compounds (metals, ceramics, glass, oxides, carbon, etc.)
Titanium (Ti) is one of the best biocompatible metals and used most widely as implant [13, 154]. Besides, there are other metallic implants made of pure Zr, Hf, V, Nb, Ta, Re , Ni, Fe, Cu [155, 156, 157], Ag, stainless steels, and various alloys  suitable for biomedical application. Recent studies revealed even a greater biomedical potential of porous metals [158, 159, 160]. The metallic implants provide the necessary strength and toughness that are required in load-bearing parts of the body and, due to these advantages, metals will continue to play an important role as orthopedic biomaterials in the future, even though there are concerns with regard to the release of certain ions from and corrosion products of metallic implants. Of course, neither metals nor alloys are biomimetic3 in terms of chemical composition because there are no elemental metals in the human body. In addition, even biocompatible metals are bioinert: while not rejected by the human body, any metallic implants cannot actively interact with the surrounding tissues. Nevertheless, in some cases (especially when they are coated by calcium orthophosphates; however, that is another story) the metallic implants can show a reasonable biocompatibility . Only permanent implants are made of metals and alloys, in which degradation or corrosion is not desirable. However, during recent years a number of magnesium alloys have been proposed, which are aimed to degrade in the body in order to make room for the ingrowing bone [160, 163].
Special types of glasses and glass ceramics are also suitable materials for biomedical applications [164, 165, 166] and a special Na2O–CaO–SiO2–P2O5 glass named Bioglass® [11, 24, 27, 28, 167, 168] is the most popular among them. They are produced via standard glass production techniques and require pure raw materials. Bioglass® is a biocompatible and osteoconductive biomaterial. It bonds to bone without an intervening fibrous connective tissue interface and, due to these properties, it has been widely used for filling bone defects . The primary shortcoming of Bioglass® is mechanical weakness and low fracture toughness due to an amorphous two-dimensional glass network. The bending strength of most Bioglass® compositions is in the range of 40 to 60 MPa, which is not suitable for major load-bearing applications. Making porosity in Bioglass®-based scaffolds is beneficial for even better resorption and bioactivity .
By heat treatment, a suitable glass can be converted into glass–crystal composites containing crystalline phase(s) of controlled sizes and contents. The resultant glass ceramics can have superior mechanical properties to the parent glass as well as to sintered crystalline ceramics. The bioactive apatite–wollastonite (A-W) glass ceramics is made from the parent glass in the pseudoternary system 3CaO · P2O5–CaO · SiO2–MgO · CaO · 2SiO2, which is produced by a conventional melt-quenching method. The bioactivity of A-W glass ceramics is much higher than that of sintered HA. It possesses excellent mechanical properties and has therefore been used clinically for iliac and vertebrae prostheses and as intervertebral spacers [13, 171, 172].
Metal oxide ceramics, such as alumina (Al2O3, high purity, polycrystalline, fine grained), zirconia (ZrO2), and some other oxides (e.g., TiO2), have been widely studied due to their bioinertness, excellent tribological properties, high wear resistance, fracture toughness and strength, as well as a relatively low friction [13, 173]. Unfortunately, due to transformation from the tetragonal to the monoclinic phase, a volume change occurs when pure zirconia is cooled down, which causes cracking of the zirconia ceramics. Therefore, additives such as calcia (CaO), magnesia (MgO), and yttria (Y2O3) must be mixed with zirconia to stabilize the material in either the tetragonal or the cubic phase. Such material is called PSZ [174, 175, 176]. However, the brittle nature of any ceramics has limited their scope of clinical applications and hence more research needs to be conducted to improve their properties.
Calcium orthophosphate-based biocomposites and hybrid biomaterials
biocomposites with polymers,
cement-based biocomposites and concretes,
nano-calcium orthophosphate-based biocomposites and nanocomposites,
biocomposites with collagen,
biocomposites with other bioorganic compounds and biological macromolecules,
injectable bone substitutes (IBS),
biocomposites with glasses, inorganic compounds, and metals,
functionally graded biocomposites,
The details of each subject are given below.
Biocomposites with polymers
Typically, the polymeric components of biocomposites and hybrid biomaterials comprise polymers that both have shown a good biocompatibility and are routinely used in surgical applications. In general, since polymers have a low modulus (2–7 GPa, as the maximum) as compared with that of bone (3–30 GPa), calcium orthophosphate bioceramics need to be loaded at a high-weight-percent ratio. Besides, general knowledge on composite mechanics suggests that any high-aspect-ratio particles, such as whiskers or fibers, significantly improve the modulus at a lower loading . Thus, some attempts have been already performed to prepare biocomposites containing whisker-like [177, 178, 179, 180] or needle-like [181, 182, 183] calcium orthophosphates, as well as calcium orthophosphate fibers [45, 184].
The history of implantable polymer–calcium orthophosphate biocomposites and hybrid biomaterials started in 19814 from the pioneering study by Prof. William Bonfield and colleagues performed on HA/PE composites [186, 187]. That initial study introduced a bone-analogue concept, when proposed biocomposites comprised a polymer ductile matrix of PE and a ceramic stiff phase of HA, and was substantially extended and developed in further investigations by that research group [94, 188, 189, 190, 191, 192, 193, 194, 195, 196, 197, 198, 199, 200, 201, 202, 203, 204, 205]. More recent studies included investigations on the influence of surface topography of HA/PE composites on cell proliferation and attachment [206, 207, 208, 209, 210, 211, 212]. The material is composed of a particular combination of HA particles at a volume loading of ~40% uniformly dispensed in a HDPE matrix. The idea was to mimic bone by using a polymeric matrix that can develop a considerable anisotropic character through adequate orientation techniques reinforced with a bone-like ceramics that assures both a mechanical reinforcement and a bioactive character of the composite. Following FDA approval in 1994, in 1995 this material has become commercially available under the trade name HAPEX™ (Smith and Nephew, Richards, USA), and until now remains the only clinically successful bioactive composite that appeared to be a major step in the implant field [28, 213]. The major production stages of HAPEX™ include blending, compounding, and centrifugal milling. A bulk material or device is then created from this powder by compression and injection molding . Besides, HA/HDPE biocomposites might be prepared by a hot rolling technique that facilitated uniform dispersion and blending of the reinforcements in the matrix .
A mechanical interlock between the two phases of HAPEX™ is formed by shrinkage of HDPE onto the HA particles during cooling [94, 215]. Both HA particle size and their distribution in the HDPE matrix were recognized as important parameters affecting the mechanical behavior of HAPEX™ . Namely, smaller HA particles were found to lead to stiffer composites due to general increasing of interfaces between the polymer and the ceramics; furthermore, rigidity of HAPEX™ was found to be proportional to HA volume fraction . In this formulation, HA could be replaced by other calcium orthophosphates .
Initial clinical applications of HAPEX™ came in orbital reconstruction  but since 1995, the main uses of this composite have been in the shafts of middle ear implants for the treatment of conductive hearing loss [218, 219]. In both applications, HAPEX™ offers the advantage of in situ shaping, so a surgeon can make final alterations to optimize the fit of the prosthesis to the bone of a patient and subsequent activity requires only limited mechanical loading with virtually no risk of failure from insufficient tensile strength [94, 167]. As compared with cortical bones, HA/PE composites have a superior fracture toughness for HA concentrations below 40% and similar fracture toughness in the 45–50% range. Their Young’s modulus is in the range of 1 to 8 GPa, which is quite close to that of bone. The examination of the fracture surfaces revealed that only mechanical bond occurs between HA and PE. Unfortunately, the HA/PE composites are not biodegradable, the available surface area of HA is low and the presence of bioinert PE decreases the ability to bond to bones. Furthermore, HAPEX™ has been designed with a maximized density to increase its strength but the resulting lack of porosity limits the ingrowth of osteoblasts when the implant is placed into the body [26, 168]. Further details on HAPEX™ are available elsewhere . Except of HAPEX™, other types of HA/PE biocomposites are also known [220, 221, 222, 223, 224].
Both linear and branched PE was used as a matrix and the biocomposites with the former were found to give a higher modulus . The reinforcing mechanisms in calcium orthophosphate/polymer biocomposites have yet to be convincingly disclosed. Generally, if a poor filler choice is made, the polymeric matrix might be affected by the filler through reduction of molecular weight during composite processing, formation of an immobilized shell of polymer around the particles (transcrystallization, surface-induced crystallization, or epitaxial growth) and changes in conformation of the polymer due to particle surfaces and inter-particle spacing . On the other hand, the reinforcing effect of calcium orthophosphate particles might depend on the molding technique employed: a higher orientation of the polymeric matrix was found to result in a higher mechanical performance of the composite [225, 226].
Many other blends of calcium orthophosphates with various polymers are possible, including rather unusual formulations with dendrimers . The list of the appropriate calcium orthophosphates is shown in Table 3 (except of MCPM and MCPA—both are too acidic and, therefore, are not biocompatible ), while many biomedically suitable polymers have been listed above. The combination of calcium orthophosphates and polymers into biocomposites has a twofold purpose. The desirable mechanical properties of polymers compensate for a poor mechanical behavior of calcium orthophosphate bioceramics, while in turn the desirable bioactive properties of calcium orthophosphates improve those of polymers, expanding the possible uses of each material within the body [127, 128, 129, 228, 229, 230, 231]. Namely, polymers have been added to calcium orthophosphates in order to improve their mechanical strength [127, 228] and calcium orthophosphate fillers have been blended with polymers to improve their compressive strength and modulus, in addition to increase their osteoconductive properties [48, 129, 137, 232, 233, 234, 235, 236]. Furthermore, biocompatibility of such biocomposites is enhanced because calcium orthophosphate fillers induce an increased initial flash spread of serum proteins compared with the more hydrophobic polymer surfaces . What’s more, experimental results of these biocomposites indicate favorable cell–material interactions with increased cell activities as compared with each polymer alone . As a rule, with increasing of calcium orthophosphate content, both Young’s modulus and bioactivity of the biocomposites increase, while the ductility decreases [26, 232]. Furthermore, such formulations can provide a sustained release of calcium and orthophosphate ions into the milieus, which is important for mineralized tissue regeneration . Indeed, a combination of two different materials draws on the advantages of each one to create a superior biocomposite with respect to the materials on their own.
It is logical to assume that the proper biocomposite of a calcium orthophosphate (for instance, CDHA) with a bioorganic polymer (for instance, collagen) would yield the physical, chemical, and mechanical properties similar to those of human bones. Different ways have been already realized to bring these two components together into composites, like mechanical blending, ball milling, dispersion of ceramic fillers into a polymer–solvent solution, a melt extrusion of a ceramic/polymer powder mixture, coprecipitation, and electrochemical codeposition [32, 59, 238, 239, 240]. Besides, there is an in situ formation, which involves either synthesizing the reinforcement inside a preformed matrix material or synthesizing the matrix material around the reinforcement [59, 241]. For example, several papers have reported this method to produce various composites of apatites with carbon nanotubes [242, 243, 244, 245, 246, 247]. Another example comprises using amino acid-capped gold nanoparticles as scaffolds to grow CDHA . In certain cases, a mechano-chemical route , emulsions [250, 251, 252, 253], freeze-drying  and freeze-thawing techniques , flame-sprayed technique , or gel-templated mineralization  might be applied to produce calcium othophosphates-based biocomposites. Various fabrication procedures are available elsewhere [32, 59, 238], where the interested readers are referred.
The interfacial bonding between a calcium orthophosphate and a polymer is an important issue of any biocomposite. If adhesion between the phases is poor, the mechanical properties of a biocomposite suffer. In order to solve the problem, various approaches have been already introduced. For example, a diisocyanate coupling agent was used to bind PEG/PBT (Polyactive™) block copolymers to HA filler particles. Using surface-modified HA particles as a filler in a PEG/PBT matrix significantly improved the elastic modulus and strength of the polymer as compared with the polymers filled with ungrafted HA [234, 258]. Another group used processing conditions to achieve a better adhesion of the filler to the matrix. Ignjatovic et al. [127, 128, 259] prepared poly(l-lactic acid) (PLLA)/HA composites by pressing blends of varying PLLA and HA content at different temperatures and pressures. They found that maximum compressive strength was achieved at ~15 wt% of PLLA. Using blends with 20 wt% of PLLA, the authors also established that increasing the pressing temperature and pressure improved the mechanical properties. The former was explained by decrease in viscosity of the PLLA associated with a temperature increase, hence leading to improved wettability of HA particles. The latter was explained by increased compaction and penetration of pores at higher pressure, in conjunction with a greater fluidity of the polymer at higher temperatures. The combination of high pressures and temperatures was found to decrease porosity and guarantee a close apposition of a polymer to the particles, thereby improving the compressive strength  and fracture energy  of the biocomposites. The PLLA/HA biocomposites scaffolds were found to improve cell survival over plain PLLA scaffolds .
It is also possible to introduce porosity into calcium orthophosphate-based biocomposites, which is advantageous for most applications as bone substitution material. The porosity facilitates the migration of osteoblasts from surrounding bones to the implant site [129, 262, 263]. Various material processing strategies to prepare composite scaffolds with interconnected porosity comprise thermally induced phase separation, solvent casting, and particle leaching, solid freeform fabrication techniques, microsphere sintering, and coating [142, 264, 265, 266]. A supercritical gas foaming technique might be used as well [238, 267, 268].
A biological apatite is known to be the major inorganic phase of mammalian calcified tissues [21, 22]. Consequently, CDHA, HA, carbonateapatite (both with and without dopants) and, occasionally, FA have been applied to prepare biocomposites with other compounds, usually with the aim to improve the bioactivity. For example, PS composed with HA can be used as a starting material for long-term implants [269, 270, 271]. Retrieved in vivo, HA/PS biocomposite-coated samples from rabbit distal femurs demonstrated direct bone apposition to the coatings, as compared with the fibrous encapsulation that occurred when uncoated samples were used . The resorption time of such biocomposites is a very important factor, which depends on polymer’s microstructure and the presence of modifying phases .
Various apatite-containing biocomposites with PVA [255, 272, 273, 274, 275, 276, 277, 278], polyvinyl alcohol phosphate (PVAP) , and several other polymeric components [279, 281, 282, 283, 284, 285, 286, 287, 288, 289, 290, 291, 292] have already been developed. Namely, PVA/CDHA biocomposite blocks were prepared by precipitation of CDHA in aqueous solutions of PVA . An artificial cornea consisted of a porous nano-HA/PVA hydrogel skirt and a transparent center of PVA hydrogel has been prepared as well. The results displayed a good biocompatibility and interlocking between artificial cornea and host tissues [276, 277]. PVAP has been chosen as a polymer matrix, because its phosphate groups can act as a coupling/anchoring agent, which has a higher affinity toward the HA surface . Greish and Brown [283, 284, 285] developed HA/Ca poly(vinyl phosphonate) biocomposites. A template-driven nucleation and mineral growth process for the high-affinity integration of CDHA with polyhydroxyethyl methacrylate (PHEMA) hydrogel scaffold have been developed as well .
Polyetheretherketone (PEEK) [177, 179, 293, 294, 295, 296, 297, 298, 299] and high-impact polystyrene  were applied to create biocomposites with HA having a potential for clinical use in load-bearing applications. The study on reinforcing PEEK with thermally sprayed HA particles revealed that the mechanical properties increased monotonically with the reinforcement concentration, with a maximum value in the study of 40% volume fraction of HA particles [295, 296, 297]. The reported ranges of stiffness within 2.8–16.0 GPa and strength within 45.5–69 MPa exceeded the lower values for human bone (7–30 GPa and 50–150 MPa, respectively) . Modeling of the mechanical behavior of HA/PEEK biocomposites is available elsewhere .
Biodegradable poly(α-hydroxyesters) are well established in clinical medicine. Currently, they provide with a good choice when a suitable polymeric filler material is sought. For example, HA/PLGA composites were developed, which appeared to possess a cellular-compatibility suitable for bone tissue regeneration [301, 302, 303, 304, 305, 306, 307, 308]. Zhang and Ma [48, 233] seeded highly porous PLLA foams with HA particles in order to improve the osteoconductivity of polymer scaffolds for bone tissue engineering. They pointed out that hydration of the foams prior to incubation in simulated body fluid increased the amount of carbonated CDHA material due to an increase in COOH and OH groups on the polymer surface, which apparently acted as nucleation sites for apatite. The following values of Young’s modulus, compressive, bending, and tensile strengths for PLLA/HA composites have been achieved: 5–12 GPa, 78–137 MPa, 44–280 MPa, and 10–30 MPa, respectively . However, these data do not appear to be in a good agreement with HA/PLLA biocomposite unit cell model predictions .
On their own, PGA and PLA are known to degrade to acidic products (glycolic and lactic acids, respectively) that both catalyze polymer degradation and cause inflammatory reactions of the surrounding tissues . Thus, in biocomposites of poly(α-hydroxyesters) with calcium orthophosphates, the presence of slightly basic compounds (HA, TTCP) to some extent neutralizes the acid molecules, provides with a weak pH-buffering effect at the polymer surface and, therefore, more or less compensates these drawbacks [137, 312, 313, 314]. However, additives of even more basic chemicals (e.g., CaO, CaCO3) might be necessary [142, 313, 315, 316]. Extensive cell culture experiments on pH-stabilized composites of PGA and carbonateapatite were reported, which afterwards were supported by extensive in vitro pH-studies . A consequent development of this approach has led to designing of functionally graded composite skull implants consisting of polylactides, carbonateapatite, and CaCO3 [318, 319]. Besides the pH-buffering effect, inclusion of calcium orthophosphates was found to modify both surface and bulk properties of the biodegradable poly(α-hydroxyesters) by increasing the hydrophilicity and water absorption of the polymer matrix, thus altering the scaffold degradation kinetics. For example, polymer biocomposites filled with HA particles was found to hydrolyze homogeneously due to water penetrating into interfacial regions .
The mechanical properties of poly(α-hydroxyesters) could be substantially improved by the addition of calcium orthophosphates [326, 327]. Shikinami and Okuno  developed CDHA/PLLA composites of very high mechanical properties; mini-screws and mini-plates made of these composites have been manufactured and tested . They have shown easy handling and shaping according to the implant site geometry, total resorbability, good ability to bond directly to the bone tissue without interposed fibrous tissue, osteoconductivity, biocompatibility and high stiffness retainable for the period necessary to achieve bone union . The initial bending strength of 280 MPa exceeded that of cortical bone (120–210 MPa), while the modulus was as high as 12 GPa . The strength could be maintained above 200 MPa up to 25 weeks in phosphate-buffered saline solution. Such biocomposites were obtained from precipitation of a PLLA/dichloromethane solution, where small granules of uniformly distributed CDHA microparticles (average size of 3 μm) could be prepared . Porous scaffolds of poly-dl-lactic acid (PDLLA) and HA have been manufactured as well [268, 328, 329]. Upon implantation into rabbit femora, a newly formed bone was observed and biodegradation was significantly enhanced if compared with single-phase HA bioceramics. This might be due to a local release of lactic acid, which in turn dissolves HA. In other studies, PLA and PGA fibers were combined with porous HA scaffolds. Such reinforcement did not hinder bone ingrowth into the implants, which supported further development of such biocomposites as bone graft substitutes [47, 48, 309, 330, 331].
Recently, blends (named as SEVA-C) of ethylene-vinyl alcohol copolymer (EVOH) with starch filled with 10–30 wt% HA have been fabricated to yield biocomposites with modulus up to ~7 GPa with a 30% HA loading [332, 333, 334, 335, 336, 337]. The incorporation of bioactive fillers such as HA in SEVA-C aimed to assure the bioactive behavior of the composite and to provide the necessary stiffness within the typical range of human cortical bone properties. These biocomposites exhibited a strong in vitro bioactivity that was supported by the polymer’s water-uptake capability . However, the reinforcement of SEVA-C by HA particles was found to affect the rheological behavior of the blend. A degradation model of these biocomposites is available .
Higher homologues poly(3-hydroxybutyrate), 3-PHB, and poly(3-hydroxyvalerate), 3-PHV, show almost no biodegradation. Nevertheless, biocomposites of these polymers with calcium orthophosphates showed a good biocompatibility both in vitro and in vivo [94, 340, 341, 342, 343, 344, 345]. Both bioactivity and mechanical properties of these biocomposites can be tailored by varying the volume percentage of calcium orthophosphates. Similarly, biocomposites of poly(hydroxybutyrate-co-hydroxyvalerate) (PHBHV) with both HA and amorphous carbonated apatite (almost ACP) appeared to have a promising potential for repair and replacement of damaged bones [346, 347, 348, 349].
Along this line, PCL is used as a slowly biodegradable, a but well-biocompatible polymer. PCL/HA composites have been already discussed as suitable materials for substitution, regeneration, and repair of bone tissues [264, 350, 351, 352, 353, 354, 355, 356, 357]. For example, biocomposites were obtained by infiltration of ε-caprolactone monomer into porous apatite blocks and in situ polymerization . The composites were found to be biodegradable and might be applied as cancellous or trabecular bone replacement material or for cartilage regeneration. Both the mechanical performance and biocompatibility in osteoblast cell culture of PCL were shown to be strongly increased when HA was added . Several preparation techniques of PCL/HA composites are known. For example, to make composite fibers of PCL/nano-HA, the desired amount of nano-HA powder was dispersed in a solvent using magnetic stirrer followed by ultrasonication for 30 min. Then, PCL was dissolved in this suspension, followed by the solvent evaporation . The opposite preparation order is also possible: PCL was initially dissolved in chloroform at room temperature (7–10% weight/volume), then HA (∼10 μm particle size) was suspended in the solution, sonicated for 60 s, followed by the solvent evaporation  or salt-leaching . The mechanical properties obtained by this technique were about one-third that of trabecular bone. In a comparative study, PCL and biological apatite were mixed in the ratio 19:1 in an extruder . At the end of the preparation, the mixture was cooled in an atmosphere of nitrogen. The authors observed that the presence of biological apatite improved the modulus while concurrently increasing the hydrophilicity of the polymeric substrate. Besides, an increase in apatite concentration was found to increase both the modulus and yield stress of the composite, which indicated to good interfacial interactions between the biological apatite and PCL. It was also observed that the presence of biological apatite stimulated osteoblasts attachment to the biomaterial and cell proliferation . In another study, a PCL/HA biocomposite was prepared by blending in melt form at 120 °C until the torque reached equilibrium in the rheometer that was attached to the blender . Then the sample was compression-molded and cut into specimens of appropriate size for testing. It was observed that the composite containing 20 wt% HA had the highest strength . However, a direct grafting of PCL on the surface of HA particles seems to be the most interesting preparation technique . HA porous scaffolds were coated by a PCL/HA composite coating . In this system, PCL, as a coating component, was able to improve the brittleness and low strength of the HA scaffolds, whereas the particles in the coating were to improve the osteoconductivity and bioactivity of the coating layer. More complex PDLLA/PCL/HA biocomposites have been prepared as well . Further details on both PCL/HA biocomposites and processing methodologies thereof might be found elsewhere .
The spread of attached human osteoblasts onto PLA and PCL films reinforced with CDHA and sintered HA was shown to be higher than for the polymers alone . Moreover, biochemical assays relating cell activity to DNA content allowed concluding that cell activity was more intense for the composite films . Kim et al.  coated porous HA blocks with PCL from dichloromethane solution and performed drug-release studies. The antibiotic tetracycline hydrochloride was added into this layer, yielding a bioactive implant with drug release for longer than a week.
Both α-TCP and β-TCP have a higher solubility than HA (Table 3). Besides, they are faster resorbed in vivo.5 Therefore, these calcium orthophosphates were used instead of HA to prepare completely biodegradable biocomposites [376, 377, 378, 379, 380, 381, 382, 383, 384, 385, 386, 387, 388, 389, 390, 391, 392, 393, 394]. For example, a biodegradable and osteoconductive biocomposite made of β-TCP particles and gelatin was proposed . This material was tested in vivo with good results. It was found to be biocompatible, osteoconductive, and biodegradable with no need for a second surgical operation to remove the device after healing occurred. Herbal extracts might be added to this biocomposite . Another research group prepared biocomposites of crosslinked gelatin with β-TCP; they found both a good biocompatibility and bone formation upon subcutaneous implantation in rats . Yang et al.  extended this to porous (porosity about 75%) β-TCP/gelatin biocomposites those also contained BMP-4. Besides, cell-compatible and possessive some osteoinductive properties porous β-TCP/alginate-gelatin hybrid scaffolds were prepared and successfully tested in vitro . More to the point, biocomposites of β-TCP with PLLA [382, 383] and copolyester lactide-co-glycolide-co-ε-caprolactone  were prepared. Although β-TCP was able to counter the acidic degradation of the polyester to some extent, it did not prevent a pH drop down to ~6. Nevertheless, implantation of this biocomposite in beagles’ mandibular bones was successful .
Based on the self-reinforcement concept, biocomposites of TCP with polylactides were prepared and studied using conventional mechanical testing . Bioresorbable scaffolds were fabricated from such biocomposites . Chitosan was also used as the matrix for the incorporation of β-TCP by a solid/liquid phase separation of the polymer solution and subsequent sublimation of the solvent. Due to complexation of the functional groups of chitosan with calcium ions of β-TCP, these biocomposites had a better compressive modulus and strength . PCL/β-TCP biocomposites were developed as well [398, 399, 400, 401] and their in vitro degradation behavior was systematically monitored by immersion in simulated body fluid at 37 °C . To extend this topic further, the PCL/β-TCP biocomposites might be loaded by drugs .
Cell culture tests on β-TCP/PLLA biocomposites were reported; the biocomposites showed no cytotoxicity and evidenced good cell attachment to its surface . An in vitro study with primary rat calvarial osteoblasts showed an increased cellular activity in the BMP-loaded samples . Other researchers investigated BMP-2-loaded porous β-TCP/gelatin biocomposites (porosity 95%, average pore size 180–200 μm)  and confirmed the precious study. Biocomposites of β-TCP and glutaraldehyde crosslinked gelatin were manufactured and tested in vitro to measure the material cytotoxicity . The experimental results revealed that the amount of glutaraldehyde crosslinking agent should be less than 8% to decrease the toxicity on the osteoblasts and to avoid inhibition of cellular growth caused by the release of residual or uncrosslinked glutaraldehyde.
A long-term implantation study of PDLLA/α-TCP composites in a loaded sheep implant model showed good results after 12 months, but a strong osteolytic reaction after 24 months. This was ascribed to the almost complete dissolution of α-TCP to this time and an adverse reaction of the remaining PDLLA .
More complex calcium orthophosphate-based biocomposites are known as well. For example, there is a composite consisting of three interpenetrating networks: TCP, CDHA, and PLGA . Firstly, a porous TCP network was produced by coating a polyurethane foam by hydrolysable α-TCP slurry. Then, a CDHA network was derived from a calcium orthophosphate cement filled in the porous TCP network. Finally, the remaining open pore network in the CDHA/α-TCP structures was infiltrated with PLGA. This biocomposite consists of three phases with different degradation behavior. It was postulated that bone would grow on the fastest degrading network of PLGA, while the remaining calcium orthophosphate phases would remain intact thus maintaining their geometry and load-bearing capability .
Other calcium orthophosphate-based biocomposites
The number of research papers devoted to biocomposites based on other calcium orthophosphates is substantially lesser than those devoted to apatites and TCP. Biphasic calcium phosphate (BCP)6 appears to be the most popular among the remaining calcium orthophosphates. Collagen-coated BCP ceramics was studied and the biocompatibility toward osteoblasts was found to increase upon coating with collagen . Another research group created porous PDLLA/BCP scaffolds and coated them with a hydrophilic PEG/vancomycin composite for both drug-delivery purposes and surface modification . More to the point, PLGA/BCP composites were fabricated [407, 408] and their cytotoxicity and fibroblast properties were found to be acceptable for natural bone tissue reparation, filling, and augmentation [409, 410]. PCL/BCP biocomposites are known as well .
A choice of DCPD-based biocomposites of DCPD, albumin, and duplex DNA was prepared by water/oil/water interfacial reaction method . Core-shell type DCPD/chitosan biocomposite fibers were prepared by a wet spinning method in another study . The energy-dispersive X-ray spectroscopy analysis indicated that Ca and P atoms were mainly distributed on the outer layer of the composite fibers; however, a little amount of P atoms remained inside the fibers. This indicated that the composite fibers formed a unique core-shell structure with shell of calcium orthophosphate and core of chitosan . Although, this is not to the point, it is interesting to mention that some DCPD/polymer composites could be used as proton conductors in battery devices [413, 414]. Nothing has been reported on their biocompatibility but, perhaps, sometime the improved formulations will be used to fabricate biocompatible batteries for implantable electronic devices.
Various ACP-based biocomposites for dental applications were developed [415, 416, 417, 418]. Besides, several ACP-based formulations were investigated as potential biocomposites for bone grafting [349, 419, 420, 421]. Namely, ACP/PPF biocomposites were prepared by in situ precipitation , while PHB/carbonated ACP and PHBHV/carbonated ACP biocomposites appeared to be well suited as slowly biodegradable bone substitution material . Another example comprises hybrid nano-capsules of ~50–70 nm in diameter which were fabricated by ACP mineralization of shell crosslinked polymer micelles and nanocages . These nano-capsules consisted of a continuous ultrathin inorganic surface layer that infiltrated the outer crosslinked polymeric domains. They might be used as structurally robust, pH-responsive biocompatible hybrid nanostructures for drug delivery, bioimaging, and therapeutic applications .
Calcium orthophosphate cement-based biocomposites and concretes
Inorganic self-setting calcium orthophosphate cements, which harden in the body, were introduced by LeGeros et al.  and Brown and Chow [423, 424] in the early 1980s.7 Since then, these cements have been broadly studied and many formulations have been proposed . The cements set and harden due to various chemical interactions among calcium orthophosphates that finally lead to formation of a monolithic body consisting of either CHDA or DCPD with possible admixtures of other phases. Unfortunately, having the ceramic nature, calcium orthophosphate cements are brittle after hardening and the setting time is sometimes unsuitable for clinical procedures . Therefore, various attempts have been performed to transform the cements into biocomposites, e.g., by adding hydroxylcarboxylic acids, to control the setting time , gelatin to improve both the mechanical properties and the setting time [391, 429, 430, 431] or osteocalcin/collagen to increase the bioactivity . More to the point, various reinforcement additives of different shapes and nature are widely used to improve the mechanical properties of calcium orthophosphate cements . Even carbon nanotubes were used for this purpose ! Although the biomaterials community does not use this term, a substantial amount of the reinforced cement formulations might be defined as calcium orthophosphate-based concretes.8 The idea behind the concretes is simple: if a strong filler is present in the matrix, it might stop crack propagation.
Various apatite-containing biocomposite formulations based on PMMA [435, 436, 437, 438, 439, 440, 441, 442, 443, 444, 445] and PEMA [94, 446, 447] have been already developed. Such biocomposites might be prepared by dispersion of apatite powder into a PMMA viscous fluid  and used for drug-delivery purposes . When the mechanical properties of the biocomposite concretes composed of PMMA matrix and HA particles of various sizes were tested, the tensile results showed that strength was independent on particle sizes. In addition, up to 40 wt% HA could be added without impairing the mechanical properties [438, 439]. After immersion into Ringer’s solution, the tensile strength was not altered, whereas the fatigue properties were significantly reduced. The biocompatibility of PMMA/HA biocomposites was tested in vivo and enhanced osteogenic properties of the implants compared with single-phase PMMA were observed [436, 440, 441, 442, 443]. It was shown that not only the mechanical properties of PMMA were improved but the osteoblast response of PMMA was also enhanced with the addition of HA . Thereby, by adding calcium orthophosphates, a non-biodegradable PMMA was made more bioactive and osteoconductive, yielding a well-processable biocomposite concrete. As a drawback, the PMMA/HA formulations possess a low flexural, compressive, and tensile strength.
A biocomposite made from HA granules and bis-phenol-α-glycidylmethacrylate-based resin appeared to possess comparable mechanical and biological properties to typical PMMA cement, leading to potential uses for implant fixation . In order to improve the mechanical properties of calcium orthophosphate cements and stabilize them at the implant site, various researchers have resorted to formulations that set in situ, primarily through crosslinking reactions of the polymeric matrix. For example, TTCP was reacted with polyacrylic acid (PAA), forming a crosslinked CDHA/calcium polyacrylate biocomposite . In aqueous solutions, TTCP hydrolyzes to CDHA  and the liberated calcium cations react with PAA, forming the crosslinked network . Reed et al.  synthesized a dicarboxy polyphosphazene that can be crosslinked by calcium cations and cement-based (TTCP + DCPD) CDHA/polyphosphazene biocomposites with a compressive strength ~10 MPa and of ~65% porosity were prepared as a result. To mimic PMMA cements, PFF/β-TCP biocomposites were prepared with the addition of vinyl monomer to crosslink PPF. As a result, quick setting and degradable biocomposite cements with a low-heat output and compressive strengths in the range of 1 to 12 MPa were prepared by varying the molecular weight of PPF, as well as the contents of the monomer, β-TCP, initiator, and porogen (NaCl) [453, 454]. An acrylic cement with Sr-containing HA as a filler  and an injectable polydimethylsiloxane/HA cement  have been prepared as well.
In order to improve the mechanical properties of calcium orthophosphate cements, numerous researchers blended various polymers with the cements. For example, gelatin might be added to calcium orthophosphate cement formulations, primarily to stabilize the paste in aqueous solution before it develops adequate rigidity and, secondly, to improve the compressive strength [391, 429, 456]. Adding rod-like fillers to the cement formulations also caused an improvement in the mechanical properties . For example, PAA and PVA were successfully used to improve the mechanical properties of a TTCP + DCPD cement but, unfortunately, with an inevitable and unacceptable reduction of both workability and setting time [457, 458]. Similar findings were reported in the presence of sodium alginate and sodium polyacrylate . Other polymers, such as polyphosphazene, might be used as well [460, 461, 462]. Other examples of polymer/calcium orthophosphate cement formulations might be found elsewhere [463, 464].
Porous calcium orthophosphate scaffolds with interconnected macropores (∼1 mm), micropores (∼5 μm), and of high porosity (∼80%) were prepared by coating polyurethane foams with a TTCP + DCPA cement, followed by firing at 1200 °C. In order to improve the mechanical properties of the scaffolds, the open micropores of the struts were then infiltrated by a PLGA solution to achieve an interpenetrating bioactive ceramic/biodegradable polymer composite structure. The PLGA-filled struts were further coated with a 58S bioactive glass/PLGA composite coating. The obtained complex porous biocomposites could be used as tissue engineering scaffolds for low-load-bearing applications . A more complicated construction, in which the PLGA macroporous phase has been reinforced with a bioresorbable TTCP + DCPA cement, followed by surface coating of the entire construct by a non-stoichiomentic CDHA layer, has been designed as well . The latter approach has culminated in a unique, three-phase biocomposite that is simple to fabricate, osteoconductive, and completely biodegradable.
A porosity level of 42 to 80% was introduced into calcium orthophosphate cement/chitosan biocomposites by the addition of the water-soluble mannitol . Chitosan significantly improved the mechanical strength of the entire biocomposite . A similar approach was used by other researchers who studied the effect of the addition of PLGA microparticles [469, 470, 471, 472] (which can also be loaded with drugs or growth factors [473, 474, 475]) to calcium orthophosphate cements. These biocomposites were implanted into cranial defects of rats and a content of ~30 wt% of the microparticles was found to give the best results , while the addition of a growth factor to the biocomposites significantly increased bone contact at 2 weeks and enhanced new bone formation at 8 weeks . The in vivo rabbit femur implant tests showed that PLGA/calcium orthophosphate cement formulations exhibited outstanding biocompatibility and bioactivity, as well as a better osteoconduction and degradability than pure calcium orthophosphate cements . Further details on calcium orthophosphate cement-based biocomposites and concretes might be found in Ref. [427, chapter “Reinforced calcium orthophosphate cements”].
Nano-calcium orthophosphate-based biocomposites and nano-biocomposites
Nanophase materials are the materials that have grain sizes under ~100 nm. They have different mechanical and optical properties if compared with the large-grained materials of the same chemical composition. Namely, nanophase materials have the unique surface properties, such as an increased number of atoms, grain boundaries, and defects at the surface, huge surface area and altered electronic structure, if compared with the conventional micron-sized materials. For example, nano-HA (size ~67 nm) has a higher surface roughness of 17 nm if compared with 10 nm for the conventional submicron size HA (~180 nm), while the contact angles (a quantitative measure of the wetting of a solid by a liquid) are significantly lower for nano-HA (6.1) if compared with the conventional HA (11.51). Additionally, the diameter of individual pores in a nano-HA compact is five times smaller (pore diameter ~6.6 Å) than that in the conventional grain-sized HA compacts (pore diameter within 19.8–31.0 Å) [476, 477, 478]. Besides, nano-HA promotes osteoblast cells adhesion, differentiation, and proliferation, osteointegration and deposition of calcium containing minerals on its surface better than microcrystalline HA; thus enhancing formation of a new bone tissue within a short period [476, 477, 478]. More to the point, nano-HA was found to cause apoptosis of the leukemia P388 cells .
Composites of two or more materials, in which at least one of the materials is of a nanometer-scale, are defined as nanocomposites . Natural bone mineral is a hierarchical nanocomposite of biological origin, because it consists of nano-sized blade-like crystals of biological apatite grown in intimate contact with an organic matrix rich in collagen fibers and organized in a complicated hierarchical structure [21, 22, 38]. Given the fact that the major organic phase of bone is collagen, i.e., a natural polymer (Table 1), it is obvious that a composite of a nanophase calcium orthophosphate with a biodegradable polymer should be advantageous as bone substitution material. The inorganic nanophase would be responsible for the mechanical strength (hardness) and bioactivity, while the polymer phase would provide the elasticity. In addition, the solubility of calcium orthophosphates depends on their crystallite size (smaller crystals have a higher solubility) and on their carbonate content (higher carbonate content increases the solubility) . To the author’s best knowledge, among calcium orthophosphates listed in Table 3, before very recently only apatites (CDHA, HA and, perhaps, FA) have been available in the nanocrystalline state. However, very recently, nano-DCPA [481, 482, 483] and nano-MCPM  have been synthesized and applied to prepare nano-biocomposites with strong ionic release to combat tooth caries.
A number of investigations have been conducted recently to determine the mineralization, biocompatibility, and mechanical properties of the nano-biocomposites based on various (bio)polymers and nano-HA.9 These studies covered nano-HA/PLA [268, 485, 486, 487, 488, 489, 490, 491, 492] and its copolymer with PGA [493, 494, 495], nano-HA/collagen [496, 497, 498, 499, 500, 501, 502, 503, 504, 505, 506, 507, 508], nano-HA/collagen/PLA [508, 509, 510, 511, 512, 513, 514, 515, 516], nano-HA/collagen/PVA , nano-HA/collagen/alginate [518, 519], nano-HA/gelatin [520, 521, 522, 523, 524, 525], nano-HA/poly(hexamethylene adipamide) , nano-HA/PPF , nano-HA/polyamide [528, 529, 530, 531, 532, 533, 534, 535, 536, 537, 538, 539], nano-HA/PVA [276, 277, 540, 541, 542], nano-HA/PVAP , nano-HA/poly(ethylene-co-acrylic) acid [543, 544], nano-HA/chitosan [545, 546, 547, 548], nano-HA/konjac glucomannan/chitosan , nano-HA/PHEMA/PCL , nano-HA/PCL [322, 359, 551, 552], nano-HA/Ti [553, 554], PCL semi-interpenetrating nanocomposites , and many other biocompatible hybrid formulations [223, 257, 271, 347, 556, 557, 558, 559, 560, 561, 562, 563, 564, 565, 566, 567, 568, 569, 570, 571, 572, 573, 574]. Several nano-biocomposites were found to be applicable as carriers for growth factors delivery [34, 575, 576]. Besides, the data are available on the excellent biocompartibility of such nano-biocomposites . The dispersion state of nanoparticles appears to be the critical parameter in controlling the mechanical properties of nano-biocomposites, as nanoparticles always tend to aggregate owing to their high surface energy .
Porous (porosity ~85%) biocomposites of nano-HA with collagen and PLA have been prepared by precipitation and freeze-drying; the nano-biocomposites did not show a pH drop upon in vitro degradation [509, 510, 511]. They were implanted in the radius of rabbits and showed a high biocompatibility and partial resorption after 12 weeks. Nano-HA/chitosan biocomposites with improved mechanical stability were prepared from HA/chitosan nanorods . Nano-HA/PLLA biocomposites of high porosity (~90%) were prepared using thermally induced phase separation . Besides, nano-HA was used to prepare biocomposites with PAA and the nanostructure of the resulting nanocrystals exhibited a core-shell configuration [579, 580].
Nano-HA crystals appeared to be suitable for intraosseous implantation and offered a potential to formulate enhanced biocomposites for clinical applications . Thus, the biocompatibility of chitosan in osteoblast cell culture was significantly improved by addition of nano-HA . Similar finding is valid for nano-HA/polyamide biocomposites . Further details on nano-HA-based biocomposites might be found in an excellent review . More to the point, a more general review on nanobiomaterial applications in orthopedics is also available , where the interested readers are referred.
Biocomposites with collagen
The main constituent of the bioorganic matrix of bones is type I collagen10 (Table 1) with molecules about 300 nm in length. This protein is conducive to crystal formation in the associated inorganic matrix. It is easily degraded and resorbed by the body and allows good attachment to cells. Collagen alone is not effective as an osteoinductive material, but it becomes osteoconductive in combination with calcium orthophosphates . Both collagen type I and HA were found to enhance osteoblast differentiation  but combined together, they were shown to accelerate osteogenesis. However, this tendency is not so straightforward: the data are available that implanted HA/collagen biocomposites enhanced regeneration of calvaria bone defects in young rats but postponed the regeneration of calvaria bone in aged rats . Finally, the addition of calcium orthophosphates to collagen sheets was found to give a higher stability and an increased resistance to 3D swelling compared with the collagen reference . Therefore, a bone-analogue based on these two constituents should possess the remarkable properties. Furthermore, the addition of bone marrow constituents gives osteogenic and osteoinductive properties to calcium orthophosphate/collagen biocomposites .
The unique characteristics of bones are the spatial orientation between the calcium orthophosphate nanophase and collagen macromolecules at the nanolevel , where nanocrystals (about 50-nm-length) of biological apatite are aligned parallel to the collagen fibrils [21, 22, 31, 38], which is believed to be the source of the mechanical strength of bones. The collagen molecules and the nanocrystals of biological apatite assembled into mineralized fibrils are approximately 6-nm-diameter and 300-nm-long [31, 35, 38, 510, 589]. Although the complete mechanisms involved in the bone building strategy are still unclear, the strengthening effect of apatite nanocrystals in calcified tissues might be explained by the fact that the collagen matrix is a load transfer medium and thus transfers the load to the intrinsically rigid inorganic nanocrystals. Furthermore, nanocrystals of biological apatite located in between tangled fibrils crosslink the fibers either through a mechanical interlocking or by forming calcium ion bridges, thus increasing deformation resistance of the collagenous fiber network .
When calcium orthophosphates are combined with collagen in a laboratory, the biocomposites appear to be substantially different from natural bone tissue due to a lack of real interaction between the two components, i.e., interactions that are able to modify the intrinsic characteristics of the singular components themselves. The main characteristics of the route, by which the mineralized hard tissues are formed in vivo, are that the organic matrix is laid down first and the inorganic reinforcing phase grows within this organic matrix [21, 22, 31, 38]. Although to date, neither the elegance of the biomineral assembly mechanisms nor the intricate composite nano-architectures have been duplicated by non-biological methods, the best way to mimic bone is to copy the way it is formed, namely by nucleation and growth of CDHA nanocrystals from a supersaturated solution both onto and within the collagen fibrils [591, 592, 593]. Such syntheses were denoted as “biologically inspired” which means they reproduce an ordered pattern and an environment very similar to natural ones [594, 595, 596]. The biologically inspired biocomposites of collagen and calcium orthophosphates (mainly, apatites) for bone substitute have a long history [29, 364, 499, 597, 598, 599, 600, 601, 602, 603, 604, 605, 606, 607, 608, 609, 610, 611, 612, 613, 614, 615] and started from the pioneering study by Mittelmeier and Nizard , who mixed calcium orthophosphate granules with a collagen web. Such combinations were found to be bioactive, osteoconductive, osteoinductive [29, 585, 617, 618, 619] and, in general, artificial grafts manufactured from this type of the biocomposites are likely to behave similarly to bones and be of more use in surgery than those prepared from any other materials. Indeed, some data are available on the superiority of calcium orthophosphate/collagen biocomposite scaffolds over the artificial polymeric and calcium orthophosphate bioceramic scaffolds individually .
It has been found that calcium orthophosphates may be successfully precipitated onto a collagen substrate of whatever form or source [29, 36, 499, 621, 622]. However, adherence of calcium orthophosphate crystals to collagen did depend on how much the collagen had been denatured: the more fibrillar the collagen, the greater attachment. Clarke et al.  first reported the production of a biocomposite produced by precipitation of DCPD onto a collagen matrix with the aid of phosphorylated amino acids commonly associated with fracture sites. Apatite cements (DCPD + TTCP) have been mixed with a collagen suspension, hydrated, and allowed to set. CDHA crystals were found to nucleate on the collagen fibril network, giving a material with the mechanical properties weaker than those reported for bone. More to the point, these biocomposites were without the nanostructure similar to that of bone [599, 623]. The oriented growth of OCP crystals on collagen was achieved by an experimental device in which Ca2+ and PO43− ions diffused into a collagen disk from the opposite directions [622, 624, 625]. Unfortunately, these experiments were designed to simulate the mechanism of in vivo precipitation of biological apatite only; due to this reason, the mechanical properties of the biocomposites were not tested .
Conventionally, collagen/calcium orthophosphate biocomposites can be prepared by blending or mixing of collagen and calcium orthophosphates, as well as by biomimetic methods [29, 32, 34, 37, 496, 499, 510, 576, 589, 594, 595, 596, 599, 621, 627, 628, 629, 630, 631, 632, 633]. Besides, collagen might be incorporated into calcium orthophosphate cements [599, 623, 634]. Typically, the type I collagen sponge is presoaked in PO43−-containing a highly basic aqueous solution and then is immersed into a Ca2+-containing solution to allow mineral deposition. Also, collagen I fibers might be dissolved in acetic acid and then this solution is added to phosphoric acid, followed by the neutralization synthesis (performed at 25 °C and solution pH within 9–10) between an aqueous suspension of Ca(OH)2 and the H3PO4/collagen solution [594, 595]. In order to ensure the quality of the final product, it is necessary to control the Ca/P ionic ratio in the reaction solution. One way to do this is to dissolve a commercial calcium orthophosphate in an acid; another is to add Ca2+ and PO43− ions in a certain ratio to the solution and after that induce the reaction . Biomimetically, one can achieve an oriented growth of CDHA crystals onto dissolved collagen fibrils in aqueous solutions via a self-organization mechanism . A number of authors produced calcium orthophosphate/collagen biocomposites by mixing preformed ceramic particles with a collagen suspension [635, 636, 637]. However, in all blended composites, the crystallite sizes of calcium orthophosphates were not uniform and the crystals were often aggregated and randomly distributed within a fibrous matrix of collagen. Therefore, no structural similarity to natural bone was obtained, and only a compositional similarity to that of natural bone was achieved. Crystallization of CDHA in aqueous solutions might be performed in the presence of a previously dispersed collagen [29, 499]. More to the point, collagen might be first dispersed in an acidic solution, followed by addition of calcium and orthophosphate ions and then coprecipitation of collagen and CDHA might be induced by either increasing the solution pH or adding mixing agents . Although it resulted in biocomposites with poor mechanical properties, pressing of the HA/collagen mixtures at 40 °C under 200 MPa for several days is also known . Attempts have been performed for a computer simulation of apatite/collagen composite formation process . It is interesting to note, that collagen/HA biocomposites were found to possess some piezoelectric properties .
As the majority of the collagen/HA, biocomposites are conventionally processed by anchoring micro-HA particles into collagen matrix, it makes quite difficult to obtain a uniform and homogeneous composite graft. Besides, such biocomposites have inadequate mechanical properties; over and above, the proper pore sizes have not been achieved either. Further, microcrystalline HA, which is in contrast to nanocrystalline natural bone apatite, might take a longer time to be remodeled into a new bone tissue upon the implantation. In addition, some of the biocomposites exhibited very poor mechanical properties, probably due to a lack of strong interfacial bonding between the constituents. The aforementioned data clearly demonstrate that the chemical composition similar to bone is insufficient for manufacturing the proper bone grafts; both the mechanical properties and mimetic of the bone nanostructure are necessary to function as bone in recipient sites. There is a chance for improving osteointegration by reducing the grain size of HA crystals by activating ultrafine apatite growth into the matrix. This may lead to enhance the mechanical properties and osteointegration with improved biological and biochemical affinity to the host bone. Besides, the unidirectional porosity was found to have a positive influence on the ingrowth of the surrounding tissues into the pores of collagen/HA biocomposites .
Bovine collagen might be mixed with HA and such biocomposites are marketed commercially as bone-graft substitutes those further can be combined with bone marrow aspirated from the iliac crest of the site of the fracture. Application of these materials was compared with autografts for the management of acute fractures of long bones with defects, which had been stabilized by internal or external fixation [642, 643]. These biocomposites are osteogenic, osteoinductive, and osteoconductive; however, they lack the structural strength and require harvest of the patient’s bone marrow. Although no transmission of diseases has been recorded yet, the use of bovine collagen might be a source of concern .
Collagen sponges with an open porosity (30–100 μm) were prepared by a freeze-drying technique and then their surface was coated by a 10-μm layer of biomimetic apatite precipitated from simulated body fluid . The researchers found a good in vitro performance with fibroblast cell culture. Collagen/HA microspheres or gel beads have been prepared in the intention of making injectable bone fillers [645, 646]. Liao et al.  succeeded in mimicking the bone structure by blending carbonateapatite with collagen. A similar material (mineralized collagen) was implanted into femur of rats and excellent clinical results were observed after 12 weeks . Collagen/HA biocomposites were prepared and their mechanical performance was increased by crosslinking the collagen fibers with glutaraldehyde [500, 502, 503]. These biocomposites were tested in rabbits and showed a good biological performance, osteoconductivity, and biodegradation. A similar approach was selected to prepare HA/collagen microspheres (diameter ~5 μm) by a water–oil emulsion technique in which the surface was also crosslinked by glutaraldehyde . That material showed a good in vitro performance with osteoblast cell culture. A porous bone-graft substitute was formed from a nano-HA/collagen biocomposite combined with PLA by a freeze-drying method; the resulting material was found to mimic natural bone at several hierarchical levels . Subsequent in vitro experiments confirmed a good adhesion, proliferation, and migration of osteoblasts into this composite . A further increase in biocompatibility might be achieved by the addition of silicon; thus, to enhance bone substitution, Si-substituted HA/collagen composites have been developed with silicon located preferentially in the collagen phase . Porous (porosity level ~95% with interconnected pores of 50–100 μm) biocomposites of collagen (crosslinked with glutaraldehyde) and β-TCP have been prepared by a freeze-drying technique, followed by sublimation of the solvent; the biocomposites showed a good biocompatibility upon implantation in the rabbit jaw .
Biocomposites of calcium orthophosphates with collagen were found to be useful for drug-delivery purposes [519, 607, 650, 651, 652]. Namely, an HA/collagen–alginate (20 μL) with the rh-BMP2 (100 μg/mL, 15 μL) showed bone formation throughout the implant 5 weeks after implantation without obvious deformation of the material . Gotterbarm et al.  developed a two-layered collagen/β-TCP implant augmented with chondral inductive growth factors for the repair of osteochondral defects in the trochlear groove of minipigs. This approach might be a new promising option for the treatment of deep osteochondral defects in joint surgery.
To conclude this part, one should note that biocomposites of apatites with collagen are a very hot topic of the research and up to now, just a few papers are devoted to biocomposites of other calcium orthophosphates with collagen [651, 653]. These biomaterials mimic natural bones to some extent, while their subsequent biological evaluation suggests that they are readily incorporated into the bone metabolism in a way similar to bone remodeling, instead of acting as permanent implant [510, 616]. Collagraft®, Bio-Oss®, and Healos® are the several examples of the commercially available calcium orthophosphate/collagen bone grafts for clinical use . However, the performance of these biocomposites depends on the source of collagen from which it was processed. Several attempts have been made to simulate the collagen–HA interfacial behavior in real bone by means of crosslinking agents such as glutaraldehyde [500, 502, 503, 621, 646, 649] with the purpose to improve the mechanical properties of these biocomposites. Unfortunately, a further progress in this direction is restricted by a high cost, difficulty to control cross-infection, a poor definition of commercial sources of collagens, as well as by a lack of an appropriate technology to fabricate bone-resembling microstructures. Further details on calcium orthophosphate/collagen composites, including the list of the commercially available products, might be found elsewhere [32, 611].
Biocomposites with other bioorganic compounds and biological macromolecules
Besides collagen, both human and mammalian bodies contain dozens types of various bioorganic compounds, proteins, and biological macromolecules. The substantial amounts of them potentially might be used to prepare biocomposites with calcium orthophosphates. For example, a biologically strong adhesion (to prevent invasion of bacteria) between teeth and the surrounding epithelial tissues is attributed to a cell-adhesive protein, laminin . In order to mimic the nature, a laminin/apatite biocomposite layer was successfully created on the surface of both titanium  and EVOH [656, 657] using the biomimetic approach.
Calcium orthophosphate/gelatin biocomposites are widely investigated as potential bone replacement biomaterials [254, 272, 273, 274, 366, 367, 368, 369, 370, 371, 372, 373, 374, 385, 386, 387, 388, 389, 390, 391, 392, 402, 429, 430, 431, 456, 520, 521, 522, 523, 524, 525, 658, 659, 660, 661, 662, 663, 664, 665, 666, 667, 668, 669]. For example, gelatin foams were successfully mechanically reinforced by HA and then crosslinked by a carbodiimide derivative . Such foams were shown to be a good carrier for antibiotic tetracycline . Several biocomposites of calcium orthophosphates with alginates11 have been prepared [389, 518, 519, 523, 595, 670]. For example, porous HA/alginate composites based on hydrogels were prepared both biomimetically  and by using a freeze-drying technique . Another research group succeeded in preparation of biphasic but monolithic scaffolds using a similar preparation route . Their biocompatibility in cell culture experiments and in vitro biodegradability were high; however, a mechanical strength could be better.
Various biocomposites of calcium orthophosphates with chitosan [239, 397, 412, 419, 435, 467, 545, 546, 547, 548, 549, 566, 567, 577, 582, 663, 669, 672, 673, 674, 675, 676, 677, 678, 679, 680, 681, 682, 683] and chitin [183, 394, 513, 684, 685, 686, 687, 688] are also very popular. For example, a solution-based method was developed to combine HA powders with chitin, in which the ceramic particles were uniformly dispersed [684, 685]. Unfortunately, it was difficult to obtain the uniform dispersions. The mechanical properties of the final biocomposites were not very good; due to a poor adhesion between the filler and the matrix both the tensile strength and modulus were found to decrease with the increase in the HA amount. Microscopic examination revealed that HA particles were intervened between the polymer chains, weakening their interactions, and decreasing the entire strength [684, 685].
Biocomposites of CDHA with water-soluble proteins, such as bovine serum albumin (BSA), might be prepared by a precipitation method [463, 689, 690, 691, 692]. In such biocomposites, BSA is not strongly fixed to solid CDHA, which is useful for a sustained release. However, this is not the case if a water/oil/water interfacial reaction route has been used . To extend this subject, inclusion of DNA into CDHA/BSA biocomposites was claimed [250, 693, 694, 695]. Besides, bionanocomposites of an unspecified calcium orthophosphate with DNA were prepared as well .
Akashi and co-workers  developed a procedure to prepare calcium orthophosphate-based biocomposites by soaking hydrogels in supersaturated by Ca2+ and PO43− ions solutions in order to precipitate CDHA in the hydrogels (up to 70 wt% of CDHA could be added to these biocomposites). This procedure was applied to chitosan; the 3D shape of the resulting biocomposite was controlled by the shape of the starting chitosan hydrogel . Another research group developed biocomposites based on in situ calcium orthophosphate mineralization of self-assembled supramolecular hydrogels .
Various biocomposites of CDHA with glutamic and aspartic amino acids, as well as poly-glutamic and poly-aspartic amino acids have been prepared and investigated by Bigi et al. [279, 281, 700, 701, 702, 703]. These (poly)amino acids were quantitatively incorporated into CDHA crystals, provoking a reduction of the coherent length of the crystalline domains and decreasing the crystal sizes. The relative amounts of the (poly)amino acid content in the solid phase, determined through HPLC analysis, increased with their concentration in solution up to a maximum of about 7.8 wt% for CDHA/aspartic acid and 4.3 wt% for CDHA/glutamic acid biocomposites. The small crystal dimensions, which implied a great surface area, and the presence of (poly)amino acids were suggested to be relevant for possible application of these biocomposites for hard tissues replacement [279, 281, 700, 701, 702, 703].
Recently, BCP (HA + β-TCP)/agarose macroporous scaffolds with controlled and complete interconnection, high porosity, thoroughly open pores, and tailored pore size were prepared for tissue engineering application [704, 705]. Agarose, a biodegradable polymer, was selected as the organic matrix, because it was a biocompatible hydrogel, which acted as gelling agent leading to strong gels and fast room temperature polymerization. Porous scaffolds with the designed architecture were manufactured by combining a low-temperature shaping method with stereo-lithography and two drying techniques. The biocompatibility of this BCP/agarose system was tested with mouse L929 fibroblast and human Saos-2 osteoblast during different colonization times .
Fibrin sealants are non-cytotoxic, fully resorbable, biological matrices that simulate the last stages of a natural coagulation cascade, forming a structured fibrin clot similar to a physiological clot . Biocomposites of calcium orthophosphates with fibrin sealants might develop the clinical applications of bone substitutes. The 3D mesh of fibrin sealant interpenetrates the macro- and micro-porous structure of calcium orthophosphate ceramics . The physical, chemical, and biological properties of calcium orthophosphate bioceramics and the fibrin glue might be cumulated in biocomposites, suitable for preparation of advanced bone grafts [707, 708, 709, 710, 711, 712, 713, 714, 715, 716, 717, 718].
Furthermore, there are biocomposites of calcium orthophosphates with bisphosphonates , silk fibroin (that is a hard protein extracted from silk cocoon) [249, 562, 563, 564, 569, 570, 720, 721, 722, 723, 724, 725], chitosan + silk fibroin , fibronectin , and casein phosphopeptides . Besides, the reader’s attention is pointed out to an interesting approach to crystallize CDHA inside poly(allylamine)/poly(styrene sulfonate) polyelectrolyte capsules resulting in empty biocomposite spheres of micron size . Depending on the amount of precipitated CDHA, the thickness of the shell of biocomposite spheres can be varied between 25 and 150 nm. These biocomposite capsules might find application as medical agents for bone repairing and catalytic microreactors .
Injectable bone substitutes
IBS represent ready-to-use suspensions of calcium orthophosphate powder(s) in a liquid carrier phase. They look like viscous pastes with the rheological properties, sufficient to inject them into bone defects by means of surgical syringes and needles. Usually, the necessary level of viscosity is created by the addition of water-soluble polymers [104, 730, 731]. Therefore the majority of calcium orthophosphate-based IBS formulations might be considered as a subgroup of calcium orthophosphate/polymer biocomposites. For example, an IBS was described that involved a silanized hydroxyethylcellulose carrier with BCP, consisting of HA and β-TCP . The suspension is liquid at pH within 10–12, but gels quickly at pH < 9. Injectable composites can be formed with β-TCP to improve mechanical integrity . Similarly, Bennett et al.  showed that a polydioxanone-co-glycolide-based biocomposite reinforced with HA or β-TCP can be used as an injectable or moldable putty. During the crosslinking reaction following injection, carbon dioxide is released allowing the formation of interconnected pores.
Daculsi et al. [84, 731, 734, 735, 736, 737, 738, 739, 740] developed viscous IBS biocomposites based on BCP (60% HA + 40% β-TCP) and 2% aqueous solution of hydroxypropylmethylcellulose (HPMC) that was said to be perfectly biocompatible, resorbable, and easily fitted bone defects (due to an initial plasticity). The best ratio BCP/HPMC aqueous solution was found to be at ~65/35 w/w. To extend this subject further, this type of IBS might be loaded by cells  or by microparticles .
The advanced characteristics of IBS come from their good mechanical properties and biocompatibility and the ease of tissue regeneration. Although the fabrication of IBS biocomposites in most cases improved the mechanical properties of the system and provided the material with resistance to fluids penetration, these achievements were limited by the amount of polymer that can be added to the paste. For instance, Mickiewicz et al.  reported that after a critical concentration (that depended on the type and molecular weight of the polymer, but was always around 10%), the polymer started forming a thick coating on the crystal clusters, preventing them from interlocking, originating plastic flow and, as a consequence, decreasing mechanical properties. More to the point, Fujishiro et al.  reported a decrease in mechanical properties with higher amounts of gel, which was attributed to the formation of pores due to leaching of gelatin in solution. Therefore, it seems that mechanical properties, although improved by the addition of polymers, are still a limitation for the application of calcium orthophosphate-based IBS formulations in load-bearing sites .
Biocomposites with glasses, inorganic materials, and metals
In order to overcome the problem of poor mechanical properties of calcium orthophosphate bioceramics, suitable biocomposites of calcium orthophosphates reinforced by various inorganic materials, glasses, and metals have been developed. Such biocomposites are mainly prepared by the common ceramic processing techniques such as thermal treatment after kneading [743, 744, 745], powder slurry coating , and metal–sol mixing . For example, HA was combined with Bioglass® (Novabone Products, Alachua, FL) [748, 749] and with other glasses  to form glass–ceramics biocomposites. Other reinforcement materials for calcium orthophosphates are differentiated by either shape of the fillers, namely, particles [751, 752], platelets [753, 754], whiskers [484, 755, 756], fibers [757, 758, 759], or their chemical composition: zirconia and/or PSZ [250, 743, 744, 745, 746, 755, 760, 761, 762, 763, 764, 765, 766, 767, 768, 769, 770, 771, 772, 773, 774, 775, 776, 777, 778, 779, 780, 781, 782, 783, 784, 785, 786, 787, 788, 789, 790, 791, 792, 793], alumina [250, 751, 754, 793, 794, 795, 796, 797, 798, 799, 800, 801, 802], titania [307, 747, 752, 803, 804, 805, 806, 807, 808, 809, 810, 811, 812, 813, 814, 815, 816, 817], other oxides [818, 819, 820, 821], silica and/or glasses [822, 823, 824, 825, 826, 827, 828, 829], wollastonite [171, 830, 831, 832, 833, 834, 835, 836, 837], various metals and alloys [759, 794, 817, 838, 839, 840, 841, 842, 843, 844, 845, 846, 847, 848, 849, 850, 851], calcium sulfate [852, 853, 854], silicon carbide , barium titanate , zeolite , and several other materials [271, 857, 858, 859]. All these materials have been added to calcium orthophosphate bioceramics to improve its reliability. Unfortunately, significant amounts of the reinforcing phases are needed to achieve the desired properties and, as these materials are either bioinert, significantly less bioactive than calcium orthophosphates or not bioresorbable, the ability of the biocomposites to form a stable interface with bone is poorer if compared with calcium orthophosphate bioceramics alone. Due to the presence of bioinert compounds, such formulations might be called bioinert/bioactive composites . The ideal reinforcement material would impart mechanical integrity to a biocomposite at low loadings, without diminishing its bioactivity. As clearly seen from the amount of the references, apatite/zirconia biocomposites are most popular ones among the researchers.
There are several types of HA/glass biocomposites. The first one is also called bioactive glass–ceramics. A dense and homogeneous biocomposite was obtained after a heat treatment of the parent glass, which comprised ~38 wt% oxy-FAP (Ca10(PO4)6(O,F)2) and ~34 wt% β-wollastonite (CaO · SiO2) crystals, 50–100 nm in size in a MgO–CaO–SiO2 glassy matrix [171, 830, 831, 832, 833, 834, 835, 836, 837]. A-W glass–ceramics is an assembly of small apatite particles effectively reinforced by wollastonite. The bending strength, fracture toughness, and Young’s modulus of A-W glass–ceramics are the highest among bioactive glass and glass ceramics, enabling it to be used in some major compression load-bearing applications, such as vertebral prostheses and iliac crest replacement. It combines a high bioactivity with the suitable mechanical properties . β-TCP/wollastonite biocomposites are also known [861, 862, 863]. More complicated biocomposites have been developed as well. For example, (A-W)/HDPE composite (AWPEX) biomaterials have been designed to match the mechanical strength of human cortical bone and to provide favorable bioactivity, with potential use in many orthopedic applications [864, 865, 866, 867]. Other examples comprise wollastonite-reinforced HA/Ca polycarboxylate  and glass-reinforced HAP/polyacrylate  biocomposites.
HA/glass biocomposites can be prepared by simple sintering of appropriate HA/glass powder mixtures [870, 871, 872, 873]. If sintering is carried out below 1000 °C, HA does not react with the bioactive glass [871, 872] or this reaction is limited . Besides, reaction between HA and glasses depends on the glass composition. In another approach, small quantities of bioactive glass have been added to HA bioceramics in order to improve densification and/or mechanical properties . In addition, biocomposites might be sintered from HA and silica . In general, bioactive glass–ceramics maintain a high strength for a longer time than HA bioceramics under both the in vitro and in vivo conditions [829, 834].
Carbon nanotubes with their small dimensions, a high-aspect-ratio (length-to-diameter) as well as the exceptional mechanical properties, including extreme flexibility and strength, significant resistance to bending, high resilience and the ability to reverse any buckling of the tube, have the excellent potential to accomplish necessary mechanical properties . Recent studies have even suggested that they may possess some bioactivity [875, 876, 877, 878]. However, due to a huge difference in shapes, it is a challenge to prepare homogeneous mixtures of calcium orthophosphates and carbon nanotubes: “one can imagine something similar to achieving a homogeneous mixture of peas and spaghetti” [874, p. 7]. Additionally, non-functionalized carbon nanotubes tend to agglomerate and form bundles; besides, they are soluble in neither water nor organic solvents. Chemical functionalization allows carbon nanotubes to be dispersed more easily, which can improve interfacial bonding with calcium orthophosphates [247, 874].
Different strategies might be employed to prepare calcium orthophosphate/carbon nanotubes biocomposites. For example, apatites might be chemically synthesized using carboxyl-functionalized carbon nanotubes as a matrix [242, 243, 244, 245, 246, 247]. Physico-chemical characterization of these biocomposites showed that nucleation of CDHA initiates through the carboxyl group . Hot-pressing , plasma spraying , and laser surface alloying [881, 882, 883] techniques might be applied as well. The research on calcium orthophosphate (up to now, only apatites)/carbon nanotube biocomposites is in its early stages, with the first papers published in 2004 [246, 433]. Due to this reason, the mechanical property data for such biocomposites have been reported only in few papers; however, these results are encouraging. For example, Chen et al.  performed nanoindentation tests on biocomposite coatings to give hardness and Young’s modulus values. They found that the higher the loading of nanotubes, the better the properties. Namely, at 20 wt% loading, hardness was increased by 43% and Young’s modulus by 21% over a single-phase HA coating . Scratching test results indicated that as alloyed HA biocomposite coatings exhibited improved wear resistance and lower friction coefficient with increasing the amount of carbon nanotubes in the precursor material powders . Additionally, measurements of the elastic modulus and hardness of the biocomposite coatings indicated that the mechanical properties were also affected by the amount of carbon nanotubes . Another research group performed compression tests on bulk HA/nanotubes biocomposites and found an increase in strength over single-phase HA . However, the highest compressive strength they achieved for any material was only 102 MPa, which is similar to that of cortical bone but much lower than the typical values for dense HA . More complex formulations, such as poly-l-lysine/HA/carbon nanotube hybrid nanocomposites, have also been developed . Unfortunately, carbon nanotubes are very stable substances; they are neither bioresorbable nor biodegradable. Therefore, during the in vivo bioresorption, the nanotubes will get into the human body from the biocomposite matrix and might cause uncertain health problems. Except of carbon nanotubes, carbon fibers of microscopic dimensions are also used to reinforce HA bioceramics [885, 886, 887].
The main disadvantage of HA reinforced by PSZ is degradation of zirconia in wet environments [755, 760, 761, 783]. Transformation of the tetragonal ZrO2 to the monoclinic phase on the surface results in formation of microcracks and consequently lowers the strength of the implant [888, 889].
An HA-based biocomposite reinforced with 20 vol.% of Ti particles was fabricated by hot-pressing . Besides, calcium orthophosphates/Ti biocomposites might be prepared by powder metallurgy processing [842, 843, 844]. At high temperatures, the presence of Ti metal phase was found to promote dehydration and decomposition of HA into β-TCP and TTCP [840, 842] or partial formation of β-TCP and calcium titanate instead of HA [554, 843, 844]. Comparing with pure HA bioceramics manufactured under the same conditions, the HA/Ti biocomposites possessed a higher fracture toughness, bending strength, work of fracture, porosity, and lower elastic modulus, which is more suitable for biomedical applications. However, the mechanical properties appeared to be not high enough to use HA/Ti biocomposites in load-bearing applications. Luckily, the histological evaluations revealed that HA/Ti biocomposites could be partially integrated with newborn bone tissues after 3 weeks and fully osteointegrated at 12 weeks in vivo . Similar findings had been earlier made for HA bioceramics reinforced by addition of silver particulates (5–30 vol.%) and subsequent sintering of the HA/Ag powder compacts [838, 839]. Other studies on calcium orthophosphate/Ti biocomposites are available elsewhere [845, 846, 847, 848].
To conclude this part, biocomposites consisting of calcium orthophosphates only should be briefly described. First of all, BCP itself, consisting of HA and α- or β-TCP, should be mentioned . In the 1980s, BCP was called as “TCP ceramics complexed with HA” . More to the point, 70% HA-powder + 30% HA-whisker biocomposites have been fabricated by pressureless sintering, hot-pressing, and hot-isostatic pressing. These biocomposites were found to exhibit an improved toughness, attaining the lower fracture-toughness limit of bone without a decrease of bioactivity and biocompatibility [891, 892]. Besides, a dual HA biocomposite that combined two HA materials with different porosities: HA with 75% porosity, for bone ingrowth and HA with 0% porosity, for load-bearing was manufactured. This dual HA biocomposite appeared to be suitable for use as an implant material for spinal interbody fusion as a substitute for iliac bone grafts, which could eliminate the disadvantages associated with autograft harvesting . A biodegradable nanocomposite porous scaffold comprising a β-TCP matrix and HA nanofibres was developed and studied for load-bearing bone tissue engineering. HA nanofibres were prepared by a biomimetic precipitation method, the inclusion of which significantly enhanced the mechanical property of the scaffold, attaining a compressive strength of 9.87 MPa, comparable to the high-end value (2–10 MPa) of cancellous bone .
Functionally graded biocomposites
Although, in most cases, the homogeneous distribution of filler(s) inside a matrix is required , there are composites, where this is not the case. For example, functionally graded materials (commonly referred to as FGM) might be characterized by the intentional variations in composition and/or structure gradually over volume, resulting in corresponding changes in the properties of the composite. The main feature of such materials is the almost continuously graded composition that results in two different properties at the two ends of the structure. Such composites can be designed for specific function and applications. Various approaches based on the bulk (particulate processing), preform processing, layer processing, and melt processing are used to fabricate the functionally graded materials.
Bone is a biologically formed composite with variable density ranging from very dense and stiff (the cortical bone) to a soft and foamed structure (the trabecular bone). Normally the outer part of long bones consists of cortical bone with the density decreasing toward the core, where the trabecular bone is found. The trabecular bone is porous and the porosity is filled with osseous medulla [21, 22]. This brief description clearly indicates that bones are natural functionally graded composites.
A biosensor is a device for detection of an analyte that combines a biological component with a physicochemical detector component. Very briefly, it consists of three parts: a sensitive biological element; a transducer or a detector element that transforms the signal resulting from the interaction of the analyte with the biological element into another signal; and associated electronics that is primarily responsible for the display of the results in a user-friendly way .
The surface of biologically relevant calcium orthophosphates (CDHA, HA, α-TCP, β-TCP) has an excellent ability of adsorption for functional biomolecules such as proteins, albumins, DNA, and so on. Therefore, some calcium orthophosphate-based biocomposites and hybrid biomaterials were found to be applicable for biosensor manufacturing [288, 542, 851, 884]. For example, formation of poly-l-lysine/HA/carbon nanotube hybrid nanoparticles was described, and a general design strategy for an immunosensing platform was proposed based on adsorption of antibodies onto this nanocomposite . In another article, a hybrid material formed by assembling of gold nanoparticles onto nano-HA was employed for the interface design of piezoelectric immunosensor, on which the antibodies were bound. The developed sensing interface appeared to possess some advantages, such as activation-free immobilization and high antigen-binding activities of antibodies, over using either nano-HA or gold nanoparticles alone . Until now, just a few papers have been published on biosensor application of calcium orthophosphate-based biocomposites. Presumably, this subject will be further developed in the future and, perhaps, sometime implantable biosensors will be designed to perform the continuous concentration monitoring of the important biological macromolecules. Possibly, those biocencors might be able to use an electric power, generated by DCPD/polymer composite-based battery devices [413, 414].
Interaction between the phases in calcium orthophosphate-based biocomposites
An important aspect that should be addressed in details is a mutual interaction between calcium orthophosphates and other phases in biocomposites and hybrid biomaterials. In general, an interaction between the phases in any composite can be either mechanical, when it results from radial compression forces exerted by the matrix on the filler particles (e.g., developed during cooling due to thermal contraction), or chemical, when the reactivity of the filler toward the matrix has an important role. In the latter case, it is important to distinguish a physical interaction from chemical bonding . According to Wypych , physical interaction is more or less temporary, implicating hydrogen bonding or van der Waals forces, whereas chemical bonding is stronger and more permanent, involving covalent bond formation. Thus, a chemical interfacial bond between the phases is preferred to achieve a higher strength of a composite. The magnitude of the interfacial bond between the phases determines how well a weak matrix transmits stress to the strong fibers. However, while a bond between the matrix and reinforcement must exist for the purpose of stress transfer, it should not be so strong that it prevents toughening mechanisms, such as debonding and fiber pullout .
Except of FTIR spectroscopy, other measurement techniques are also able to show some evidences of a chemical interaction between calcium orthophosphates and other compounds in biocomposites [280, 382, 536, 539, 541, 911, 912, 913]. For example, for CDHA/alendronate nanocrystals such evidences were observed by thermogravimetric analysis: DTG plots of the nanocrystals appeared to be quite different from those obtained from mechanical mixtures of CDHA and calcium alendronate with similar compositions . Analogous DTG results were obtained for nano-HA/PVA . In the case of nano-HA/polyamide biocomposites, a hydrogen bonding between the phases was detected by differential scanning calorimetry technique . Another example comprises application of the dynamic mechanical analysis to investigate softening mechanism of β-TCP/PLLA biocomposites . In the case of nano-HA/PVAP composites, the indirect evidences of chemical bonding between the phases were found by X-ray diffraction and thermogravimetric analysis . A strong structural correlation between the orientation of FA crystallites and the gelatin within the FA/gelatin composite spheres was discovered that indicated to a substantial reorganization of the macromolecular matrix within the area of a growing aggregate .
By means of the X-ray photo-electronic spectroscopy (XPS) technique, binding energies of Ca, P, and O atoms were found to have some differences between nano-HA (Ca, 350.5 and 345.5; O, 530.2; P, 132.5 eV) and nano-HA/konjac glucomannan/chitosan biocomposite (Ca, 352.1 and 347.4; O, 531.2; P, 133.4 eV), respectively . Further measurements by FTIR and X-ray diffraction revealed that nano-HA was mainly linked with konjac glucomannan and chitosan by hydrogen bonding among OH− and PO43− of nano-HA and –C=O and –NH of konjac glucomannan and chitosan copolymer and there was a stable interface formed between the three phases in the biocomposite. Meanwhile, coordinate bonding might be formed between Ca2+ and –NH. Stable interfaces have been formed among the three phases in a biocomposite . In HA/collagen biocomposites, a covalent bond formation between Ca2+ of HA and RCOO− of collagen molecules was found by XPS . Similar XPS observations were also made for several other calcium orthophosphate-based biocomposites [529, 556, 565].
The interaction and adhesion between calcium orthophosphate fillers and respective matrixes have a significant effect on the properties of particulate-filled reinforced materials, being essential to transfer the load between the phases and thus improve the mechanical performance of the composites . However, for the substantial amount of the biocomposites discussed in this review, the interaction between the phases is mechanical in nature. This is because the matrix often consists of compounds with no functional groups or unsaturated bonds, which can form ionic complexes with the constituents of calcium orthophosphates. Obviously, less coupling exists between non-polar polymers and calcium orthophosphate ceramic particles. Therefore, polymers with functional groups pendant to the polymer backbone, which can act as sites for bridging to calcium orthophosphates, are more promising in this respect . Besides, the surface of calcium orthophosphates might be modified as well [116, 416, 417, 552, 914, 915]. In order to improve the situation, various supplementary reagents are applied. Namely, if the primary effect of a processing additive is to increase the interaction between the phases, such an additive can be regarded as a coupling agent . Coupling agents establish chemical bridges between the matrix and the fillers, promoting the adhesion between the phases. In many cases, their effect is not unique, influencing also the rheology of composites .
Optimization of biocomposite properties with coupling agents is currently an important area of the research. The control and development of molecular-level associations of polymer with calcium orthophosphates is suggested to be significant for the resulting mechanical responses in the composites. It appears that a fundamental molecular understanding of interfacial behavior in biocomposite systems is an area not sufficiently addressed in the literature. Various experimental characterization techniques using electron microscopy, vibrational spectroscopy, X-ray diffraction, scanning probe microscopy, and others are used routinely to characterize these materials besides mechanical property characterization. In addition, atomic scale models for simulating the phase interaction and predicting responses in the novel material systems, where nanostructure and nanointerfaces are included, are important to understand and predict the load deformation behavior .
A hexamethylene diisocyanate coupling agent was used to bind PEG/PBT (Polyactive™) block copolymers  and other polymers  to HA filler particles. Thermogravimetric and infrared analysis demonstrated that the polymers were chemically bonded to the HA particles through the isocyanate groups, making it a suitable approach to improve the adhesion . Other researchers used glutaraldehyde as a crosslinked reagent in various calcium orthophosphate-based biocomposites [388, 392, 500, 502, 503, 520, 525, 585, 621, 646, 649, 917]. The interfacial bonding between calcium orthophosphates and other components might be induced by using various coupling agents and surface modifiers, such as silanes [192, 234, 337, 540, 918, 919, 920, 921, 922, 923], zirconates [225, 337, 339, 914, 924], titanates [225, 337, 924], phosphoric acid , alkaline pretreatment [722, 725], polyacids [115, 116, 234], and other chemicals. Besides, some polymers might be grafted onto the surface of calcium orthophosphates . Structural modifications of the polymeric matrices, for instance, with the introduction of acrylic acid [195, 234, 919, 920], have also proved to be effective methods. For example, application of polyacids as a bonding agent for HA/Polyactive™ composites caused the surface-modified HA particles to maintain better contact with the polymer at fracture and improved mechanical properties [115, 116, 234]. The use of titanate and zirconate coupling agents appeared to be very dependent on the molding technique employed . Silane-coupled HA powders were tested before applying them as fillers in biodegradable composites [921, 922, 923]. This treatment allowed HA withstanding the attack of water without impairing overall bioactivity. Besides, chemically modified reinforcement phase–matrix interface was found to improve the mechanical properties of the biocomposites. Examples of such interface-modified biocomposites include chemically coupled HA/PE [919, 920], chemically formed HA/Ca poly(vinylphosphonate) , and PLA/HA fibers . These biocomposites are able to consume a large amount of energy in the fracture.
The action of some coupling agents was found to combine two distinct mechanisms: (i) crosslinking of the polymeric matrix (valid for zirconate and titanate coupling agents) and (ii) improvement of the interfacial interactions between the major phases of the composites. This interfacial adhesion improvement appeared to be much dependent on the chemical nature (pH and type of metallic center) of the coupling agents . Several studies claimed that silanes do interact with HA [192, 919, 920, 921, 922, 923]. It was shown that a silicon-containing inter-phase existed between HA and PE, which promoted the chemical adhesion between the HA particles and the polymer. A silane-coupling agent also facilitated penetration of PE into cavities of individual HA particles, which resulted in enhanced mechanical interlocking at the matrix-reinforcement interface [919, 920].
Addition of adhesion promoting agents might be an alternative to improve the interaction between the fillers and the matrix. For example, Morita et al.  used incorporation of 4-methacryloyloxyethyl trimellitate anhydride to promote adhesion of the polymer to HA. In another study, phosphoric ester was added to the liquid component of the formulation . Both the strength and the affinity index of biocomposites were found to increase, probably due to the effects of copolymerization.
Possible interactions between BCP and HPMC have been investigated in IBS composites [736, 737, 927]. After mixing, there was a decrease in the mean diameter of BCP granules and this influenced the viscosity of the paste. Dissolution of grain boundaries of β-TCP crystals and precipitation of CDHA on HA crystal surface was found during the interaction between BCP and HPMC in aqueous solutions. Both phenomena were responsible for the observed granulometric changes [736, 737]; however, within the sensitivity of the employed measurement techniques, no chemical bonding between BCP and HPMC was detected .
A coprecipitation method was used to prepare CDHA/chitosan biocomposites . Growth of CDHA crystals was inhibited by organic acids with more than two carboxyl groups, which strongly bind to CDHA surfaces via a COO–Ca bond. Transmission electron microscopy images revealed that CDHA-formed elliptic aggregates with chemical interactions (probably coordination bond) between Ca on its surface and amino groups of chitosan; the CDHA nanocrystals were found to align along the chitosan molecules, with the amino groups working as the nucleation sites . Formation of calcium crosslinked polymer carboxylate salts was suggested during the setting of calcium orthophosphate cement (TTCP + DCPA)/polyphosphazane biocomposites; the chemical involvement of the polymer in the cement setting was concluded based on the results of pH monitoring [460, 461, 462].
A chemical bond between the phases was presumed in PCL/HA composites, prepared by the grafting technique ; unfortunately, no strong experimental evidences were provided. In another study, CDHA/poly(α-hydroxyester) composites were prepared by a low-temperature chemical route . In that study, pre-composite structures were prepared by combining α-TCP with PLA, PLGA and copolymers thereof. The final biocomposite structure was achieved by in situ hydrolysis of α-TCP to CDHA performed at 56 °C either in solvent cast or pressed pre-composites. That transformation occurred without any chemical reaction between the polymer and calcium orthophosphates, as it was determined by FTIR spectroscopy .
In nearly every study on HA/carbon nanotubes biocomposites, the nanotubes have been functionalized before combining them with HA. Most researchers have done this by oxidation [242, 243, 244, 245, 246], although non-covalent functionalizing with sodium dodecylsulfate  and coating the nanotubes by a polymer  before combining them with HA have also been reported. Several studies by transmission electron microscopy have shown evidences that the functionalization has enhanced interaction between carbon nanotubes and HA [245, 246, 929].
If calcium orthophosphate-based biocomposites are able to sustain a high-temperature sintering (valid for the formulations consisting of inorganic components only), an inter-diffusion of chemical elements will take place between the phases. Such effect has been detected by energy-dispersive X-ray spectroscopy in HA/TiO2 biocomposite particles with partial formation of calcium titanates; this process was found to be favorable to enhancing the cohesive strength of particles in the composite coating . A similar high-temperature interaction between HA and zirconia [743, 768], as well as between HA and Ti [554, 840, 842, 843, 844], was also detected. Besides, partial decomposition of HA and formation of different calcium aluminates were detected in HA/Al2O3 biocomposites after sintering at 1200–1300 °C [795, 801, 802].
Bioactivity and biodegradation of calcium orthophosphate-based biocomposites
The continuous degradation of an implant causes a gradual load transfer to the healing tissue, preventing stress-shielding atrophy and stimulates the healing and remodeling of bones. Some requirements must be fulfilled by the ideal prosthetic biodegradable materials, such as biocompatibility, adequate initial strength and stiffness, retention of mechanical properties throughout sufficient time to assure its biofunctionality and non-toxicity of the degradation by-products . Generally speaking, bioactivity (i.e., ability of bonding to bones) of biologically relevant calcium orthophosphates reinforced by other materials is usually lower than that of pure calcium orthophosphates [27, 28, 930].
Biodegradability of polymers generally depends on the following factors: (1) chemical stability of the polymer backbone, (2) hydrophobicity of the monomer, (3) morphology of the polymer, (4) initial molecular weight, (5) fabrication processes, (6) geometry of the implant, (7) properties of the scaffold such as porosity and pore diameter . A summary on degradation of PLA and PGA, as well as that of starch/ethylene vinyl alcohol copolymer (SEVA) is available in literature [146, p. 798 and p. 803, respectively], where the interested readers are referred to. Biodegradation of HA/PLLA and CDHA/PLLA composite rods in subcutis and medullary cavities of rabbits were investigated mechanically and histologically; the degradation was found to be faster for the case of using uncalcinated CDHA instead of calcinated HA . In a more detailed study, new bone formation was detected at 2 weeks after implantation, especially for formulations with a high HA content . More to the point, a direct contact between bones and these composites without intervening fibrous tissue was detected in this case [934, 935]. SEVA-C and SEVA-C/HA biocomposites were found to exhibit a non-cytotoxic behavior [936, 937], inducing a satisfactory tissue response when implanted as shown by in vivo studies . Furthermore, SEVA-C/HA biocomposites induce a positive response on osteoblast-like cells to what concerns cell adhesion and proliferation .
Both in vitro (the samples were immersed into 1% trypsin/phosphate-buffered saline solution at 37 °C) and in vivo (implantation of samples into the posterolateral lumbar spine of rabbits) biodegradation have been investigated for nano-HA/collagen/PLA biocomposites . The results demonstrated that weight loss increased continuously in vitro with a reduction in mass of 19.6% after 4 weeks. During the experimental period in vitro, the relative rate of reduction of the three components in this material was shown to differ greatly: collagen decreased the fastest, from 40% by weight to 20% in the composite; HA content increased from 45 to 60%, whereas PLA changed little. In vivo, the collagen/HA ratio appeared to be slightly higher near the transverse process than in the central part of the intertransverse process . These data clearly demonstrate a biodegradation independence of various components of biocomposites.
Some challenges and critical issues
There are not enough reliable experimental and clinical data supporting the long-term performance of biocomposites with respect to monolithic traditional materials.
The design of biocomposites and hybrid biomaterials is far more complex than that of conventional monolithic materials because of the large number of additional design variables that must be considered.
The available fabrication methods may limit the possible reinforcement configurations, may be time consuming, expensive, highly skilled and may require special cleaning and sterilization processes.
There are no satisfactory standards yet for biocompatibility testing of the biocomposite implants because the ways in which the different components of any biocomposite interact to living tissues are not completely understood.
There are no adequate standards for the assessment of biocomposite fatigue performance because the fatigue behavior of such materials is far more complex and difficult to predict than that of traditional materials .
Optimizing biocomposite processing conditions.
Optimization of interfacial bonding and strength equivalent to natural bone.
Optimization of the surface properties and pore size to maximize bone growth.
Maintaining the adequate volume of the construct in vivo to allow bone formation to take place.
Withstanding the load-bearing conditions.
Matching the bioresorbability of the grafts and their biomechanical properties while forming new bone.
Understanding the molecular mechanisms by which the cells and the biocomposite matrix interact with each other in vivo to promote bone regeneration.
The aforementioned critical issues have to be solved before a widespread commercial use of calcium orthophosphate-based biocomposites and hybrid biomaterials can be made in surgery and medicine.
All types of calcified tissues of humans and mammals appear to possess a complex hierarchical composite structure. Their mechanical properties are outstanding (considering weak constituents from which they are assembled) and far beyond those, that can be achieved using the same synthetic materials with present technologies. This is because biological organisms produce biocomposites that are organized in terms of both composition and structure, containing both brittle calcium orthophosphates and ductile bioorganic components in very complex structures, hierarchically organized at the nano-, micro-, and meso-levels. Additionally, the calcified tissues are always multifunctional, e.g., bone provides structural support for the body plus blood cell formation. The third defining characteristic of biological systems, in contrast with current synthetic systems, is their self-healing ability, which is nearly universal in nature. These complex structures, which have risen from millions of years of evolution, inspire materials scientists in the design of novel biomaterials .
Until now, still no reasonable alternative exists to autogenous bone grafts in surgery. However, the studies summarized in this review have shown that the proper combination of a ductile matrix with a brittle, hard, and bioactive calcium orthophosphate filler offers many advantages for biomedical applications. Namely, the desirable properties of some components can compensate for a poor mechanical behavior of calcium orthophosphate bioceramics, while in turn the desirable bioactive properties of calcium orthophosphates improve those of other phases, thus expanding the possible application of each material within the body . However, the reviewed literature clearly indicates that among possible types of calcium orthophosphate-based biocomposites and hybrid biomaterials only simple, complex, and graded ones (see classification of the composites in the section “General information on composites and biocomposites”) have been investigated. Presumably, a future progress in this subject will require concentrating efforts on elaboration and development of hierarchical biocomposites. Furthermore, following the modern tendency of tissue engineering, a novel generation of calcium orthophosphate-based biocomposites and hybrid biomaterials should also contain a biological living part.
Much study remains to be done on a long way from a laboratory to clinics, and the success in this field depends on the effective cooperation of clinicians, chemists, biologists, bioengineers, and materials scientists.
One molecule of collagen type I is a triple helix with 338 repetitions of amino acid residues and is about 300 nm in length . Additionally, bone contains small quantities of other bioorganic materials, such as proteins, polysaccharides, and lipids, as well as bone contains cells and blood vessels.
Chitosan is a biodegradable and semicrystalline polysaccharide obtained from N-deacetylation of chitin, which is harvested from the exoskeleton of marine crustaceans.
The term biomimetic can be defined as a processing technique that either mimics or inspires the biological mechanism, in part or whole .
However, a more general topic “ceramic–plastic material as a bone substitute” is, at least, 18 years older .
However, there are some reports about a lack of TCP biodegradation after implantation in calvarial defects .
BCP is a solid composite of HA and β-TCP; however, similar composites of HA and α-TCP are possible as well .
According to Wikipedia, the free encyclopedia: “Concrete is a construction material that consists of a cement (commonly Portland cement), aggregates (generally gravel and sand) and water. It solidifies and hardens after mixing and placement due to a chemical process known as hydration. The water reacts with the cement, which bonds the other components together, eventually creating a stone-like material” .
Unfortunately, in the majority of the already published papers it often remained unclear whether “nano-HA” represented the stoichiometric nano-HA or a non-stoichiometric nano-CDHA.
The structural and biochemical properties of collagens have been widely investigated and over 25 collagen subtypes have been identified .
Alginates are a family of unbranched binary copolymers with a structure comprising 1–4 glycosidically linked β-d-mannuronic acid and its C-5 epimer α-Lguluronic acid .
I would like to express the profound gratitude to Dr. Sergey Yakovlev and Dr. Besim Ben-Nissan for their generous assistance in getting pdf-versions and/or hard copies of many unavailable for me scientific papers.
- 1.Keating JF, McQueen MM (2001) J Bone Joint Surg Br 82B:3Google Scholar
- 2.Meyer U, Joos U, Wiesmann HP (2004) Int J Oral Maxillofac Surg 33:635Google Scholar
- 3.Lane JM, Tomin E, Bostrom MPG (1999) Clin Orthop Rel Res 367S:107Google Scholar
- 4.Murugan R, Ramakrishna S (2005) In: Nalwa HS (ed) Handbook of nanostructured biomaterials and their applications in nanobiotechnology, vol 2. American Scientific Publishers, Stevenson Ranch, p 141Google Scholar
- 5.Keller EE, Triplett WW (1987) J Oral Maxillofac Surg 45:11Google Scholar
- 6.Laurie SW, Kaban LB, Mulliken JB, Murray JE (1984) Plast Reconstr Surg 73:933Google Scholar
- 7.Younger EM, Chapman MW (1989) J Orthop Trauma 3:192Google Scholar
- 8.Neumann M, Epple M (2006) Eur J Trauma 32:125Google Scholar
- 9.Le Guéhennec L, Layrolle P, Daculsi G (2004) Eur Cells Mater 8:1Google Scholar
- 10.Fuchs JR, Nasseri BA, Vacanti JP (2001) Ann Thorac Surg 72:557Google Scholar
- 11.Hench LL, Wilson J (1984) Science 226:630Google Scholar
- 12.Rose FRAJ, Oreffo ROC (2002) Biochem Biophys Res 292:1Google Scholar
- 13.Kokubo T, Kim HM, Kawashita M (2003) Biomaterials 24:2161Google Scholar
- 14.Rueger JM (1998) Orthopäde 27:72Google Scholar
- 15.Greenwald AS, Boden SD, Goldberg VM, Khan Y, Laurencin CT, Rosier RN (2001) J Bone Joint Surg Am 83:98Google Scholar
- 16.Finkemeier CG (2002) J Bone Joint Surg Am 84:454Google Scholar
- 17.Giannoudis PV, Dinopoulos H, Tsiridis E (2005) Injury 36(Suppl 3):S20Google Scholar
- 18.Yang S, Leong KF, Du Z, Chua CK (2001) Tissue Eng 7:679Google Scholar
- 19.Burg KJL, Porter S, Kellam JF (2000) Biomaterials 21:2347Google Scholar
- 20.Holy CE, Shoichet MS, Davies JE (2000) J Biomed Mater Res 51:376Google Scholar
- 21.Lowenstam HA, Weiner S (1989) On biomineralization. Oxford University Press, New YorkGoogle Scholar
- 22.Weiner S, Wagner HD (1998) Ann Rev Mater Sci 28:271Google Scholar
- 24.Hench LL, Wilson J (1993) In: Hench LL, Wilson J (eds) Advanced series in ceramics, vol 1. World Scientific, Singapore, p 1Google Scholar
- 25.Tadic D, Epple M (2004) Biomaterials 25:987Google Scholar
- 26.Suchanek W, Yoshimura M (1998) J Mater Res 13:94Google Scholar
- 27.Hench LL (1991) J Am Ceram Soc 74:1487Google Scholar
- 28.Hench LL (1998) J Am Ceram Soc 81:1705Google Scholar
- 29.Itoh S, Kikuchi M, Koyama Y, Takakuda K, Shinomiya K, Tanaka J (2002) Biomaterials 23:3919Google Scholar
- 30.Thompson JB, Kindt JH, Drake B, Hansma HG, Morse DE, Hansma PK (2001) Nature 414:773Google Scholar
- 31.Fratzl P, Gupta HS, Paschalis EP, Roschger P (2004) J Mater Chem 14:2115Google Scholar
- 32.Murugan R, Ramakrishna S (2005) Compos Sci Technol 65:2385Google Scholar
- 33.Burr DB (2002) Bone 31:8Google Scholar
- 34.Itoh S, Kikuchi M, Koyama Y, Matumoto HN, Takakuda K, Shinomiya K, Tanaka J (2005) Biomed Mater Eng 15:29Google Scholar
- 35.Cui FZ, Li Y, Ge J (2007) Mater Sci Eng R 57:1Google Scholar
- 36.Vallet-Regi M, Arcos D (2006) Curr Nanosci 2:179Google Scholar
- 37.Chan CK, Kumar TSS, Liao S, Murugan R, Ngiam M, Ramakrishna S (2006) Nanomedicine 1:177Google Scholar
- 38.Olszta MJ, Cheng XG, Jee SS, Kumar BR, Kim YY, Kaufman MJ, Douglas EP, Gower LB (2007) Mater Sci Eng R 58:77Google Scholar
- 39.Bauer T, Muschler G (2000) Clin Orthop Relat Res 371:10Google Scholar
- 40.Athanasiou KA, Zhu CF, Lanctot DR, Agrawal CM, Wang X (2000) Tissue Eng 6:361Google Scholar
- 41.Zioupos P (1998) Mater Sci Eng C 6:33Google Scholar
- 42.Doblaré M, Garcia JM, Gómez MJ (2004) Eng Fract Mech 71:1809Google Scholar
- 43.Vallet-Regi M (2006) Dalton Trans 5211Google Scholar
- 44.Huiskes R, Ruimerman R, Harry van Lenthe G, Janssen JD (2000) Nature 405:704Google Scholar
- 45.Thomson RC, Yaszemski MJ, Powers JM, Mikos AG (1998) Biomaterials 19:1935Google Scholar
- 46.Boccaccini AR, Blaker JJ (2005) Expert Rev Med Devices 2:303Google Scholar
- 47.Verheyen CCPM, de Wijn JR, van Blitterswijk CA, de Groot K, Rozing PM (1993) J Biomed Mater Res 27:433Google Scholar
- 48.Zhang RY, Ma PX (1999) J Biomed Mater Res 44:446Google Scholar
- 49.Durucan C, Brown PW (2001) Adv Eng Mater 3:227Google Scholar
- 50.Kim HW, Knowles JC, Kim HE (2004) Biomaterials 25:1279Google Scholar
- 51.Hutmacher DW, Schantz JT, Lam CXF, Tan KC, Lim TC (2007) J Tissue Eng Regen Med 1:245Google Scholar
- 52.Guarino V, Causa F, Ambrosio L (2007) Expert Rev Med Devices 4:405Google Scholar
- 54.Hench LL, Polak JM (2002) Science 295:1014Google Scholar
- 55.Crane GM, Ishaug SL, Mikos AG (1995) Nat Med 1:1322Google Scholar
- 56.LeGeros RZ (1988) Adv Dent Res 2:164Google Scholar
- 57.Mathijsen A (1852) Nieuwe Wijze van Aanwending van het Gips-Verband bij Beenbreuken. J.B. van Loghem, HaarlemGoogle Scholar
- 58.Dreesman H (1892) Beitr Klin Chir 9:804Google Scholar
- 59.Wang M (2003) Biomaterials 24:2133Google Scholar
- 60.https://doi.org/en.wikipedia.org/wiki/Composite_material. Assessed June 2008
- 61.Evans SL, Gregson PJ (1998) Biomaterials 19:1329Google Scholar
- 62.Habibovic P, Barrère F, van Blitterswijk CA, de Groot K, Layrolle P (2002) J Am Ceram Soc 85:517Google Scholar
- 63.Zhang RY, Ma PX (2004) Macromol Biosci 4:100Google Scholar
- 64.Oliveira AL, Mano JF, Reis RL (2003) Curr Opin Solid State Mater Sci 7:309Google Scholar
- 65.Wan YZ, Hong L, Jia SR, Huang Y, Zhu Y, Wang YL, Jiang HJ (2006) Compos Sci Technol 66:1825Google Scholar
- 66.Wan YZ, Huang Y, Yuan CD, Raman S, Zhu Y, Jiang HJ, He F, Gao C (2007) Mater Sci Eng C 27:855Google Scholar
- 67.Ohtsuki C, Kamitakahara M, Miyazaki T (2007) J Tissue Eng Regen Med 1:33Google Scholar
- 68.de Groot K, Geesink RGT, Klein CPAT, Serekian P (1987) J Biomed Mater Res 21:1375Google Scholar
- 69.de Groot K, Wolke JGC, Jansen JA (1998) Proc Inst Mech Eng H 212:137Google Scholar
- 70.Ignjatovic NL, Liu CZ, Czernuszka JT, Uskokovic DP (2007) Acta Biomater 3:927Google Scholar
- 71.Manso M, Langlet M, Fernandez M, Vasquez L, Martinez-Duart JM (2003) Mater Sci Eng C 23:451Google Scholar
- 72.Sun L, Berndt CC, Gross KA, Kucuk A (2001) J Biomed Mater Res Appl Biomater 58:570Google Scholar
- 73.Yoshida K, Hashimoto K, Toda Y, Udagawa S, Kanazawa T (2006) J Eur Ceram Soc 26:515Google Scholar
- 74.Planeix JM, Jaunky W, Duhoo T, Czernuszka JT, Hosseini MW, Brès EF (2003) J Mater Chem 13:2521Google Scholar
- 75.Dong J, Uemura T, Kojima H, Kikuchi M, Tanaka J, Tateishi T (2001) Mater Sci Eng C 17:37Google Scholar
- 76.Zerbo IR, Bronckers ALJJ, de Lange G, Burger EH (2005) Biomaterials 26:1445Google Scholar
- 77.Krout A, Wen HB, Hippensteel E, Li P (2005) J Biomed Mater Res A 73A:377Google Scholar
- 78.Matthews FL, Rawlings RD (2000) Composite materials: engineering and science. CRC Press LLC, Boca Raton, FL, p 480Google Scholar
- 79.Xia Z, Riester L, Curtin WA, Li H, Sheldon BW, Liang J, Chang B, Xu JM (2004) Acta Mater 52:931Google Scholar
- 80.Williams DF (1990) Encyclopedia of biomaterials. Pergamon, OxfordGoogle Scholar
- 81.Ong JL, Chan DCN (1999) Crit Rev Biomed Eng 28:667Google Scholar
- 82.Davies JE (1996) Anat Rec 245:426Google Scholar
- 83.Anselme K (2000) Biomaterials 21:667Google Scholar
- 84.Gauthier O, Bouler JM, Weiss P, Bosco J, Daculsi G, Aguado E (1999) J Biomed Mater Res 47:28Google Scholar
- 85.Hing KA, Best SM, Bonfield W (1999) J Mater Sci Mater Med 10:135Google Scholar
- 86.Carotenuto G, Spagnuolo G, Ambrosio L, Nicolais L (1999) J Mater Sci Mater Med 10:671Google Scholar
- 87.LeGeros RZ (1991) In: Myers HM (ed) Monographs in oral science, vol 15. Karger, Basel, p 201Google Scholar
- 88.Elliot JC (1994) Structure and chemistry of the apatites and other calcium orthophosphates. Studies in inorganic chemistry, vol 18. Elsevier, Amsterdam, p 389Google Scholar
- 89.Brown PW, Constantz B (eds) (1994) Hydroxyapatite and related materials. CRC Press, Boca Raton, p 343Google Scholar
- 90.Amjad Z (ed) (1997) Calcium phosphates in biological and industrial systems. Kluwer Academic Publishers, Boston, MA, p 529Google Scholar
- 91.Hughes JM, Kohn M, Rakovan J (eds) (2002) Phosphates: geochemical, geobiological and materials importance. Reviews in mineralogy and geochemistry, vol 48. Mineralogical Society of America, Washington, DCGoogle Scholar
- 92.Chow LC, Eanes ED (eds) (2001) Octacalcium phosphate. Monographs in oral science, vol 18. S. Karger AG, Basel, 168 ppGoogle Scholar
- 93.Brès E, Hardouin P (eds) (1998) Les matériaux en phosphate de calcium. Aspects fondamentaux/calcium phosphate materials. Fundamentals. Sauramps Medical, Montpellier, p 176Google Scholar
- 94.Rea SM, Bonfield W (2004) J Aust Ceram Soc 40:43Google Scholar
- 95.Langer R (2000) Acc Chem Res 33:94Google Scholar
- 96.Thomson RC, Ak S, Yaszemski MJ, Mikos AG (2000) Principles of tissue engineering. Academic Press, NY, p 251Google Scholar
- 97.Ramakrishna S, Mayer J, Wintermantel E, Leong KW (2001) Compos Sci Technol 61:1189Google Scholar
- 98.Langer R, Vacanti JP (1993) Science 260:920Google Scholar
- 99.Lanza RP, Hayes JL, Chick WL (1996) Nat Biotechnol 14:1107Google Scholar
- 100.Agrawal CM, Ray RB (2001) J Biomed Mater Res 55:141Google Scholar
- 101.Kweon H, Yoo M, Park I, Kim T, Lee H, Lee S, Oh J, Akaike T, Cho C (2003) Biomaterials 24:801Google Scholar
- 102.de Groot JH, de Vrijer R, Pennings AJ, Klompmaker J, Veth RPH, Jansen HWB (1996) Biomaterials 17:163Google Scholar
- 103.Resiak I, Rokicki G (2000) Polimery 45:592Google Scholar
- 104.Temenoff JS, Mikos AG (2000) Biomaterials 21:2405Google Scholar
- 105.Behravesh E, Yasko AW, Engel PS, Mikos AG (1999) Clin Orthop Relat Res 367S:S118Google Scholar
- 106.Lewandrowski KU, Gresser JD, Wise DL, White RL, Trantolo DJ (2000) Biomaterials 21:293Google Scholar
- 107.Peter SJ, Miller MJ, Yaszemski MJ, Mikos AG (1997) In: Domb AJ, Kost J, Wiseman DM (eds) Handbook of biodegradable polymers. Harwood Academic, Amsterdam, p 87Google Scholar
- 108.Boland ED, Coleman BD, Barnes CP, Simpson DG, Wnek GE, Bowlin GL (2005) Acta Biomater 1:115Google Scholar
- 109.Gilbert JL (2001) Encyclopedia of materials: science and technology. Elsevier, Amsterdam, p 11Google Scholar
- 110.Li YW, Leong JCY, Lu WW, Luk KDK, Cheung KMC, Chiu KY, Chow SP (2000) J Biomed Mater Res 52:164Google Scholar
- 111.Mckellop H, Shen F, Lu B, Campbell P, Salovey R (1999) J Orthop Res 17:157Google Scholar
- 112.Kurtz SM, Muratoglu OK, Evans M, Edidin AA (1999) Biomaterials 20:1659Google Scholar
- 113.Laurencin CT, Ambrosio MA, Borden MD, Cooper JA Jr (1999) Ann Rev Biomed Eng 1:19Google Scholar
- 114.Jansen JA, de Ruijter JE, Janssen PT, Paquay YG (1995) Biomaterials 16:819Google Scholar
- 115.Liu Q, de Wijn JR, Bakker D, van Blitterswijk CA (1996) J Mater Sci Mater Med 7:551Google Scholar
- 116.Liu Q, de Wijn JR, Bakker D, van Toledo M, van Blitterswijk CA (1998) J Mater Sci Mater Med 9:23Google Scholar
- 117.Meijer GJ, Cune MS, van Dooren M, de Putter C, van Blitterswijk CA (1997) J Oral Rehabil 24:85Google Scholar
- 118.Meijer GJ, Dalmeijer RA, de Putter C, van Blitterswijk CA (1997) J Oral Rehabil 24:93Google Scholar
- 119.Svensson A, Nicklasson E, Harrah T, Panilaitis B, Kaplan DL, Brittberg M, Gatenholm P (2005) Biomaterials 26:419Google Scholar
- 121.Thomas V, Dean DR, Vohra YK (2006) Curr Nanosci 2:155Google Scholar
- 122.Li SM, Garreau H, Vert M (1990) J Mater Sci Mater Med 1:123Google Scholar
- 123.Daniels AU, Adriano KP, Smuts WP, Chang MKO, Keller J (1994) J Appl Biomater 5:51Google Scholar
- 124.Adriano KP, Pohjonen T, Törmällä P (1994) J Appl Biomater 5:133Google Scholar
- 125.Athanasiou KA, Niederauer GG, Agrawal CM (1996) Biomaterials 17:93Google Scholar
- 126.Dee KC, Bizios R (1996) Biotechnol Bioeng 50:438Google Scholar
- 127.Ignjatovic N, Tomic S, Dakic M, Miljkovic M, Plavsic M, Uskokovic D (1999) Biomaterials 20:809Google Scholar
- 128.Ignjatovic N, Savic V, Najman S, Plavsic M, Uskokovic D (2001) Biomaterials 22:571Google Scholar
- 129.Marra KG, Szem JW, Kumta PN, DiMilla PA, Weiss LE (1999) J Biomed Mater Res 47:324Google Scholar
- 130.Ashammakhi N, Rokkanen P (1997) Biomaterials 18:3Google Scholar
- 131.Boyan B, Lohmann C, Somers A, Neiderauer G, Wozney J, Dean D, Carnes D, Schwartz Z (1999) J Biomed Mater Res 46:51Google Scholar
- 132.Hofmann GO (1995) Arch Orthop Trauma Surg 114:123Google Scholar
- 133.Hollinger JO, Leong K (1996) Biomaterials 17:187Google Scholar
- 134.Griffith LG (2000) Acta Mater 48:263Google Scholar
- 135.Peter SJ, Miller MJ, Yasko AW, Yaszemski MJ, Mikos AG (1998) J Biomed Mater Res 43:422Google Scholar
- 136.Ishuang SL, Payne RG, Yaszemski MJ, Aufdemorte TB, Bizios R, Mikos AG (1996) Biotechnol Bioeng 50:443Google Scholar
- 137.Shikinami Y, Okuno M (1999) Biomaterials 20:859Google Scholar
- 138.Khor E, Lim LY (2003) Biomaterials 24:2339Google Scholar
- 139.Ishihara M, Nakanishi K, Ono K, Sato M, Kikuchi M (2002) Biomaterials 23:833Google Scholar
- 140.Di Martino A, Sittinger M, Risbud MV (2005) Biomaterials 26:5983Google Scholar
- 141.Piskin E, Bölgen N, Egri S, Isoglu IA (2007) Nanomedicine 2:441Google Scholar
- 142.Rezwana K, Chena QZ, Blakera JJ, Boccaccini AR (2006) Biomaterials 27:3413Google Scholar
- 143.Mohanty AK, Misra M, Hinrichsen G (2000) Macromol Mater Eng 276(277):1Google Scholar
- 144.Seal BL, Otero TC, Panitch A (2001) Mater Sci Eng R 34:147Google Scholar
- 145.An YH, Woolf SK, Friedman RJ (2000) Biomaterials 21:2635Google Scholar
- 146.Mano JF, Sousa RA, Boesel LF, Neves NM, Reis RL (2004) Compos Sci Technol 64:789Google Scholar
- 147.Katti KS (2004) Colloids Surf B Biointerfaces 39:133Google Scholar
- 148.Hayashi T (1994) Prog Polym Sci 19:663Google Scholar
- 149.Middleton J, Tipton A (2000) Biomaterials 21:2335Google Scholar
- 150.Ma PX (2008) Adv Drug Deliv Rev 60:184Google Scholar
- 151.Coombes AG, Meikle MC (2004) Clin Mater 17:35Google Scholar
- 152.Okada M (2002) Prog Polym Sci 27:87Google Scholar
- 153.Jordan J, Jacob KI, Tannenbaum R, Sharaf MA, Jasiuk I (2005) Mater Sci Eng A 393:1Google Scholar
- 154.Matsuno H, Yokoyama A, Watari F, Uo M, Kawasaki T (2001) Biomaterials 22:1253Google Scholar
- 155.Uo M, Watari F, Yokoyama A, Matsuno H, Kawasaki T (1999) Biomaterials 20:747Google Scholar
- 156.Uo M, Watari F, Yokoyama A, Matsuno H, Kawasaki T (2001) Biomaterials 22:1787Google Scholar
- 157.Uo M, Watari F, Yokoyama A, Matsuno H, Kawasaki T (2001) Biomaterials 21:677Google Scholar
- 158.Ryan G, Pandit A, Apatsidis DP (2006) Biomaterials 27:2651Google Scholar
- 159.Shimko DA, Shimko VF, Sander EA, Dickson KF, Nauman EA (2005) J Biomed Mater Res B Appl Biomater 73B:315Google Scholar
- 160.Wen CE, Yamada Y, Shimojima K, Chino Y, Hosokawa H, Mabuchi M (2004) Mater Lett 58:357Google Scholar
- 161.Green D, Walsh D, Mann S, Oreffo ROC (2002) Bone 30:810Google Scholar
- 162.Kokubo T (1998) Acta Mater 46:2519Google Scholar
- 163.Witte F, Reifenrath J, Müller PP, Crostack HA, Nellesen J, Bach FW, Bormann D, Rudert M (2006) Matwiss u Werkstofflech 37:504Google Scholar
- 164.Uo M, Mizuno M, Kuboki Y, Makishima A, Watari F (1998) Biomaterials 19:2277Google Scholar
- 165.Imai T, Watari F, Yamagata S, Kobayashi M, Nagayama K, Nakamura S (1998) Biomaterial 19:2195Google Scholar
- 167.Hench LL (2006) J Mater Sci Mater Med 17:967Google Scholar
- 168.Cao W, Hench LL (1996) Ceram Int 22:493Google Scholar
- 169.Vogel M, Voigt C, Gross U, Müller-Mai C (2001) Biomaterials 22:357Google Scholar
- 170.de Aza P, Luklinska Z, Santos C, Guitian F, de Aza S (2003) Biomaterials 24:1437Google Scholar
- 171.Ikeda N, Kawanabe K, Nakamura T (1999) Biomaterials 20:1087Google Scholar
- 172.Weizhong Y, Dali Z, Guangfu Y (2003) J Biomed Eng 20:541Google Scholar
- 173.Piconi C, Maccauro G (1999) Biomaterials 20:1Google Scholar
- 174.Christel P, Meunier A, Heller M, Torre JP, Peille CN (1989) J Biomed Mater Res 23:45Google Scholar
- 176.Burger W, Richter HG, Piconi C, Vatteroni R, Cittadini A, Bocccalari M (1997) J Mater Sci Mater Med 8:113Google Scholar
- 177.Converse GL, Yue W, Roeder RK (2007) Biomaterials 28:927Google Scholar
- 178.Yue W, Roeder RK (2006) J Mater Res 21:2136Google Scholar
- 179.Converse GL, Roeder RK (2005) Mater Res Soc Symp Proc 898:44Google Scholar
- 180.Mizutani Y, Hattori M, Okuyama M, Kasuga T, Nogami M (2006) Key Eng Mater 309–311:1079Google Scholar
- 181.Watanabe T, Ban S, Ito T, Tsuruta S, Kawai T, Nakamura H (2004) Dent Mater J 23:609Google Scholar
- 182.Li H, Chen Y, Xie Y (2003) Mater Lett 57:2848Google Scholar
- 183.Peng Q, Weng J, Li X, Gu Z (2005) Key Eng Mater 288–289:199Google Scholar
- 184.Kasuga T, Ota Y, Nogami M, Abe Y (2000) Biomaterials 22:19Google Scholar
- 185.Smith L (1963) Arch Surg 87:653Google Scholar
- 186.Bonfield W, Grynpas MD, Tully AE, Bowman J, Abram J (1981) Biomaterials 2:185Google Scholar
- 187.Bonfield W, Bowman J, Grynpas MD (1981) UK patent 8032647Google Scholar
- 188.Bonfield W (1988) J Biomed Eng 10:522Google Scholar
- 189.Wang M, Porter D, Bonfield W (1994) Br Ceram Trans 93:91Google Scholar
- 190.Guild FJ, Bonfield W (1993) Biomaterials 14:985Google Scholar
- 191.Huang J, Di Silvio L, Wang M, Tanner KE, Bonfield W (1997) J Mater Sci Mater Med 8:775Google Scholar
- 192.Deb S, Wang M, Tanner KE, Bonfield W (1996) J Mater Sci Mater Med 7:191Google Scholar
- 193.Wang M, Joseph R, Bonfield W (1998) Biomaterials 19:2357Google Scholar
- 194.Suwanprateeb J, Tanner KE, Turner S, Bonfield W (1997) J Mater Sci Mater Med 8:469Google Scholar
- 195.Ladizesky NH, Ward IM, Bonfield W (1997) J Appl Polym Sci 65:1865Google Scholar
- 196.Ladizesky NH, Pirhonen EM, Appleyard DB, Ward IM, Bonfield W (1998) Compos Sci Technol 58:419Google Scholar
- 197.Nazhat SN, Joseph R, Wang M, Smith R, Tanner KE, Bonfield W (2000) J Mater Sci Mater Med 11:621Google Scholar
- 198.Ladizesky ΝH, Ward IM, Bonfield W (1996) Polym Adv Technol 8:496Google Scholar
- 199.Guild FJ, Bonfield W (1998) J Mater Sci Mater Med 9:497Google Scholar
- 200.Di Silvio L, Dalby M, Bonfield W (1998) J Mater Sci Mater Med 9:845Google Scholar
- 202.That PT, Tanner KE, Bonfield W (2000) J Biomed Mater Res 51:453Google Scholar
- 203.That PT, Tanner KE, Bonfield W (2000) J Biomed Mater Res 51:461Google Scholar
- 204.Bonner M, Ward IM, McGregor W, Tanner KE, Bonfield W (2001) J Mater Sci Lett 20:2049Google Scholar
- 206.Dalby MJ, Di Silvio L, Davies GW, Bonfield W (2000) J Mater Sci Mater Med 12:805Google Scholar
- 207.Di Silvio L, Dalby MJ, Bonfield W (2002) Biomaterials 23:101Google Scholar
- 208.Dalby MJ, Kayser MV, Bonfield W, Di Silvio L (2002) Biomaterials 23:681Google Scholar
- 209.Dalby MJ, Di Silvio L, Gurav N, Annaz B, Kayser MV, Bonfield W (2002) Tissue Eng 8:453Google Scholar
- 210.Zhang Y, Tanner KE, Gurav N, Di Silvio L (2007) J Biomed Mater Res A 81A:409Google Scholar
- 211.Rea SM, Best SM, Bonfield W (2004) J Mater Sci Mater Med 15:997Google Scholar
- 212.Rea SM, Brooks RA, Schneider A, Best SM, Bonfield W (2004) J Biomed Mater Res B Appl Biomater 70:250Google Scholar
- 213.Salernitano E, Migliaresi C (2003) J Appl Biomater Biomech 1:3Google Scholar
- 215.Sousa RA, Reis RL, Cunha AM, Bevis MJ (2003) Compos Sci Technol 63:389Google Scholar
- 216.Homaeigohar SS, Shokrgozar MA, Khavandi A, Sadi AY (2008) J Biomed Mater Res A 84A:491Google Scholar
- 217.Downes RN, Vardy S, Tanner KE, Bonfield W (1991) Bioceramics 4:239Google Scholar
- 218.Dornhoffer HL (1998) Laryngoscope 108:531Google Scholar
- 219.Swain RE, Wang M, Beale B, Bonfield W (1999) Biomed Eng Appl Basis Commun 11:315Google Scholar
- 220.Yi Z, Li Y, Jidong L, Xiang Z, Hongbing L, Yuanyuan W, Weihu Y (2007) Mater Sci Eng A 452–453:512Google Scholar
- 222.Fang LM, Leng Y, Gao P (2006) Biomaterials 27:3701Google Scholar
- 223.Fang LM, Gao P, Leng Y (2007) Composites B 38:345Google Scholar
- 224.Fang LM, Leng Y, Gao P (2005) Biomaterials 26:3471Google Scholar
- 225.Sousa RA, Reis RL, Cunha AM, Bevis MJ (2002) J Appl Polym Sci 86:2873Google Scholar
- 226.Reis RL, Cunha AM, Oliveira MJ, Campos AR, Bevis MJ (2001) Mat Res Innovat 4:263Google Scholar
- 227.Donners JJJM, Nolte RJM, Sommerdijk NAJM (2003) Adv Mater 15:313Google Scholar
- 228.Ignjatovic NL, Plavsic M, Miljkovic MS, Zivkovic LM, Uskokovic DP (1999) J Microsc (Oxford) 196:243Google Scholar
- 229.Skrtic D, Antonucci JM, Eanes ED (2003) J Res Natl Inst Stand Technol 108:167Google Scholar
- 230.Rizzi SC, Heath DJ, Coombes AGA, Bock N, Textor M, Downes S (2001) J Biomed Mater Res 55:475Google Scholar
- 232.Damien CJ, Parsons JR (1991) J Appl Biomater 2:187Google Scholar
- 233.Zhang RY, Ma PX (1999) J Biomed Mater Res 45:285Google Scholar
- 234.Liu Q, de Wijn JR, van Blitterswijk CA (1998) J Biomed Mater Res 40:490Google Scholar
- 235.Cerrai P, Guerra GD, Tricoli M, Krajewski A, Ravaglioli A, Martinetti R, Dolcini L, Fini M, Scarano A, Piattelli A (1999) J Mater Sci Mater Med 10:677Google Scholar
- 236.Roeder RK, Sproul MM, Turner CH (2003) J Biomed Mater Res A 67A:801Google Scholar
- 237.Hutmacher DW (2000) Biomaterials 21:2529Google Scholar
- 238.Mathieu LM, Bourban PE, Manson JAE (2006) Compos Sci Technol 66:1606Google Scholar
- 239.Redepenning J, Venkataraman G, Chen J, Stafford N (2003) J Biomed Mater Res A 66A:411Google Scholar
- 240.Rhee SH, Tanaka J (2001) J Am Ceram Soc 84:459Google Scholar
- 241.Pezzotti G, Asmus SMF (2001) Mater Sci Eng A 316:231Google Scholar
- 242.Kealley C, Ben-Nissan B, van Riessen A, Elcombe M (2006) Key Eng Mater 309–311:597Google Scholar
- 243.Kealley C, Elcombe M, van Riessen A, Ben-Nissan B (2006) Physica B 385–386:496Google Scholar
- 244.Aryal S, Bahadur KCR, Dharmaraj N, Kim KW, Kim HY (2006) Scr Mater 54:131Google Scholar
- 245.Wei Q, Yang XP, Chen GQ, Tang JT, Deng XL (2005) N Carbon Mater 20:164Google Scholar
- 246.Zhao LP, Gao L (2004) Carbon 42:423Google Scholar
- 247.Aryal S, Bhattarai SR, Bahadur KCR, Khil MS, Lee DR, Kim HY (2006) Mater Sci Eng A 426:202Google Scholar
- 248.Rautaray D, Mandal S, Sastry M (2005) Langmuir 21:5185Google Scholar
- 249.Memoto R, Nakamura S, Isobe T, Senna M (2001) J Sol Gel Sci Technol 21:7Google Scholar
- 250.Fujiwara M, Shiokawa K, Morigaki K, Tatsu Y, Nakahara Y (2008) Mater Sci Eng C 28:280Google Scholar
- 251.Nagata F, Miyajima T, Yokogawa Y (2006) J Eur Ceram Soc 26:533Google Scholar
- 254.Kim HW, Knowles JC, Kim HE (2005) J Biomed Mater Res A 72A:136Google Scholar
- 255.Sinha A, Das G, Sharma BK, Roy RP, Pramanick AK, Nayar S (2007) Mater Sci Eng C 27:70Google Scholar
- 256.Sun L, Berndt CC, Gross KA (2002) J Biomater Sci Polym Edn 13:977Google Scholar
- 257.Sugawara A, Yamane S, Akiyoshi K (2006) Macromol Rapid Commun 27:441Google Scholar
- 258.Liu Q, de Wijn JR, van Blitterswijk CA (1997) Biomaterials 18:1263Google Scholar
- 259.Uskokovic PS, Tang CY, Tsui CP, Ignjatovic N, Uskokovic DP (2007) J Eur Ceram Soc 27:1559Google Scholar
- 261.Woo KM, Seo J, Zhang RY, Ma PX (2007) Biomaterials 28:2622Google Scholar
- 262.Ma PX, Zhang R, Xiao G, Franceschi R (2001) J Biomed Mater Res 54:284Google Scholar
- 263.Wang M, Chen LJ, Ni J, Weng J, Yue CY (2001) J Mater Sci Mater Med 12:855Google Scholar
- 264.Baji A, Wong SC, Srivatsan TS, Njus GO, Mathur G (2006) Mater Manuf Process 21:211Google Scholar
- 265.Wei G, Ma PX (2006) J Biomed Mater Res A 78A:306Google Scholar
- 266.Guan L, Davies JE (2004) J Biomed Mater Res A 71A:480Google Scholar
- 267.Teng XR, Ren J, Gu SY (2007) J Biomed Mater Res B Appl Biomater 81B:185Google Scholar
- 268.Ren J, Zhao P, Ren T, Gu S, Pan K (2008) J Mater Sci Mater Med 19:1075Google Scholar
- 269.Wang M, Yue CY, Chua B (2001) J Mater Sci Mater Med 12:821Google Scholar
- 270.Chlopek J, Rosol P, Morawska-Chochol A (2006) Compos Sci Technol 66:1615Google Scholar
- 271.Szaraniec B, Rosol P, Chlopek J (2005) e-Polymers 030:1Google Scholar
- 272.Nayar S, Sinha A (2004) Colloids Surf B Biointerfaces 35:29Google Scholar
- 275.You C, Miyazaki T, Ishida E, Ashizuka M, Ohtsuki C, Tanihara M (2007) J Eur Ceram Soc 27:1585Google Scholar
- 276.Xu F, Li Y, Yao X, Liao H, Zhang L (2007) J Mater Sci Mater Med 18:635Google Scholar
- 277.Xu F, Li Y, Deng Y, Xiong G (2008) J Biomater Sci Polym Edn 19:431Google Scholar
- 278.Nayar S, Pramanick AK, Sharma BK, Das G, Kumar BR, Sinha A (2008) J Mater Sci Mater Med 19:301Google Scholar
- 279.Bigi A, Boanini E, Gazzano M, Rubini K (2005) Cryst Res Technol 40:1094Google Scholar
- 280.Pramanik N, Biswas SK, Pramanik P (2008) Int J Appl Ceram Technol 5:20Google Scholar
- 281.Bertoni E, Bigi A, Falini G, Panzavolta S, Roveri N (1999) J Mater Chem 9:779Google Scholar
- 282.Qiu HJ, Yang J, Kodali P, Koh J, Ameer GA (2006) Biomaterials 27:5845Google Scholar
- 283.Greish YE, Brown PW (2001) Biomaterials 22:807Google Scholar
- 284.Greish YE, Brown PW (2001) J Mater Sci Mater Med 12:407Google Scholar
- 285.Greish YE, Brown PW (2002) J Am Ceram Soc 85:1738Google Scholar
- 288.Zhang H, Xu JJ, Chen HY (2007) J Phys Chem C 111:16564Google Scholar
- 289.Piticescu RM, Chitanu GC, Albulescu M, Giurginca M, Popescu ML, Łojkowski W (2005) Solid State Phenom 106:47Google Scholar
- 290.Enlow D, Rawal A, Kanapathipillai M, Schmidt-Rohr K, Mallapragada S, Lo CT, Thiyagarajan P, Akin M (2007) J Mater Chem 17:1570Google Scholar
- 291.Kaito T, Myoui A, Takaoka K, Saito N, Nishikawa M, Tamai N, Ohgushi H, Yoshikawa H (2005) Biomaterials 26:73Google Scholar
- 292.Song J, Saiz E, Bertozzi CR (2003) J Am Chem Soc 125:1236Google Scholar
- 293.Meenan BJ, McClorey C, Akay M (2000) J Mater Sci Mater Med 11:481Google Scholar
- 294.Fan JP, Tsui CP, Tang CY, Chow CL (2004) Biomaterials 25:5363Google Scholar
- 295.Abu Bakar MS, Cheng MHW, Tang SM, Yu SC, Liao K, Tan CT, Khor KA, Cheang P (2003) Biomaterials 24:2245Google Scholar
- 296.Abu Bakar MS, Cheang P, Khor KA (2003) Compos Sci Technol 63:421Google Scholar
- 297.Abu Bakar MS, Cheang P, Khor KA (2003) Mater Sci Eng A 345:55Google Scholar
- 298.Fan JP, Tsui CP, Tang CY (2004) Mater Sci Eng A 382:341Google Scholar
- 299.Yu S, Hariram KP, Kumar R, Cheang P, Aik KK (2005) Biomaterials 26:2343Google Scholar
- 300.Gong XH, Tang CY, Hu HC, Zhou XP (2004) J Mater Sci Mater Med 15:1141Google Scholar
- 301.Laurencin CT, Attawia MA, Elgendy HE, Herbert KM (1996) Bone 91:S93Google Scholar
- 302.Laurencin CT, Attawia MA, Lu LQ, Borden MD, Lu HH, Gorum WJ, Lieberman JR (2001) Biomaterials 22:1271Google Scholar
- 303.Kim SS, Ahn KM, Park MS, Lee JH, Choi CY, Kim BS (2007) J Biomed Mater Res A 80A:206Google Scholar
- 304.Oliveira J, Miyazaki T, Lopes M, Ohtsuki C, Santos J (2005) J Mater Sci Mater Med 16:253Google Scholar
- 305.Kim S, Kim SS, Lee SH, Ahn SE, Gwak SJ, Song JH, Kim BS, Chung HM (2008) Biomaterials 29:1043Google Scholar
- 306.Petricca SE, Marra KG, Kumta PN (2006) Acta Biomater 2:277Google Scholar
- 307.Sato M, Slamovich EB, Webster TJ (2005) Biomaterials 26:1349Google Scholar
- 308.Gu SY, Zhan H, Ren J, Zhou XY (2007) Polym Polym Compos 15:137Google Scholar
- 309.Verheyen CCPM, de Wijin JR, van Blitterwijk CA, de Groot K (1992) J Biomed Mater Res 26:1277Google Scholar
- 310.Balac I, Uskokovic PS, Aleksic R, Uskokovic D (2002) J Biomed Mater Res 63:793Google Scholar
- 311.Dawes E, Rushton N (1994) Clin Mater 17:157Google Scholar
- 312.Verheyen CCPM, Klein CPAT, de Blieck-Hogervorst JMA, Wolke JGC, de Wijn JR, van Blitterswijk CA, de Groot K (1993) J Mater Sci Mater Med 4:58Google Scholar
- 313.Li H, Chang J (2005) Compos Sci Technol 65:2226Google Scholar
- 314.Agrawal CM, Athanasiou KA (1997) J Biomed Mater Res Appl Mater 38:105Google Scholar
- 315.Peter SJ, Miller ST, Zhu G, Yasko AW, Mikos AG (1998) J Biomed Mater Res 41:1Google Scholar
- 316.Ara M, Watanabe M, Imai Y (2002) Biomaterials 23:2479Google Scholar
- 317.Linhart W, Peters F, Lehmann W, Schwarz K, Schilling A, Amling M, Rueger JM, Epple M (2001) J Biomed Mater Res 54:162Google Scholar
- 318.Schiller C, Epple M (2003) Biomaterials 24:2037Google Scholar
- 319.Schiller C, Rasche C, Wehmöller M, Beckmann F, Eufinger H, Epple M, Weihe S (2004) Biomaterials 25:1239Google Scholar
- 320.Shikinami Y, Okuno M (2001) Biomaterials 22:3197Google Scholar
- 321.Russias J, Saiz E, Nalla RK, Gryn K, Ritchie RO, Tomsia AP (2006) Mater Sci Eng C 26:1289Google Scholar
- 322.Kim HW, Lee HH, Knowles JC (2006) J Biomed Mater Res A 79A:643Google Scholar
- 323.Gross KA, Rodríguez-Lorenzo LM (2004) Biomaterials 25:4955Google Scholar
- 324.Durucan C, Brown PW (2000) J Biomed Mater Res 51:717Google Scholar
- 325.Durucan C, Brown PW (2000) J Biomed Mater Res 51:726Google Scholar
- 326.Ignjatovic N, Suljovrujic E, Biudinski-Simendic J, Krakovsky I, Uskokovic D (2004) J Biomed Mater Res B Appl Biomater 71B:284Google Scholar
- 327.Nazhat SN, Kellomäki M, Törmälä P, Tanner KE, Bonfield W (2001) J Biomed Mater Res 58:335Google Scholar
- 328.Hasegawa S, Tamura J, Neo M, Goto K, Shikinami Y, Saito M, Kita M, Nakamura T (2005) J Biomed Mater Res A 75A:567Google Scholar
- 329.Hasegawa S, Neo M, Tamura J, Fujibayashi S, Takemoto M, Shikinami Y, Okazaki K, Nakamura T (2007) J Biomed Mater Res A 81A:930Google Scholar
- 330.Higashi S, Yamamuro T, Nakamura T, Ikada Y, Hyon SH, Jamshidi K (1986) Biomaterials 7:183Google Scholar
- 331.Ylinen P (1994) J Mater Sci Mater Med 5:522Google Scholar
- 332.Reis RL, Cunha AM, Bevis MJ (1998) J Appl Med Polym 2:49Google Scholar
- 333.Reis RL, Cunha AM (2000) J Appl Med Polym 4:1Google Scholar
- 334.Sousa RA, Mano JF, Reis RL, Cunha AM, Bevis MJ (2002) Polym Eng Sci 42:1032Google Scholar
- 335.Marques AP, Reis RL (2005) Mater Sci Eng C 25:215Google Scholar
- 336.Reis RL, Cunha AM, Allan PS, Bevis MJ (1997) J Polym Adv Tech 16:263Google Scholar
- 337.Vaz CM, Reis RL, Cunha AM (2002) Biomaterials 23:629Google Scholar
- 338.Leonor IB, Ito A, Onuma K, Kanzaki N, Reis RL (2003) Biomaterials 24:579Google Scholar
- 339.Vaz CM, Reis RL, Cunha AM (2001) Mater Res Innovat 4:375Google Scholar
- 340.Boeree N, Dove J, Cooper JJ, Knowles JC, Hastings GW (1993) Biomaterials 14:793Google Scholar
- 341.Doyle C, Tanner ET, Bonfield W (1991) Biomaterials 12:841Google Scholar
- 342.Chen LJ, Wang M (2002) Biomaterials 23:2631Google Scholar
- 343.Ni J, Wang M (2002) Mater Sci Eng C 20:101Google Scholar
- 344.Knowles JC, Hastings GW, Ohta H, Niwa S, Boeree N (1992) Biomaterials 13:491Google Scholar
- 345.Luklinska ZB, Bonfield W (1997) J Mater Sci Mater Med 8:379Google Scholar
- 346.Chen DZ, Tang CY, Chan KC, Tsui CP, Yu PHF, Leung MCP, Uskokovic PS (2007) Compos Sci Technol 67:1617Google Scholar
- 347.Rai B, Noohom W, Kithva PH, Grøndahl L, Trau M (2008) Chem Mater 20:2802Google Scholar
- 348.Wang YW, Wu Q, Chen J, Chen GQ (2005) Biomaterials 26:899Google Scholar
- 350.Azevedo M, Reis RL, Claase M, Grijpma D, Feijen J (2003) J Mater Sci Mater Med 14:103Google Scholar
- 351.Choi D, Marra KG, Kumta PN (2004) Mater Res Bull 39:417Google Scholar
- 352.Hao J, Yuan M, Deng X (2003) J Appl Polym Sci 86:676Google Scholar
- 353.Walsh D, Furuzono T, Tanaka J (2001) Biomaterials 22:1205Google Scholar
- 354.Cerrai P, Guerra GD, Tricoli M, Krajewski A, Guicciardi S, Ravaglioli A, Maltinti S, Masetti G (1999) J Mater Sci Mater Med 10:283Google Scholar
- 355.Kim HW (2007) J Biomed Mater Res A 83A:169Google Scholar
- 356.Kim HW, Knowles JC, Kim HE (2004) J Biomed Mater Res A 70A:240Google Scholar
- 357.Guerra GD, Cerrai P, Tricoli M, Krajewski A, Ravaglioli A, Mazzocchi M, Barbani N (2006) J Mater Sci Mater Med 17:69Google Scholar
- 358.Causa F, Netti PA, Ambrosio L, Ciapetti G, Baldini N, Pagani S, Martini D, Giunti A (2006) J Biomed Mater Res A 76A:151Google Scholar
- 359.Thomas V, Jagani S, Johnson K, Jose MV, Dean DR, Vohra YK, Nyairo E (2006) J Nanosci Nanotechol 6:487Google Scholar
- 360.Dunn A, Campbell P, Marra KG (2001) J Mater Sci Mater Med 12:673Google Scholar
- 361.Calandrelli L, Immirzi B, Malinconico M, Volpe M, Oliva A, Ragione F (2000) Polymer 41:8027Google Scholar
- 362.Chen B, Sun K (2005) Polym Test 24:64Google Scholar
- 363.Ural E, Kesenci K, Fambri L, Migliaresi C, Piskin E (2000) Biomaterials 21:2147Google Scholar
- 364.Yoon BH, Kim HW, Lee SH, Bae CJ, Koh YH, Kong YM, Kim HE (2005) Biomaterials 26:2957Google Scholar
- 365.Kim HW, Lee EJ, Kim HE, Salih V, Knowles JC (2005) Biomaterials 26:4395Google Scholar
- 366.Busch S, Dolhaine H, DuChesne A, Heinz S, Hochrein O, Laeri F, Podebrad O, Vietze U, Weiland T, Kniep R (1999) Eur J Inorg Chem 1643Google Scholar
- 367.Busch S, Schwarz U, Kniep R (2003) Adv Funct Mater 13:189Google Scholar
- 368.Simon P, Carrillo-Cabrera W, Formanek P, Göbel C, Geiger D, Ramlau R, Tlatlik H, Buder J, Kniep R (2004) J Mater Chem 14:2218Google Scholar
- 369.Göbel C, Simon P, Buder J, Tlatlik H, Kniep R (2004) J Mater Chem 14:2225Google Scholar
- 370.Simon P, Schwarz U, Kniep R (2005) J Mater Chem 15:4992Google Scholar
- 371.Tlatlik H, Simon P, Kawska A, Zahn D, Kniep R (2006) Angew Chem Int Ed Engl 45:1905Google Scholar
- 372.Simon P, Zahn D, Lichte H, Kniep R (2006) Chem Int Ed Engl 45:1911Google Scholar
- 373.Kniep R, Simon P (2007) In: Naka K (ed) Crystallization and self-organization process. Topics in current chemistry, vol 270. Springer, Berlin, p 73Google Scholar
- 374.Kniep R, Simon P (2008) Angew Chem Int Ed Engl 47:1405Google Scholar
- 375.Handschel J, Wiesmann HP, Stratmann U, Kleinheinz J, Meyer U, Joos U (2002) Biomaterials 23:1689Google Scholar
- 376.Kikuchi M, Tanaka J, Koyama Y, Takakuda K (1999) J Biomed Mater Res 48:108Google Scholar
- 377.Yaszemski MJ, Payne RG, Hayes WC, Langer R, Mikos AG (1996) Biomaterials 17:2117Google Scholar
- 378.Wang M, Wang J, Ni J (2000) Biomechanics 192:741Google Scholar
- 379.Kikuchi M, Koyama Y, Takakuda K, Miyairi H, Shirahama N, Tanaka J (2002) J Biomed Mater Res 62:265Google Scholar
- 380.Ignatius AA, Augat P, Claes LE (2001) J Biomater Sci Polym Edn 12:185Google Scholar
- 381.Ignatius AA, Wolf S, Augat P, Claes LE (2001) J Biomed Mater Res 57:126Google Scholar
- 382.Kikuchi M, Tanaka J (2000) J Ceram Soc Jpn 108:642Google Scholar
- 383.Aunoble S, Clement D, Frayssinet P, Harmand MF, le Huec JC (2006) J Biomed Mater Res A 78A:416Google Scholar
- 384.Kikuchi M, Koyama Y, Yamada T, Imamura Y, Okada T, Shirahama N, Akita K, Takakuda K, Tanaka J (2004) Biomaterials 25:5979Google Scholar
- 385.Chen TM, Yao CH, Wang HJ, Chou GH, Lee TW, Lin FH (1998) Mater Chem Phys 55:44Google Scholar
- 386.Dong GC, Chen HM, Yao CH (2008) J Biomed Mater Res A 84A:167Google Scholar
- 387.Yao CH, Liu BS, Hsu SH, Chen YS, Tsai CC (2004) J Biomed Mater Res A 69A:709Google Scholar
- 388.Lin FH, Yao CH, Sun JS, Liu HC, Huang CW (1998) Biomaterials 19:905Google Scholar
- 389.Eslaminejad MB, Mirzadeh H, Mohamadi Y, Nickmahzar A (2007) J Tissue Eng Regen Med 1:417Google Scholar
- 390.Takahashi Y, Yamamoto M, Tabata Y (2005) Biomaterials 26:3587Google Scholar
- 391.Bigi A, Cantelli I, Panzavolta S, Rubini K (2004) J Appl Biomat Biomech 2:81Google Scholar
- 392.Yang SH, Hsu CK, Wang KC, Hou SM, Lin FH (2005) J Biomed Mater Res B Appl Biomater 74B:468Google Scholar
- 393.Kato M, Namikawa T, Terai H, Hoshino M, Miyamoto S, Takaoka K (2006) Biomaterials 27:3927Google Scholar
- 394.Muramatsu K, Oba K, Mukai D, Hasegawa K, Masuda S, Yoshihara Y (2007) J Mater Sci Mater Med 18:513Google Scholar
- 395.Bleach NC, Tanner KE, Kellomäki M, Törmälä P (2001) J Mater Sci Mater Med 12:911Google Scholar
- 396.Liu L, Xiong Z, Yan YN, Hu YY, Zhang RJ, Wang SG (2007) J Biomed Mater Res A 82A:618Google Scholar
- 397.Zhang Y, Zhang MQ (2001) J Biomed Mater Res 55:304Google Scholar
- 398.Rai B, Teoh SH, Hutmacher DW, Cao T, Ho KH (2005) Biomaterials 26:3739Google Scholar
- 399.Rai B, Teoh SH, Ho KH, Hutmacher DW, Cao T, Chen F, Yacob K (2004) Biomaterials 25:5499Google Scholar
- 400.Lei Y, Rai B, Ho KH, Teoh SH (2007) Mater Sci Eng C 27:293Google Scholar
- 401.Miyai T, Ito A, Tamazawa G, Matsuno T, Sogo Y, Nakamura C, Yamazaki A, Satoh T (2008) Biomaterials 29:350Google Scholar
- 402.Takahashi Y, Yamamoto M, Tabata Y (2005) Biomaterials 26:4856Google Scholar
- 403.Ignatius AA, Betz O, Augat P, Claes LE (2001) J Biomed Mater Res Appl Biomater 58:701Google Scholar
- 404.Miao X, Lim WK, Huang X, Chen Y (2005) Mater Lett 59:4000Google Scholar
- 405.Brodie JC, Goldie E, Connel G, Merry J, Grant MH (2005) J Biomed Mater Res A 73A:409Google Scholar
- 406.Zhang LF, Sun R, Xu L, Du J, Xiong ZC, Chen HC, Xiong CD (2008) Mater Sci Eng C 28:141Google Scholar
- 407.Ignjatovic N, Ninkov P, Ajdukovic Z, Konstantinovic V, Uskokovic D (2005) Mater Sci Forum 494:519Google Scholar
- 408.Ignjatovic N, Ninkov P, Ajdukovic Z, Vasiljevic-Radovic D, Uskokovic D (2007) J Eur Ceram Soc 27:1589Google Scholar
- 409.Ignjatovic N, Ninkov P, Kojic V, Bokurov M, Srdic V, Krnojelac D, Selakovic S, Uskokovic D (2006) Microsc Res Tech 69:976Google Scholar
- 410.Ajdukovic Z, Ignjatovic N, Petrovic D, Uskokovic D (2007) J Biomater Appl 21:317Google Scholar
- 411.Kim HW, Knowles JC, Kim HE (2004) J Biomed Mater Res A 70A:467Google Scholar
- 412.Matsuda A, Ikoma T, Kobayashi H, Tanaka J (2004) Mater Sci Eng C 24:723Google Scholar
- 413.Tortet L, Gavarri JR, Nihoul G, Dianoux AJ (1997) Solid State Ionics 97:253Google Scholar
- 414.Tortet L, Gavarri JR, Musso J, Nihoul G, Sarychev AK (1998) J Solid State Chem 141:392Google Scholar
- 415.Park MS, Eanes ED, Antonucci JM, Skrtic D (1998) Dent Mater 14:137Google Scholar
- 416.Skrtic D, Antonucci JM, Eanes ED, Eichmiller FC, Schumacher GE (2000) J Biomed Mater Res 53:381Google Scholar
- 417.Skrtic D, Antonucci JM, Eanes ED, Eidelman N (2004) Biomaterials 25:1141Google Scholar
- 418.Skrtic D, Antonucci JM (2003) Biomaterials 24:2881Google Scholar
- 419.Gutierrez MC, Jobbágy M, Ferrer ML, del Monte F (2008) Chem Mater 20:11Google Scholar
- 420.Hakimimehr D, Liu DM, Troczynski T (2005) Biomaterials 26:7297Google Scholar
- 421.Perkin KK, Turner JL, Wooley KL, Mann S (2005) Nano Lett 5:1457Google Scholar
- 422.LeGeros RZ, Chohayeb A, Shulman A (1982) J Dent Res 61(Special issue):343Google Scholar
- 423.Brown WE, Chow LC (1983) J Dent Res 62(Special issue):672Google Scholar
- 424.Brown WE, Chow LC (1985) US Patent 4518430, 21 MayGoogle Scholar
- 425.Tas AC (2007) Int J Appl Ceram Technol 4:152Google Scholar
- 426.Driskell TD, Heller AL, Koenigs JF (1975) US Patent 3913229, 21 OctoberGoogle Scholar
- 428.Barrelet JA, Hofmann M, Grover LM, Gbureck U (2003) Adv Mater 15:2091Google Scholar
- 429.Bigi A, Bracci B, Panzavolta S (2004) Biomaterials 25:2893Google Scholar
- 430.Bigi A, Panzavolta S, Sturba L, Torricelli P, Fini M, Giardino R (2006) J Biomed Mater Res A 78A:739Google Scholar
- 431.Panzavolta S, Torricelli P, Sturba L, Bracci B, Giardino R, Bigi A (2008) J Biomed Mater Res A 84A:965Google Scholar
- 432.Rammelt S, Neumann M, Hanisch U, Reinstorf A, Pompe W, Zwipp H, Biewener A (2005) J Biomed Mater Res A 73A:284Google Scholar
- 433.Wang X, Ye J, Wang Y, Chen L (2007) J Am Ceram Soc 90:962Google Scholar
- 434.https://doi.org/en.wikipedia.org/wiki/Concrete. Accessed June 2008
- 435.Kim SB, Kim YJ, Yoon TL, Park SA, Cho IH, Kim EJ, Kim IA, Shin JW (2004) Biomaterials 25:5715Google Scholar
- 436.Vallo CI, Montemartini PE, Fanovich MA, Lópes JMP, Cuadrado TR (1999) J Biomed Mater Res Appl Biomater 48:150Google Scholar
- 437.Sogal A, Hulbert SF (1992) Bioceramics 5:213Google Scholar
- 438.Harper EJ, Behiri JC, Bonfield W (1995) J Mater Sci Mater Med 6:799Google Scholar
- 439.Harper EJ, Braden M, Bonfield W (2001) J Mater Sci Mater Med 11:491Google Scholar
- 440.Moursi AM, Winnard AV, Winnard PL, Lannutti JJ, Seghi RR (2002) Biomaterials 23:133Google Scholar
- 441.Dalby MJ, Di Silvio L, Harper EJ, Bonfield W (2001) Biomaterials 22:1739Google Scholar
- 442.Dalby MJ, Di Silvio L, Harper EJ, Bonfield W (2002) Biomaterials 23:569Google Scholar
- 443.Itokawa H, Hiraide T, Moriya M, Fujimoto M, Nagashima G, Suzuki R, Fujimoto T (2007) Biomaterials 28:4922Google Scholar
- 444.Cheang P, Khor KA (2003) Mater Sci Eng A 345:47Google Scholar
- 445.Dalby MJ, Di Silvio L, Harper EJ, Bonfield W (1999) J Mater Sci Mater Med 10:793Google Scholar
- 446.Deb S, Braden M, Bonfield W (1995) Biomaterials 16:1095Google Scholar
- 447.Borzacchiello A, Ambrosio L, Nicolais L, Harper EJ, Tanner KE, Bonfield W (1998) J Mater Sci Mater Med 9:835Google Scholar
- 448.Ohgaki M, Yamashita K (2003) J Am Ceram Soc 86:1440Google Scholar
- 449.del Real RP, Padilla S, Vallet-Regi M (2000) J Biomed Mater Res 52:1Google Scholar
- 450.Saito M, Maruoka A, Mori T, Sugano N, Hino K (1994) Biomaterials 15:156Google Scholar
- 451.Watson KE, Ten Huisen KS, Brown PW (1999) J Mater Sci Mater Med 10:205Google Scholar
- 452.Reed CS, Ten Huisen KS, Brown PW, Allcock HR (1996) Chem Mater 8:440Google Scholar
- 453.Peter SJ, Kim P, Yasko AW, Yaszemski MJ, Mikos AG (1999) J Biomed Mater Res 44:314Google Scholar
- 454.He S, Yaszemski MJ, Yasko AW, Engel PS, Mikos AG (2000) Biomaterials 21:2389Google Scholar
- 455.Ignjatovic N, Jovanovic J, Suljovrujic E, Uskokovic D (2003) Biomed Mater Eng 13:401Google Scholar
- 456.Fujishiro Y, Takahashi K, Sato T (2001) J Biomed Mater Res 54:230Google Scholar
- 457.Miyazaki K, Horibe T, Antonucci JM, Takagi S, Chow LC (1993) Dent Mater 9:41Google Scholar
- 458.Miyazaki K, Horibe T, Antonucci JM, Takagi S, Chow LC (1993) Dent Mater 9:46Google Scholar
- 459.Dos Santos LA, De Oliveira LC, Rigo ECS, Carrodeguas RG, Boschi AO, De Arruda ACF (1999) Bone 25:99SGoogle Scholar
- 460.Greish YE, Brown PW, Bender JD, Allcock HR, Lakshmi S, Laurencin CT (2007) J Am Ceram Soc 90:2728Google Scholar
- 461.Greish YE, Bender JD, Lakshmi S, Brown PW, Allcock HR, Laurencin CT (2006) J Biomed Mater Res A 77A:416Google Scholar
- 462.Greish YE, Bender JD, Lakshmi S, Brown PW, Allcock HR, Laurencin CT (2005) Biomaterials 26:1Google Scholar
- 463.Mickiewicz RA, Mayes AM, Knaack D (2002) J Biomed Mater Res 61:581Google Scholar
- 464.Carey LE, Xu HHK, Simon CG, Takagi S, Chow LC (2005) Biomaterials 26:5002Google Scholar
- 465.Miao X, Tan LP, Tan LS, Huang X (2007) Mater Sci Eng C 27:274Google Scholar
- 466.Lickorish D, Guan L, Davies JE (2007) Biomaterials 28:1495Google Scholar
- 467.Xu HHK, Simon CG (2005) Biomaterials 26:1337Google Scholar
- 468.Zhang L, Li Y, Zhou G, Lu GY, Zuo Y (2006) J Inorg Mater 21:1197Google Scholar
- 469.Ruhe PQ, Hedberg EL, Padron NT, Spauwen PHM, Jansen JA, Mikos AG (2005) J Biomed Mater Res A 74A:533Google Scholar
- 470.Guo DG, Sun HL, Xu KW, Han Y (2007) J Biomed Mater Res B Appl Biomater 82B:533Google Scholar
- 471.Habraken WJEM, Wolke JGC, Mikos AG, Jansen JA (2006) J Biomater Sci Polym Edn 17:1057Google Scholar
- 472.Ruhe PQ, Hedberg-Dirk EL, Padron NT, Spauwen PHM, Jansen JA, Mikos AG (2006) Tissue Eng 12:789Google Scholar
- 473.Ruhe PQ, Hedberg EL, Padron NT, Spauwen PHM, Jansen JA, Mikos AG (2003) J Bone Joint Surg (Am) 85A(Suppl 3):75Google Scholar
- 474.Ruhe PQ, Boerman OC, Russel FGM, Spauwen PHM, Mikos AG, Jansen JA (2005) J Control Release 106:162Google Scholar
- 475.Plachokova A, Link D, van den Dolder J, van den Beucken J, Jansen JA (2007) J Tissue Eng Regen Med 1:457Google Scholar
- 476.Webster TJ, Siegel RW, Bizios R (1999) Biomaterials 20:1221Google Scholar
- 477.Webster TJ, Ergun C, Doremus RH, Siegel RW, Bizios R (2000) J Biomat Med Res 51:475Google Scholar
- 478.Webster TJ, Ergun C, Doremus RH, Siegel RW, Bizios R (2000) Biomaterials 21:1803Google Scholar
- 479.Li G, Huang J, Li Y, Zhang R, Deng B, Zhang J, Aoki H (2007) Biomed Mater Eng 17:321Google Scholar
- 480.Tadic D, Peters F, Epple M (2002) Biomaterials 23:2553Google Scholar
- 481.Xu HHK, Sun L, Weir MD, Antonucci JM, Takagi S, Chow LC, Peltz M (2006) J Dent Res 85:722Google Scholar
- 482.Xu HHK, Weir MD, Sun L, Takagi S, Chow LC (2007) J Dent Res 86:378Google Scholar
- 483.Xu HHK, Weir MD, Sun L (2007) Dent Mater 23:1482Google Scholar
- 484.Xu HHK, Sun L, Weir MD, Takagi S, Chow LC, Hockey B (2007) J Biomed Mater Res B Appl Biomater 81B:116Google Scholar
- 485.Deng XM, Hao JY, Wang CS (2001) Biomaterials 22:2867Google Scholar
- 486.Hong ZK, Zhang PB, He CL, Qiu XY, Liu AX, Chen L, Chen X, Jing X (2005) Biomaterials 26:6296Google Scholar
- 487.Deng C, Weng J, Cheng QY, Zhou SB, Lu X, Wan JX, Qu SX, Feng B, Li XH (2007) Curr Appl Phys 7:679Google Scholar
- 488.Deng C, Weng J, Lu X, Zhou SB, Wan JX, Qu SX, Feng B, Li XH, Cheng QY (2008) Mater Lett 62:607Google Scholar
- 489.Kothapalli CR, Shaw MT, Wei M (2005) Acta Biomater 1:653Google Scholar
- 490.Hong Z, Qiu X, Sun J, Deng M, Chen X, Jing X (2004) Polymer 45:6699Google Scholar
- 491.Xiao Y, Li D, Fan H, Li X, Gu Z, Zhang X (2007) Mater Lett 61:59Google Scholar
- 492.Qiu X, Han Y, Zhuang X, Chen X, Li Y, Jing X (2007) J Nanoparticle Res 9:901Google Scholar
- 493.Kim SS, Park MS, Jeon Q, Choi CY, Kim BS (2006) Biomaterials 27:1399Google Scholar
- 494.Hong Z, Zhang P, Liu A, Chen L, Chen X, Jing X (2007) J Biomed Mater Res A 81A:515Google Scholar
- 495.Huang YX, Ren J, Chen C, Ren TB, Zhou XY (2008) J Biomater Appl 22:409Google Scholar
- 496.Du C, Cui FZ, Zhu XD, de Groot K (1999) J Biomed Mater Res 44:407Google Scholar
- 497.Wang RZ, Cui FZ, Lu HB, Wen HB, Ma CL, Li HD (1995) J Mater Sci Lett 14:490Google Scholar
- 498.Du C, Cui FZ, Feng QL, Zhu XD, de Groot K (1998) J Biomed Mater Res 42:540Google Scholar
- 499.Kikuchi M, Itoh S, Ichinose S, Shinomiya K, Tanaka J (2001) Biomaterials 22:1705Google Scholar
- 500.Kikuchi M, Matsumoto HN, Yamada T, Koyama Y, Takakuda K, Tanaka J (2004) Biomaterials 25:63Google Scholar
- 501.Lynn AK, Nakamura T, Patel N, Porter AE, Renouf AC, Laity PR, Best SM, Cameron RE, Shimizu Y, Bonfield W (2005) J Biomed Mater Res A 74A:447Google Scholar
- 502.Chang MC, Tanaka J (2002) Biomaterials 23:4811Google Scholar
- 503.Chang MC, Tanaka J (2002) Biomaterials 23:3879Google Scholar
- 504.Murugan R, Ramakrishna S (2006) Appl Phys Lett 88:193124Google Scholar
- 505.Wang Y, Yang C, Chen X, Zhao N (2006) Adv Eng Mater 8:97Google Scholar
- 506.Thomas V, Dean DR, Jose MV, Mathew B, Chowdhury S, Vohra YK (2007) Biomacromolecules 8:631Google Scholar
- 507.Fukui N, Sato T, Kuboki Y, Aoki H (2008) Biomed Mater Eng 18:25Google Scholar
- 508.Liao SS, Tamura K, Zhu Y, Wang W, Uo M, Akasaka T, Cui FZ, Watari F (2006) J Biomed Mater Res A 76A:820Google Scholar
- 509.Liao SS, Cui FZ, Zhu Y (2004) J Bioact Compat Polym 19:117Google Scholar
- 510.Liao SS, Cui FZ, Zhang W, Feng QL (2004) J Biomed Mater Res B Appl Biomater 69B:158Google Scholar
- 511.Liao SS, Cui FZ (2004) Tissue Eng 10:73Google Scholar
- 512.Liao SS, Wang W, Uo M, Ohkawa S, Akasaka T, Tamura K, Cui FZ, Watari F (2005) Biomaterials 26:7564–7571Google Scholar
- 513.Li X, Feng Q, Cui FZ (2006) Mater Sci Eng C 26:716Google Scholar
- 514.Zhou DS, Zhao KB, Li Y, Cui FZ, Lee IS (2006) J Bioact Compat Polym 21:373Google Scholar
- 515.Zhang C, Hu YY, Cui FZ, Zhang SM, Ruan DK (2006) Biomed Mater 1:56Google Scholar
- 516.Liao S, Watari F, Zhu Y, Uo M, Akasaka T, Wang W, Xu G, Cui F (2007) Dent Mater 23:1120Google Scholar
- 517.Degirmenbasi N, Kalyon DM, Birinci E (2006) Colloids Surf B Biointerfaces 48:42Google Scholar
- 518.Zhang SM, Cui FZ, Liao SS, Zhu Y, Han L (2003) J Mater Sci Mater Med 14:641Google Scholar
- 519.Sotome S, Uemura T, Kikuchi M, Chen J, Itoh S, Tanaka J, Tateishi T, Shinomiya K (2004) Mater Sci Eng C 24:341Google Scholar
- 520.Chang MC, Ko CC, Douglas WH (2003) Biomaterials 24:3087Google Scholar
- 521.Kim HW, Kim HE, Vehid S (2005) Biomaterials 26:5221Google Scholar
- 522.Chang MC, Ikoma T, Tanaka J (2004) J Mater Sci 39:5547. doi: https://doi.org/10.1023/B:JMSC.0000039284.70028.fa Google Scholar
- 523.Teng S, Shi J, Peng B, Chen L (2006) Compos Sci Technol 66:1532Google Scholar
- 524.Chang MC, Ko CC, Douglas WH (2003) Biomaterials 24:2853Google Scholar
- 525.Mobini S, Javadpour J, Hosseinalipour M, Ghazi-Khansari M, Khavandi A, Rezaie HR (2008) Adv Appl Ceram 107:4Google Scholar
- 526.Wang XJ, Li Y, Wei J, de Groot K (2002) Biomaterials 23:4787Google Scholar
- 527.Lewandrowski KU, Bondre SP, Wise DL, Trantolo DJ (2003) Biomed Mater Eng 13:115Google Scholar
- 530.Wei J, Li Y (2004) Eur Polym J 40:509Google Scholar
- 531.Wang H, Li Y, Zuo Y, Li J, Ma S, Cheng L (2007) Biomaterials 28:3338Google Scholar
- 532.Sender C, Dantras E, Dantras-Laffont L, Lacoste MH, Dandurand J, Mauzac M, Lacout JL, Lavergne C, Demont P, Bernes A, Lacabanne C (2007) J Biomed Mater Res B Appl Biomater 83B:628Google Scholar
- 533.Yang K, Wei J, Wang CY, Li Y (2007) Chin Sci Bull 52:267Google Scholar
- 534.Zhang X, Li Y, Lv GY, Zuo Y, Mu YH (2006) Polym Degrad Stab 91:1202Google Scholar
- 535.Huang M, Feng J, Wang J, Zhang X, Li Y, Yan Y (2003) J Mater Sci Mater Med 14:655Google Scholar
- 536.Zhang X, Li Y, Zuo Y, Lv GY, Mu YH, Li H (2007) Composites A 38:843Google Scholar
- 537.Lan W, Li Y, Yi Z, Li Z, Mu YH, Jimei H (2006) Mater Sci Forum 510–511:938Google Scholar
- 539.Zhang X, Li Y, Lv GY, Zuo Y, Mu YH, Lan W (2005) Funct Mater 36:896Google Scholar
- 541.Xu F, Li Y, Wang X, Wei J, Yang A (2004) J Mater Sci 39:5669. doi: https://doi.org/10.1023/B:JMSC.0000040074.64787.b3 Google Scholar
- 542.Wang HS, Wang GX, Pan QX (2005) Electroanalysis 17:1854Google Scholar
- 543.Pramanik N, Mohapatra S, Pramanik P, Bhargava P (2007) J Am Ceram Soc 90:369Google Scholar
- 544.Pramanik N, Bhargava P, Alam S, Pramanik P (2006) Polym Compos 27:633Google Scholar
- 545.Zhang L, Li Y, Yang A, Peng X, Wang X, Zhang X (2005) J Mater Sci Mater Med 16:213Google Scholar
- 546.Zhang YF, Cheng XR, Chen Y, Shi B, Chen XH, Xu DX, Ke J (2007) J Biomater Appl 21:333Google Scholar
- 547.Kong L, Gao Y, Lu G, Gong Y, Zhao N, Zhang X (2006) Eur Polym J 42:3171Google Scholar
- 548.Lu XY, Wang XH, Qu SX, Weng J (2008) J Inorg Mater 23:332Google Scholar
- 550.Huang J, Lin YW, Fu XW, Best SM, Brooks RA, Rushton N, Bonfield W (2007) J Mater Sci Mater Med 18:2151Google Scholar
- 551.Lee HJ, Choi HW, Kim KJ, Lee SC (2006) Chem Mater 18:5111Google Scholar
- 552.Lee HJ, Kim SE, Choi HW, Kim CW, Kim KJ, Lee SC (2007) Eur Polym J 43:1602Google Scholar
- 553.Pang P, Li W, Liu Y (2007) Rare Met 26:118Google Scholar
- 554.Li W, Pang P, Liu Y (2007) Trans Nonferrous Met Soc China 17(Special Issue):S1148Google Scholar
- 555.Hao JY, Liu Y, Zhou S, Li Z, Deng X (2003) Biomaterials 24:1531Google Scholar
- 556.Yan Y, Li Y, Zheng Y, Yi Z, Wei J, Xia C, Chen Y (2003) Eur Polym J 39:411Google Scholar
- 557.Bhattacharyya S, Nair LS, Singh A, Krogman NR, Bender J, Greish YE, Brown PW, Allcock HR, Laurencin CT (2005) MRS Symp Proc 845:91Google Scholar
- 558.Sinha A, Nayar S, Agrawal A, Bhattacharyya D, Ramachandrarao P (2003) J Am Ceram Soc 86:357Google Scholar
- 559.Zuo Y, Li Y, Wei J, Han J, Xu F (2004) Funct Mater 35:513Google Scholar
- 560.Zhou G, Li Y, Zhang L, Zuo Y, Jansen JA (2007) J Biomed Mater Res A 83A:931Google Scholar
- 562.Furuzono T, Kishida A, Tanaka J (2004) J Mater Sci Mater Med 15:19Google Scholar
- 563.Korematsu A, Furuzono T, Yasuda S, Tanaka J, Kishida A (2004) J Mater Sci 39:3221. doi: https://doi.org/10.1023/B:JMSC.0000025865.44900.74 Google Scholar
- 564.Korematsu A, Furuzono T, Yasuda S, Tanaka J, Kishida A (2005) J Mater Sci Mater Med 16:67Google Scholar
- 565.Yang K, Wang C, Wei J (2007) Composites B 38:306Google Scholar
- 566.Jiang L, Li Y, Zhang L, Wang XJ (2008) J Inorg Mater 23:135Google Scholar
- 567.Jiang L, Li Y, Zhang L, Liao J (2008) J Mater Sci Mater Med 19:981Google Scholar
- 568.Liou SC, Chen SY, Liu DM (2004) J Mater Sci Mater Med 15:1261Google Scholar
- 569.Liu L, Liu J, Wang M, Min S, Cai Y, Zhu L, Yao J (2008) J Biomater Sci Polym Edn 19:325Google Scholar
- 570.Ren YJ, Sun XD, Cui FZ, Wei YT, Cheng ZJ, Kong XD (2007) J Bioact Compat Polym 22:465Google Scholar
- 571.Mikołajczyk T, Rabiej S, Bogun M (2006) J Appl Polym Sci 101:760Google Scholar
- 572.Wei J, Li Y, Lau KT (2007) Composites B 38:301Google Scholar
- 573.Sundaraseelan J, Sastry TP (2007) J Biomed Nanotechnol 3:401Google Scholar
- 574.Leeuwenburgh SCG, Jansen JA, Mikos AG (2007) J Biomater Sci Polym Ed 18:1547Google Scholar
- 575.Sun TS, Guan K, Shi SS, Zhu B, Zheng YJ, Cui FZ, Zhang W, Liao SS (2004) Chin J Traumatol 7:18Google Scholar
- 576.Itoh S, Kikuehi M, Koyama Y, Takakuda K, Shinomiya K, Tanaka J (2004) Cell Transplant 13:451Google Scholar
- 577.Hu Q, Li BQ, Wang M, Shen JC (2004) Biomaterials 25:779Google Scholar
- 578.Wei G, Ma PX (2004) Biomaterials 25:4749Google Scholar
- 579.Liou SC, Chen SY, Liu DM (2003) Biomaterials 24:3981Google Scholar
- 580.Liou SC, Chen SY, Liu DM (2005) J Biomed Mater Res B Appl Biomater 73B:117Google Scholar
- 581.Huang J, Best SM, Bonfield W, Brooks RA, Rushton N, Jayasinghe SN, Edirisinghe MJ (2004) J Mater Sci Mater Med 15:441Google Scholar
- 582.Kong L, Gao Y, Cao W, Gong Y, Zhao N, Zhang X (2005) J Biomed Mater Res A 75A:275Google Scholar
- 583.Christenson EM, Anseth KS, van den Beucken JJJP, Chan CK, Ercan B, Jansen JA, Laurencin CT, Li WJ, Murugan R, Nair LS, Ramakrishna S, Tuan RS, Webster TJ, Mikos AG (2007) J Orthop Res 25:11Google Scholar
- 584.Nimni ME (ed) (1988) Collagen. CRC Press, Boca Raton, FLGoogle Scholar
- 585.Olmo N, Turnay J, Herrera JI, Gavilanes JG, Lizarbe MA (1996) J Biomed Mater Res 30:77Google Scholar
- 586.Xie J, Baumann MJ, McCabe LR (2004) J Biomed Mater Res A 71A:108Google Scholar
- 587.Tcacencu I, Wendel M (2008) J Mater Sci Mater Med 19:2015Google Scholar
- 588.Yamauchi K, Goda T, Takeuchi N, Einaga H, Tanabe T (2004) Biomaterials 25:5481Google Scholar
- 589.Du C, Cui FZ, Zhang W, Feng QL, Zhu XD, de Groot K (2000) J Biomed Mater Res 50:518Google Scholar
- 590.Hellmich C, Ulm FJ (2002) J Biomech 35:1199Google Scholar
- 591.Boskey AL (1989) J Phys Chem 93:1628Google Scholar
- 592.Mathers NJ, Czernuszka JT (1991) J Mater Sci Lett 10:992Google Scholar
- 593.Sukhodub LF, Moseke C, Sukhodub LB, Sulkio-Cleff B, Maleev VYa, Semenov MA, Bereznyak EG, Bolbukh TV (2004) J Mol Struct 704:53Google Scholar
- 594.Roveri N, Falini G, Sidoti MC, Tampieri A, Landi E, Sandri M, Parma B (2003) Mater Sci Eng C 23:441Google Scholar
- 595.Tampieri A, Celotti G, Landi E (2005) Anal Bioanal Chem 381:568Google Scholar
- 596.Tampieri Α, Celotti G, Landi E, Sandri M, Roveri N, Falini G (2003) J Biomed Mater Res A 67A:618Google Scholar
- 597.Mehlisch DR, Taylor TD, Leibold DG, Hiatt R, Waite DE, Waite PD, Laskin DM, Smith ST, Koretz MM (1987) J Oral Maxillofac Surg 45:408Google Scholar
- 598.Okazaki M, Ohmae H, Takahashi J, Kimura H, Sakuda M (1990) Biomaterials 11:568Google Scholar
- 599.Ten Huisen KS, Martin RI, Klimkiewicz M, Brown PW (1995) J Biomed Mater Res 29:803Google Scholar
- 600.Marouf HA, Quayle AA, Sloan P (1990) Int J Oral Maxillofac Implants 5:148Google Scholar
- 601.Zerwekh JE, Kourosh S, Scheinberg R, Kitano T, Edwards ML, Shin D, Selby DK (1992) J Orthop Res 10:565Google Scholar
- 602.Clarke KI, Graves SE, Wong ATC, Triffit JT, Francis MJO, Czernuszka JT (1993) J Mater Sci Mater Med 4:107Google Scholar
- 603.Rovira Α, Bareille R, Lopez L, Rouasis F, Bordenave L, Rey C, Rabaud M (1993) J Mater Sci Mater Med 4:372Google Scholar
- 604.Zhang QQ, Ren L, Wang C, Liu LR, Wen XJ, Liu YH, Zhang XD (1996) Artif Cells Blood Substit Immobil Biotechnol 24:693Google Scholar
- 605.Bakoš D, Soldán M, Hernández-Fuentes I (1999) Biomaterials 20:191Google Scholar
- 606.John A, Hong L, Ikada Y, Tabata Y (2001) J Biomater Sci Polym Ed 12:689Google Scholar
- 607.ltoh S, Kikuchi M, Takakuda K, Koyama Y, Matsumoto HN, Ichinose S, Tanaka J, Kawauchi T, Shinomiya K (2001) J Biomed Mater Res 54:445Google Scholar
- 608.Shinomiya K, Itoh S, Kawauchi T, Kikuchi M, Tanaka J (2001) Tissue Eng Therap Use 5:165Google Scholar
- 609.Uskokovic V, Ignjatovic N, Petranovic N (2002) Mater Sci Forum 413:269Google Scholar
- 610.Wahl DA, Czernuszka JT (2006) Eur Cells Mater 11:43Google Scholar
- 611.Ishikawa H, Koshino T, Takeuchi R, Saito T (2001) Biomaterials 22:1689Google Scholar
- 612.Sachlos E, Gotora D, Czernuszka JT (2006) Tissue Eng 12:2479Google Scholar
- 613.Venugopal J, Ramakrishna S, Low S, Choon AT, Kumar TSS (2008) J Mater Sci Mater Med 19:2039Google Scholar
- 614.Teng SH, Lee EJ, Park CS, Choi WY, Shin DS, Kim HE (2008) J Mater Sci Mater Med 19:2453Google Scholar
- 615.Song JH, Kim HE, Kim HW (2007) J Biomed Mater Res B Appl Biomater 83B:248Google Scholar
- 616.Mittelmeier H, Nizzard M (1982) In: Hackenbroch MH, Refior HJ, Jäger MG (eds) Osteogenese und Knochenwachstum. Thieme, Stuttgart, GermanyGoogle Scholar
- 617.Serre CM, Papillard M, Chavassieux P, Boivin G (1993) Biomaterials 14:97Google Scholar
- 618.Scabbia A, Trombelli L (2004) J Clin Periodontol 31:348Google Scholar
- 619.Yamasaki Y, Yoshida Y, Okazaki M, Shimazu A, Kubo T, Akagawa Y, Uchida T (2003) Biomaterials 24:4913Google Scholar
- 620.Wang X, Grogan SP, Rieser F, Winkelmann V, Maquet V, Berge ML, Mainil-Varlet P (2004) Biomaterials 25:3681Google Scholar
- 621.Chang MC, Ikonama T, Kikuchi M, Tanaka J (2002) J Mater Sci Mater Med 13:993Google Scholar
- 622.Iijima M, Moriwaki Y, Kuboki Y (1996) Connect Tissue Res 32:519Google Scholar
- 623.Miyamoto Y, Ishikawa K, Takechi M, Toh T, Yuasa T, Nagayama M, Suzuki K (1998) Biomaterials 19:707Google Scholar
- 624.Iijima M, Moriwaki Y, Kuboki Y (1994) J Cryst Growth 137:553Google Scholar
- 625.Iijima M, Iijima K, Moriwaki Y, Kuboki Y (1994) J Cryst Growth 140:91Google Scholar
- 626.Lawson AC, Czernuszka JT (1998) Proc Inst Mech Eng H 212:413Google Scholar
- 627.Itoh S, Kikuchi M, Takakuda K, Nagaoka K, Koyama Y, Tanaka J, Shinomiya K (2002) J Biomed Mater Res 63:507Google Scholar
- 628.Kikuchi M, Ikoma T, Itoh S, Matsumoto HN, Koyama Y, Takakuda K, Shinomiya K, Tanaka J (2004) Compos Sci Technol 64:819Google Scholar
- 629.Yang XB, Bhataagar RS, Li S, Oreffo RO (2004) Tissue Eng 14:1148Google Scholar
- 630.Doi Y, Horiguchi T, Moriwaki Y, Kitago H, Kajimoto T, Iwayama Y (1996) J Biomed Mater Res 31:43Google Scholar
- 631.Bradt JH, Mertig M, Teresiak A, Pompe W (1999) Chem Mater 11:2694Google Scholar
- 632.Scharnweber D, Born R, Flade K, Roessler S, Stoelzel M, Worch H (2004) Biomaterials 25:2371Google Scholar
- 633.Li X, Chang J (2008) J Biomed Mater Res A 85A:293Google Scholar
- 634.Mai R, Reinstorf A, Pilling E, Hlawitschka M, Jung R, Gelinsky M, Schneider M, Loukota R, Pompe W, Eckelt U, Stadlinger B (2008) Oral Surg Oral Med Oral Pathol Oral Radiol Endod 105:e9Google Scholar
- 635.Young SW, Andrews WA, Muller H, Constantz B (1991) Invest Radiol 2:470Google Scholar
- 636.Rovira A, Amedee J, Bareille R, Radaud M (1996) Biomaterials 17:1535Google Scholar
- 637.Kazim M, Katowitz JA, Fallon M, Piest KL (1992) Ophthal Plast Reconstr Surg 8:94Google Scholar
- 638.Hirota K, Nishihara K, Tanaka H (1993) Biomed Mater Eng 3:147Google Scholar
- 641.Yunoki S, Ikoma T, Tsuchiya A, Monkawa A, Ohta K, Sotome S, Shinomiya K, Tanaka J (2007) J Biomed Mater Res B Appl Biomater 80B:166Google Scholar
- 642.Chapman MW, Bucholz R, Cornell C (1997) J Bone Joint Surg Am 79A:495Google Scholar
- 643.Rodrigues CVM, Serricella P, Linhares ABR, Guerdes RM, Borojevic R, Rossi MA, Duarte MEL, Farina M (2003) Biomaterials 24:4987Google Scholar
- 644.Lickorish D, Ramshaw JAM, Werkmeister JA, Glattauer V, Howlett CR (2004) J Biomed Mater Res A 68A:19Google Scholar
- 645.Hsu FY, Chueh SC, Wang JY (1999) Biomaterials 20:1931Google Scholar
- 646.Wu TJ, Huang HH, Lan CW, Lin CH, Hsu FY, Wang YJ (2004) Biomaterials 25:651Google Scholar
- 647.Liao SS, Watari F, Uo M, Ohkawa S, Tamura K, Wang W, Cui FZ (2005) J Biomed Mater Res B Appl Biomater 74B:817Google Scholar
- 648.Yokoyama A, Gelinsky M, Kawasaki T et al (2005) J Biomed Mater Res B Appl Biomater 75B:464Google Scholar
- 649.Zou C, Weng W, Deng XJ, Cheng K, Liu X, Du P, Shen G, Han G (2005) Biomaterials 26:5276Google Scholar
- 650.Martins VCA, Goissis G (2000) Artif Organs 24:224Google Scholar
- 651.Gotterbarm T, Richter W, Jung M, Berardi Vilei S, Mainil-Varlet P, Yamashita T, Breusch SJ (2006) Biomaterials 27:3387Google Scholar
- 652.Martins VC, Goissis G, Ribeiro AC, Marcantonio E Jr, Bet MR (1998) Artif Organs 22:215Google Scholar
- 653.Jayaraman M, Subramanian MV (2008) Med Sci Monit 8:BR481Google Scholar
- 654.Ikeda H, Yamaza T, Yoshinari M, Ohsaki Y, Ayukawa Y, Kido MA, Inoue T, Shimono M, Koyano K, Tanaka T (2000) J Periodontol 71:961Google Scholar
- 655.Uchida M, Oyane A, Kim HM, Kokubo T, Ito A (2004) Adv Mater 16:1071Google Scholar
- 656.Oyane A, Uchida M, Ito A (2005) J Biomed Mater Res A 72A:168Google Scholar
- 657.Oyane A, Uchida M, Onuma K, Ito A (2006) Biomaterials 27:167Google Scholar
- 659.Yaylaoglu MB, Korkusuz P, Ors U, Korkusuz F, Hasirci V (1999) Biomaterials 20:711Google Scholar
- 660.Kim HW, Song JH, Kim HE (2005) Adv Funct Mater 15:1988Google Scholar
- 661.Sivakumar M, Panduranga Rao K (2002) Biomaterials 23:3175Google Scholar
- 662.Kim HW, Knowles JC, Kim HE (2005) J Biomed Mater Res B Appl Biomater 74B:686Google Scholar
- 663.Yin YJ, Zhao F, Song XF, Yao KD, Lu WW, Leong JC (2000) J Appl Polym Sci 77:2929Google Scholar
- 664.Kim HW, Yoon BH, Kim HE (2005) J Mater Sci Mater Med 16:1105Google Scholar
- 665.Hillig WB, Choi Y, Murtha S, Natravali N, Ajayan P (2008) J Mater Sci Mater Med 19:11Google Scholar
- 666.Chang MC, Douglas WH, Tanaka J (2006) J Mater Sci Mater Med 17:387Google Scholar
- 667.Chang MC, Douglas WH (2007) J Mater Sci Mater Med 18:2045Google Scholar
- 668.Teng S, Chen L, Guo Y, Shi J (2007) J Inorg Biochem 101:686Google Scholar
- 669.Zhao F, Grayson WL, Ma T, Bunnell B, Lu WW (2006) Biomaterials 27:1859Google Scholar
- 670.Lin HR, Yeh YJ (2004) J Biomed Mater Res B Appl Biomater 71B:52Google Scholar
- 671.Gelinsky M, Eckert M, Despang F (2007) Int J Mater Res (Z Metallkd) 98:749Google Scholar
- 672.Yamaguchi I, Tokuchi K, Fukuzaki H, Koyama Y, Takakuda K, Monma H, Tanaka J (2001) J Biomed Mater Res 55:20Google Scholar
- 673.Zhao F, Yin YJ, Lu WW, Leong JC, Zhang WJ, Zhang JY, Zhang MF, Yao KD (2002) Biomaterials 23:3227Google Scholar
- 674.Shen X, Tong H, Jiang T, Zhu Z, Wan P, Hu J (2007) Compos Sci Technol 67:2238Google Scholar
- 675.Murugan R, Ramakrishna S (2004) Biomaterials 25:3829Google Scholar
- 676.Yoshida A, Miyazaki T, Ishida E, Ashizuka M (2004) Mater Trans 45:994Google Scholar
- 677.Zhang Y, Ni M, Zhang MQ, Ratner B (2003) Tissue Eng 9:337Google Scholar
- 678.Zhang Y, Zhang MQ (2001) J Non-Cryst Solids 282:159Google Scholar
- 679.Zhang Y, Zhang MQ (2002) J Biomed Mater Res 62:378Google Scholar
- 680.Tachaboonyakiat W, Ogomi D, Serizawa T, Akashi M (2006) J Bioact Compat Polym 21:579Google Scholar
- 681.Sreedhar B, Aparna Y, Sairam M, Hebalkar N (2007) J Appl Polym Sci 105:928Google Scholar
- 682.Rusu VM, Ng CH, Wilke M, Tiersch B, Fratzl P, Peter MG (2005) Biomaterials 26:5414Google Scholar
- 683.Pinheiro AG, Pereira FFM, Santos MRP, Freire FNA, Góes JC, Sombra ASB (2007) Polym Compos 28:582Google Scholar
- 684.Wan ACA, Khor E, Hastings GW (1998) J Biomed Mater Res 41:541Google Scholar
- 685.Wan ACA, Khor E, Hastings GW (1997) J Biomed Mater Res 38:235Google Scholar
- 686.Geçer A, Yldz N, Erol M, Çalml A (2008) Polymer Composites 29:84Google Scholar
- 687.Dong H, Ye JD, Wang XP, Yang JJ (2007) J Inorg Mater 22:1007Google Scholar
- 688.Wang X, Ma J, Feng Q, Cui FZ (2002) Biomaterials 23:4591Google Scholar
- 689.Wen HB, de Wijn JR, van Blitterswijk CA, de Groot K (1999) J Biomed Mater Res 46:245Google Scholar
- 690.Liu TY, Chen SY, Liu DM, Liou SC (2005) J Controlled Release 107:112Google Scholar
- 691.Liu Y, Hunziker E, Randall N, de Groot K, Layrolle P (2003) Biomaterials 24:65Google Scholar
- 692.Dorozhkin SV, Dorozhkina EI (2003) Colloids Surf A Physiochem Eng Asp 215:191Google Scholar
- 693.Fu HH, Hu YH, McNelis T, Hollinger JO (2005) J Biomed Mater Res A 74A:40Google Scholar
- 694.Bisht S, Bhakta G, Mitra S, Maitra A (2005) Int J Pharm 288:157Google Scholar
- 695.Kakizawa Y, Miyata K, Furukawa S, Kataoka K (2004) Adv Mater 16:699Google Scholar
- 696.Singh R, Saxena A, Mozumdar S (2008) Int J Appl Ceram Technol 5:1Google Scholar
- 697.Taguchi T, Kishida A, Akashi M (1998) Chem Lett 8:711Google Scholar
- 698.Tachaboonyakiat W, Serizawa T, Akashi M (2001) Polym J 33:177Google Scholar
- 699.Schnepp ZAC, Gonzalez-McQuire R, Mann S (2006) Adv Mater 18:1869Google Scholar
- 700.Bigi A, Boanini E, Gazzano M, Kojdecki MA, Rubini K (2004) J Mater Chem 14:274Google Scholar
- 701.Bigi A, Boanini E, Gazzano M, Rubini K, Torricelli P (2004) Biomed Mater Eng 14:573Google Scholar
- 702.Boanini E, Fini M, Gazzano M, Bigi A (2006) Eur J Inorg Chem 4821Google Scholar
- 703.Boanini E, Torricelli P, Gazzano M, Giardino R, Bigi A (2006) Biomaterials 27:4428Google Scholar
- 704.Sánchez-Salcedo S, Nieto A, Vallet-Regi M (2005) Chem Eng J 137:62Google Scholar
- 705.Román J, Cabañas MV, Peña J, Doadrio JC, Vallet-Regi M (2008) J Biomed Mater Res A 84A:99Google Scholar
- 706.Abiraman S, Varma H, Umashankar P, John A (2002) Biomaterials 23:3023Google Scholar
- 707.Bagot d’Arc M, Daculsi G (2003) J Mater Sci Mater Med 14:229Google Scholar
- 708.Bonucci E, Marini E, Valdinucci F, Fortunato G (1997) Eur J Oral Sci 105:557Google Scholar
- 709.Fortunato G, Marini E, Valdinucci F, Bonucci E (1997) J Cranio Maxillofac Surg 25:124Google Scholar
- 710.Jegoux F, Goyenvalle E, Bagot d’Arc M, Aguado E, Daculsi G (2005) Arch Orthop Trauma Surg 125:153Google Scholar
- 711.Le Guehennec L, Goyenvalle E, Aguado E, Pilet P, Bagot d’Arc M, Daculsi G (2005) J Mater Sci Mater Med 16:29Google Scholar
- 712.Wittkampf A (1989) J Cranio Maxillofac Surg 17:179Google Scholar
- 713.Le Nihouannen D, Guehennec LL, Rouillon T, Pilet P, Bilban M, Layrolle P, Daculsi G (2006) Biomaterials 27:2716Google Scholar
- 714.Le Nihouannen D, Saffarzadeh A, Aguado E, Goyenvalle E, Gauthier O, Moreau F, Pilet P, Spaethe R, Daculsi G, Layrolle P (2007) J Mater Sci Mater Med 18:225Google Scholar
- 715.Le Guehennec L, Goyenvalle E, Aguado E, Pilet P, Spaethe R, Daculsi G (2007) J Mater Sci Mater Med 18:1489Google Scholar
- 716.Le Nihouannen D, Goyenvalle E, Aguado E, Pilet P, Bilban M, Daculsi G, Layrolle P (2007) J Biomed Mater Res A 81A:399Google Scholar
- 717.Le Nihouannen D, Saffarzadeh A, Gauthier O, Moreau F, Pilet P, Spaethe R, Layrolle P, Daculsi G (2008) J Mater Sci Mater Med 19:667Google Scholar
- 718.Yoh R, Matsumoto T, Sasaki JI, Sohmura T (2008) J Biomed Mater Res A 87(1):222Google Scholar
- 719.Boanini E, Torricelli P, Gazzano M, Giardino R, Bigi A (2008) Biomaterials 29:790Google Scholar
- 720.Li L, Wei KM, Lin F, Kong XD, Yao JM (2008) J Mater Sci Mater Med 19:577Google Scholar
- 721.Wang L, Nemoto R, Senna M (2004) J Mater Sci Mater Med 15:261Google Scholar
- 722.Wang L, Nemoto R, Senna M (2002) J Nanoparticle Res 4:535Google Scholar
- 723.Wang L, Nemoto R, Senna M (2004) J Nanoparticle Res 6:91Google Scholar
- 724.Nemoto R, Wang L, Ikoma T, Tanaka J, Senna M (2004) J Nanoparticle Res 6:259Google Scholar
- 725.Wang L, Li CZ, Senna M (2007) J Nanoparticle Res 9:919Google Scholar
- 726.Wang L, Li CZ (2007) Carbohydr Polym 68:740Google Scholar
- 727.Sogo Y, Ito A, Matsuno T, Oyane A, Tamazawa G, Satoh T, Yamazaki A, Uchimura E, Ohno T (2007) Biomed Mater 2:116Google Scholar
- 728.Cross KJ, Huq NL, Palamara JE, Perich JW, Reynolds EC (2005) J Biol Chem 280:15362Google Scholar
- 729.Shchukin DG, Sukhorukov GB, Möhwald H (2003) Chem Mater 15:3947Google Scholar
- 730.Weiss P, Gauthier O, Bouler JM, Grimandi G, Daculsi G (1999) Bone 25(2 Suppl):67SGoogle Scholar
- 731.Daculsi G, Weiss P, Bouler JM, Gauthier O, Millot F, Aguado E (1999) Bone 25(2 Suppl):59SGoogle Scholar
- 732.Turczyn R, Weiss P, Lapkowski M, Daculsi G (2000) J Biomater Sci Polym Ed 11:217Google Scholar
- 733.Bennett S, Connolly K, Lee DR, Jiang Y, Buck D, Hollinger JO, Gruskin EA (1996) Bone 19:101SGoogle Scholar
- 734.Daculsi G, Rohanizadeh R, Weiss P, Bouler JM (2000) J Biomed Mater Res 50:1Google Scholar
- 735.Grimande G, Weiss P, Millot F, Daculsi G (1998) J Biomed Mater Res 39:660Google Scholar
- 736.Weiss P, Lapkowski M, LeGeros RZ, Bouler JM, Jean A, Daculsi G (1997) J Mater Sci Mater Med 8:621Google Scholar
- 737.Weiss P, Bohic S, Lapkowski M, Daculsi G (1998) J Biomed Mater Res 41:167Google Scholar
- 738.Schmitt M, Weiss P, Bourges X, del Valle GA, Daculsi G (2002) Biomaterials 23:2789Google Scholar
- 739.Gauthier O, Müller R, von Stechow D, Lamy B, Weiss P, Bouler JM, Aguado E, Daculsi G (2005) Biomaterials 26:5444Google Scholar
- 740.Weiss P, Layrolle P, Clergeau LP, Enckel B, Pilet P, Amouriq Y, Daculsi G, Giumelli B (2007) Biomaterials 28:3295Google Scholar
- 741.Trojani C, Boukhechba F, Scimeca JC, Vandenbos F, Michiels JF, Daculsi G, Boileau P, Weiss P, Carle GF, Rochet N (2006) Biomaterials 27:3256Google Scholar
- 742.Iooss P, Le Ray AM, Grimandi G, Daculsi G, Merle C (2001) Biomaterials 22:2785Google Scholar
- 744.Rao RR, Kannan TS (2002) Mater Sci Eng C 20:187Google Scholar
- 745.Mansur C, Pope M, Pascucci MR, Shivkumar S (1998) Ceram Int 24:77Google Scholar
- 746.Kim HW, Kim HE, Salih V, Knowles JC (2004) J Biomed Mater Res A 68A:522Google Scholar
- 747.Milella E, Cosentino F, Licciulli A, Massaro C (2001) Biomaterials 22:1425Google Scholar
- 748.Goller G, Demirkiran H, Oktar FN, Demirkesen E (2003) Ceram Int 29:721Google Scholar
- 749.Tancred DC, Carr AJ, McCormack BA (2001) J Mater Sci Mater Med 12:81Google Scholar
- 750.Lopes MA, Silva RF, Monteiro FJ, Santos JD (2000) Biomaterials 21:749Google Scholar
- 751.Juang HY, Hon MH (1994) Mater Sci Eng C 2:77Google Scholar
- 752.Li J, Forbreg S, Hermansson L (1991) Biomaterials 12:438Google Scholar
- 753.Noma T, Shoji N, Wada S, Suzuki T (1993) J Ceram Soc Japan 101:923Google Scholar
- 754.Gautier S, Champion E, Bernache-Assollant D (1999) J Mater Sci Mater Med 10:533Google Scholar
- 755.Fang Y, Roy DM, Cheng J, Roy R, Agrawal DK (1993) Ceram Trans 36:397Google Scholar
- 756.Park K, Vasilosa T (1997) Mater Lett 32:229Google Scholar
- 758.Ruys AJ, Simpson SA, Sorrell CC (1994) J Mater Sci Lett 13:1323Google Scholar
- 760.Li J, Liao H, Hermansson L (1996) Biomaterials 17:1787Google Scholar
- 761.Takagi M, Mochida M, Uchida N, Saito K, Uematsu K (1992) J Mater Sci Mater Med 3:199Google Scholar
- 762.Silva VV, Domingues RZ (1997) J Mater Sci Mater Med 8:907Google Scholar
- 763.Silva VV, Lameiras FS, Domingues RZ (2001) Ceram Int 27:615Google Scholar
- 764.Rapacz-Kmita A, Slosarczyk A, Paszkiewicz Z, Paluch D (2004) J Mater Sci 39:5865. doi: https://doi.org/10.1023/B:JMSC.0000040104.64482.4a Google Scholar
- 765.Rapacz-Kmita A, Slosarczyk A, Paszkiewicz Z (2005) Ceram Int 31:567Google Scholar
- 766.Sung YM, Kim DH (2003) J Crystal Growth 254:411Google Scholar
- 767.Silva VV, Lameiras FS (2000) Mater Charact 45:51Google Scholar
- 768.Shen Z, Adolfsson E, Nygren M, Gao L, Kawaoka H, Niihara K (2001) Adv Mater 13:214Google Scholar
- 769.Adolfsson E, Alberiushenning P, Hermansson L (2000) J Am Ceram Soc 83:2798Google Scholar
- 770.Kim HW, Noh YJ, Koh YH, Kim HE, Kim HM (2002) Biomaterials 23:4113Google Scholar
- 771.Li W, Gao L (2003) Biomaterials 24:937Google Scholar
- 772.Kim HW, Knowles JC, Li LH, Kim HE (2005) J Biomed Mater Res A 72A:258Google Scholar
- 774.Kumar BR, Prakash KH, Cheang P, Khor KA (2005) Acta Mater 53:2327Google Scholar
- 775.Ahn ES, Gleason NJ, Nakahira A, Ying JY (2001) Nano Lett 1:149Google Scholar
- 776.Silva VV, Lameiras FS, Domingues RZ (2001) Compos Sci Technol 61:301Google Scholar
- 777.Khor KA, Fu L, Lim JP, Cheang P (2001) Mater Sci Eng A 316:160Google Scholar
- 778.Fu L, Khor KA, Lim JP (2002) J Am Ceram Soc 85:800Google Scholar
- 779.Chou BY, Chang E, Yao SY, Chen JM (2002) J Am Ceram Soc 85:661Google Scholar
- 780.Wang Q, Ge S, Zhang D (2005) Wear 259:952Google Scholar
- 781.Murugan R, Ramakrishna S (2003) Mater Lett 58:230Google Scholar
- 782.Fu L, Khor KA, Lim JP (2000) Mater Sci Eng A 276:46Google Scholar
- 783.Nagarajan VS, Rao KJ (1993) J Mater Chem 3:43Google Scholar
- 784.Tamari N, Kondo I, Mouri M, Kinoshita M (1988) J Ceram Soc Japan 96:1200Google Scholar
- 787.Ahn ES, Gleason NJ, Ying JY (2005) J Am Ceram Soc 88:3374Google Scholar
- 788.Erkmen ZE, Genç Y, Oktar FN (2007) J Am Ceram Soc 90:2885Google Scholar
- 789.Rapacz-Kmita A, Slosarczyk A, Paszkiewicz Z (2006) J Eur Ceram Soc 26:1481Google Scholar
- 790.Sung YM, Shin YK, Ryu JJ (2007) Nanotechnology 18:065602 (6 pp)Google Scholar
- 791.Quan R, Yang D, Wu X, Wang H, Miao X, Li W (2008) J Mater Sci Mater Med 19:183Google Scholar
- 792.Khalil KA, Kim SW, Kim HY (2007) Mater Sci Eng A 456:368Google Scholar
- 793.Kong YM, Kim S, Kim HE, Lee IS (1999) J Am Ceram Soc 82:2963Google Scholar
- 794.Choi JW, Kong YM, Kim HE, Lee IS (1998) J Am Ceram Soc 81:1743Google Scholar
- 796.Li J, Fartash B, Hermansson L (1995) Biomaterials 16:417Google Scholar
- 797.Kim S, Kong YM, Kim HE, Lee IS (2002) J Mater Sci Mater Med 13:307Google Scholar
- 798.Chiba A, Kimura S, Raghukandan K, Morizono Y (2003) Mater Sci Eng A 350:179Google Scholar
- 799.Pang YX, Bao X, Weng L (2004) J Mater Sci 39:6311. doi: https://doi.org/10.1023/B:JMSC.0000043601.46284.a0 Google Scholar
- 800.Jun YK, Kim WH, Kweon OK, Hong SH (2003) Biomaterials 24:3731Google Scholar
- 801.Epure LM, Dimitrievska S, Merhi Y, Yahia LH (2007) J Biomed Mater Res A 83A:1009Google Scholar
- 802.Evis Z, Doremus RH (2007) Mater Sci Eng C 27:421Google Scholar
- 803.Lu YP, Li MS, Li ST, Wang ZG, Zhu RF (2004) Biomaterials 25:4393Google Scholar
- 804.Li H, Khor KA, Cheang P (2003) Biomaterials 24:949Google Scholar
- 805.Zheng XB, Ding CX (2000) J Therm Spray Technol 9:520Google Scholar
- 806.Lee SH, Kim HW, Lee EJ, Li LH, Kim HE (2006) J Biomater Appl 20:195Google Scholar
- 807.Lin C, Yen S (2004) J Mater Sci Mater Med 15:1237Google Scholar
- 808.Balamurugan A, Balossier G, Kannan S, Michel J, Rajeswari S (2007) Mater Sci Eng C 27:162Google Scholar
- 809.Gaona M, Limab RS, Marple BR (2007) Mater Sci Eng A 458:141Google Scholar
- 810.Boyd AR, Duffy H, McCann R, Meenan BJ (2008) Mater Sci Eng C 28:228Google Scholar
- 811.Fidancevska E, Ruseska G, Bossert J, Linc YM, Boccaccini AR (2007) Mater Chem Phys 103:95Google Scholar
- 812.Harle J, Kim HW, Mordan N, Knowles JC, Salih V (2006) Acta Biomater 2:547Google Scholar
- 813.Kim HW, Kim HE, Salih V, Knowles JC (2005) J Biomed Mater Res B Appl Biomater 72B:1Google Scholar
- 814.Pushpakanth S, Srinivasan B, Sreedhar B, Sastry TP (2008) Mater Chem Phys 107:492Google Scholar
- 815.Sato M, Aslani A, Sambito MA, Kalkhoran NM, Slamovich EB, Webster TJ (2008) J Biomed Mater Res 84A:265Google Scholar
- 816.Ramires PA, Romito A, Cosentino F, Milella E (2001) Biomaterials 22:1467Google Scholar
- 817.Sun R, Li M, Lu Y, An X (2006) Mater Sci Eng C 26:28Google Scholar
- 818.Lee BT, Lee CW, Gain AK, Song HY (2007) J Eur Ceram Soc 27:157Google Scholar
- 819.Kong YM, Bae CJ, Lee SH, Kim HW, Kim HE (2005) Biomaterials 26:509Google Scholar
- 820.Oktar FN, Agathopoulos S, Ozyegin LS, Gunduz O, Demirkol N, Bozkurt Y, Salman S (2007) J Mater Sci Mater Med 18:2137Google Scholar
- 822.Li XW, Yasuda HY, Umakoshi Y (2006) J Mater Sci Mater Med 17:573Google Scholar
- 823.Ragel CV, Vallet-Regi M, Rodríguez-Lorenzo LM (2002) Biomaterials 23:1865Google Scholar
- 824.Padilla S, Sánchez-Salcedo S, Vallet-Regi M (2005) J Biomed Mater Res A 75A:63Google Scholar
- 825.Lopes MA, Monterio FJ, Santos JD (1999) Biomaterials 20:2085Google Scholar
- 826.Fu Q, Zhou N, Huang W, Wang D, Zhang L, Li H (2004) J Mater Sci Mater Med 15:1333Google Scholar
- 827.Fu Q, Zhou N, Huang W, Wang D, Zhang L, Li H (2005) J Biomed Mater Res A 74A:156Google Scholar
- 828.Oktar FN, Goller G (2002) Ceram Int 28:617Google Scholar
- 829.Padilla S, Román J, Sánchez-Salcedo S, Vallet-Regi M (2006) Acta Biomater 2:331Google Scholar
- 830.Kokubo T, Shigematsu M, Nagashima Y, Tashiro M, Nakamura T, Yamamuro T, Higashi S (1982) Bull Inst Chem Res Kyoto Univ 60:260Google Scholar
- 831.Kitsugi T, Yamamuro T, Nakamura T, Higashi S, Kakutani Y, Hyakuna K, Ito S, Kokubo T, Takagi M, Shibuya T (1986) J Biomed Mater Res 20:1295Google Scholar
- 834.Kokubo T (1991) Biomaterials 12:155Google Scholar
- 835.Kokubo T, Ito S, Huang ZT, Hayashi T, Sakka S, Kitsugi T, Yamamuro T (1990) J Biomed Mater Res 24:331Google Scholar
- 836.Nishio K, Neo M, Akiyama H, Okada Y, Kokubo T, Nakamura T (2001) J Biomed Mater Res 55:164Google Scholar
- 837.Zhang D, Chang J, Zeng Y (2008) J Mater Sci Mater Med 19:443Google Scholar
- 838.Chaki TK, Wang PE (1994) J Mater Sci Mater Med 5:533Google Scholar
- 840.Chu C, Lin P, Dong Y, Xue X, Zhu J, Yin Z (2002) J Mater Sci Mater Med 13:985Google Scholar
- 841.Shi W, Kamiya A, Zhu J, Watazu A (2002) Mater Sci Eng A 337:104Google Scholar
- 842.Ning CQ, Zhou Y (2002) Biomaterials 23:2909Google Scholar
- 843.Karanjai M, Sundaresan R, Rao GVN, Rama Mohan TR, Kashyap BP (2007) Mater Sci Eng A 447:19Google Scholar
- 844.Karanjai M, Manoj Kumar BV, Sundaresan R, Basu B, Rama Mohan TR, Kashyap BP (2008) Mater Sci Eng A 475:299Google Scholar
- 845.Ning CQ, Zhou Y (2004) Biomaterials 25:3379Google Scholar
- 846.Chu C, Xue X, Zhu J, Yin Z (2004) J Mater Sci Mater Med 15:665Google Scholar
- 847.Smirnov VV, Egorov AA, Barinov SM, Shvorneva LI (2007) Dokl Chem 413:82Google Scholar
- 848.Chu C, Xue X, Zhu J, Yin Z (2006) J Mater Sci Mater Med 17:245Google Scholar
- 849.Li J, Habibovic P, Yuan H, van den Doel M, Wilson CE, de Wijn JR, van Blitterswijk CA, de Groot K (2007) Biomaterials 28:4209Google Scholar
- 850.Pattanayak DK, Mathur V, Rao BT, Rama Mohan TR (2003) Trends Biomater Artif Organs 17:8Google Scholar
- 851.Ding Y, Liu J, Wang H, Shen G, Yu R (2007) Biomaterials 28:2147Google Scholar
- 852.Damien CJ, Parsons JR, Benedict JJ, Weisman DS (1990) J Biomed Mater Res 24:639Google Scholar
- 853.Rauschmann MA, Wichelhaus TA, Stirnal V, Dingeldein E, Zichner L, Schnettler R, Alt V (2005) Biomaterials 26:2677Google Scholar
- 854.Urban RM, Turner TM, Hall DJ, Inoue N, Gitelis S (2007) Clin Orthop Relat Res 459:110Google Scholar
- 855.Gittings JP, Bowena CR, Turner IG, Baxter F, Chaudhuri J (2007) J Eur Ceram Soc 27:4187Google Scholar
- 856.Watanabe Y, Ikoma T, Suetsugu Y, Yamada H, Tamura K, Komatsu Y, Tanaka J, Moriyoshi Y (2006) J Eur Ceram Soc 26:481Google Scholar
- 857.Agathopoulos S, Tulyaganov DU, Marques PAAP, Ferro MC, Fernandes MHV, Correia RN (2003) Biomaterials 24:1317Google Scholar
- 858.Khor KA, Gu YW, Pan D, Cheang P (2004) Biomaterials 25:4009Google Scholar
- 859.Gu YW, Khor KA, Pan D, Cheang P (2004) Biomaterials 25:3177Google Scholar
- 860.Best SM, Porter AE, Thian ES, Huang J (2008) J Eur Ceram Soc 28:1319Google Scholar
- 861.de Aza PN, Guitián F, de Aza S (1997) Biomaterials 18:1285Google Scholar
- 862.Huang X, Jiang D, Tan S (2004) J Biomed Mater Res B Appl Biomater 69B:70Google Scholar
- 863.Zhang F, Chang J, Lin K, Lu J (2008) J Mater Sci Mater Med 19:167Google Scholar
- 864.Juhasz JA, Best SM, Kawashita M, Miyata N, Kokubo T, Nakamura T, Bonfield W (2003) J Biomed Mater Res A 67A:952Google Scholar
- 865.Juhasz JA, Best SM, Bonfield W, Kawashita M, Miyata N, Kokubo T, Nakamura T (2003) J Mater Sci Mater Med 14:489Google Scholar
- 866.Juhasz JA, Best SM, Brooks R, Kawashita M, Miyata N, Kokubo T, Nakamura T, Bonfield W (2004) Biomaterials 25:949Google Scholar
- 867.Rea SM, Brooks RA, Best SM, Kokubo T, Bonfield W (2004) Biomaterials 25:4503Google Scholar
- 868.Greish YE, Brown PW (2001) J Biomed Mater Res 55:618. Erratum in: J Biomed Mater Res 2001;56:459Google Scholar
- 869.Greish YE, Brown PW (2000) J Biomed Mater Res 52:687Google Scholar
- 870.Kangasniemi I, de Groot K, Wolke J, Andersson O, Luklinska Z, Becht JGM, Lakkisto M, Yli-Urpo A (1991) J Mater Sci Mater Med 2:133Google Scholar
- 871.Kangasniemi IMO, de Groot K, Becht JGM, Yli-Urpo A (1992) J Biomed Mater Res 26:663Google Scholar
- 872.Kangasniemi IMO, Vedel E, de Blick-Hogerworst J, Yli-Urpo A, de Groot K (1993) J Biomed Mater Res 27:1225Google Scholar
- 873.Maruno S, Ban S, Wang YF, Iwata H, Itoh H (1992) J Ceram Soc Jpn 100:362Google Scholar
- 874.White AA, Best SM, Kinloch IA (2007) Int J Appl Ceram Technol 4:1Google Scholar
- 875.Chlopek J, Czajkowska B, Szaraniec B, Frackowiak E, Szostak K, Beguin F (2006) Carbon 44:1106Google Scholar
- 876.Price RL, Waid MC, Haberstroh KM, Webster TJ (2003) Biomaterials 24:1877Google Scholar
- 877.Zanello LP, Zhao B, Hu H, Haddon RC (2006) Nano Lett 6:562Google Scholar
- 878.Saito N, Usui Y, Aoki K, Narita N, Shimizu M, Ogiwara N, Nakamura K, Ishigaki N, Kato H, Taruta S (2008) Curr Med Chem 15:523Google Scholar
- 879.Kobayashi S, Kawai W (2007) Composites A 38:114Google Scholar
- 880.Balani K, Anderson R, Laha T, Andara M, Tercero J, Crumpler E, Agarwal A (2007) Biomaterials 28:618Google Scholar
- 881.Chen Y, Gan CH, Zhang TH, Yu G, Bai P, Kaplan A (2005) Appl Phys Lett 86:251905 (3 pp)Google Scholar
- 882.Chen Y, Zhang TH, Gan CH, Yu G (2007) Carbon 45:998Google Scholar
- 883.Chen Y, Zhang YQ, Zhang TH, Gan CH, Zheng CY, Yu G (2006) Carbon 44:37Google Scholar
- 884.Ding Y, Liu J, Jin X, Lu H, Shen G, Yu R (2008) Analyst 133:184Google Scholar
- 885.Slosarcyk A, Klisch M, Blazewicz M, Piekarczyk J, Stobierski L, Rapacz-Kmita A (2000) J Eur Ceram Soc 20:1397Google Scholar
- 886.Dorner-Reisel A, Berroth K, Neubauer R, Nestler K, Marx G, Scislo M, Müller E, Slosarcyk A (2004) J Eur Ceram Soc 24:2131Google Scholar
- 887.Fu T, Zhao JL, Wei JH, Han Y, Xu KW (2004) J Mater Sci 39:1411. doi: https://doi.org/10.1023/B:JMSC.0000013906.60034.e8 Google Scholar
- 888.Yoshimura M (1988) Am Ceram Soc Bull 67:1950Google Scholar
- 889.Thompson I, Rawlings RD (1990) Biomaterials 11:505Google Scholar
- 890.Monma H (1987) J Ceram Soc Jpn 96:60Google Scholar
- 891.Suchanek W, Yashima M, Kakihana M, Yoshimura M (1996) Biomaterials 17:1715Google Scholar
- 892.Suchanek W, Yashima M, Kakihana M, Yoshimura M (1997) J Am Ceram Soc 80:2805Google Scholar
- 893.Kaito T, Mukai Y, Nishikawa M, Ando W, Yoshikawa H, Myoui A (2006) J Biomed Mater Res B Appl Biomater 78B:378Google Scholar
- 894.Ramay HR, Zhang M (2004) Biomaterials 21:5171Google Scholar
- 895.Watari F, Yokoyama A, Saso F, Uo M, Kawasaki T (1997) Composites B 28B:5Google Scholar
- 896.Watari F, Yokoyama A, Omori M, Hirai T, Kondo H, Uo M, Kawasaki T (2004) Compos Sci Technol 64:893Google Scholar
- 897.Chenglim C, Jingchuan Z, Zhongda Y, Shidong W (1999) Mater Sci Eng A 271:95Google Scholar
- 898.Inagaki M, Yokogawa Y, Kameyama T (2006) J Eur Ceram Soc 26:495Google Scholar
- 899.Ban S, Hasegawa J, Maruno S (1999) Mater Sci Forum 308–311:350Google Scholar
- 900.Stojanovic D, Jokic B, Veljovic DJ, Petrovic R, Uskokovic PS, Janackovic Dj (2007) J Eur Ceram Soc 27:1595Google Scholar
- 901.Nonami T, Kamiya A, Naganuma K, Kameyana T (1998) Mater Sci Eng C 6:281Google Scholar
- 902.Wong LH, Tio B, Miao X (2002) Mater Sci Eng C 20:111Google Scholar
- 903.Peltola T, Patsi M, Rahiala H, Kangasniemi I, Yli-Urpo A (1998) J Biomed Mater Res 41:504Google Scholar
- 904.Heilmann F, Standard OC, Müller FA, Hoffman M (2007) J Mater Sci Mater Med 18:1817Google Scholar
- 905.Cavalcanti A, Shirinzadeh B, Zhang M, Kretly LC (2008) Sensors 8:2932Google Scholar
- 906.Wypych G (1999) Handbook of fillers, 2nd edn. ChemTec Publishing, New YorkGoogle Scholar
- 907.Rhee SH, Lee JD, Tanaka J (2000) J Am Ceram Soc 83:2890Google Scholar
- 908.Lin X, Li X, Fan H, Wen X, Lu J, Zhang X (2004) Mater Lett 58:3569Google Scholar
- 909.Zhang W, Liao SS, Cui FZ (2003) Chem Mater 15:3221Google Scholar
- 910.Liu Q, de Wijn JR, van Blitterswijk CA (1998) J Biomed Mater Res 40:257Google Scholar
- 911.Li J, Chen YP, Yin Y, Yao F, Yao K (2007) Biomaterials 28:781Google Scholar
- 912.Boanini E, Gazzano M, Rubini K, Bigi A (2007) Adv Mater 19:2499Google Scholar
- 913.Tjandra W, Yao J, Ravi P, Tam KC, Alamsjah A (2005) Chem Mater 17:4865Google Scholar
- 914.Misra DN (1985) J Dent Res 12:1405Google Scholar
- 915.Liu Q, de Wijn JR, van Blitterswijk CA (1998) J Biomed Mater Res 40:358Google Scholar
- 916.Grossman RF (1996) In: Edenbaum J (ed) Plastics additives and modifiers handbook, 2nd edn. Chapman & Hall, New YorkGoogle Scholar
- 917.Chang MC, Ikoma T, Kikuchi M, Tanaka J (2001) J Mater Sci Lett 20:1199Google Scholar
- 918.Sousa RA, Reis RL, Cunha AM, Bevis MJ (2003) J Mater Sci Mater Med 14:475Google Scholar
- 919.Wang M, Deb S, Bonfield W (2000) Mater Lett 44:119Google Scholar
- 920.Wang M, Bonfield W (2001) Biomaterials 22:1311Google Scholar
- 921.Dupraz AMP, de Wijn JR, van der Meer SAT, Goedemoed JH (1996) J Mater Sci Mater Med 7:731Google Scholar
- 922.Dupraz AMP, de Wijn JR, van der Meer SAT, de Groot K (1996) J Biomed Mater Res 30:231Google Scholar
- 923.Liao JG, Wang XJ, Zuo Y, Zhang L, Wen JQ, Li Y (2008) J Inorg Mater 23:145Google Scholar
- 924.Sousa RA, Reis RL, Cunha AM, Bevis MJ (2002) J Appl Polym Sci 86:2866Google Scholar
- 925.Morita S, Furuya K, Ishihara K, Nakabayashi N (1998) Biomaterials 19:1601Google Scholar
- 926.Shinzato S, Nakamura T, Tamura J, Kokubo T, Kitamura Y (2001) J Biomed Mater Res 56:571Google Scholar
- 927.Dorozhkin SV (2001) Biomed Mater Res 54:247Google Scholar
- 928.Omori M, Okubo A, Otsubo M, Hashida T, Tohji K (2004) Key Eng Mater 254–256:395Google Scholar
- 929.Zhao B, Hu H, Mandal SK, Haddon RC (2005) Chem Mater 17:3235Google Scholar
- 930.Kasuga T, Yoshida M, Ikushima AJ, Tuchiya M, Kusakari H (1992) J Am Ceram Soc 75:1884Google Scholar
- 931.Dorozhkin SV (1999) Comments Inorg Chem 20:285Google Scholar
- 932.Dorozhkin SV (2002) Prog Cryst Growth Charact 44:45Google Scholar
- 933.Furukawa T, Matsusue Y, Yasunaga T, Shikinami Y, Okuno M, Nakamura T (2000) Biomaterials 21:889Google Scholar
- 934.Furukawa T, Matsusue Y, Yasunaga T, Nakagawa Y, Okada Y, Shikinami Y, Okuno M, Nakamura T (2000) J Biomed Mater Res 50:410Google Scholar
- 935.Yasunaga T, Matsusue Y, Furukawa T, Shikinami Y, Okuno M, Nakamura T (1999) J Biomed Mater Res 47:412Google Scholar
- 936.Marques AP, Reis RL, Hunt JA (2002) Biomaterials 6:1471Google Scholar
- 937.Mendes SC, Bovell YP, Reis RL, Cunha AM, de Bruijn JD, van Blitterswijk CA (2001) Biomaterials 22:2057Google Scholar
- 938.Meyers MA, Lin AYM, Seki Y, Chen PY, Kad BK, Bodde S (2006) JOM 58:36Google Scholar